 ############################################################################
 ##                                                                        ##
 #                   CIF for Sr/Cr- and Ba-doped KTP.                       #
 #    Modified and edited by Stefan Norberg, Inorganic Chemistry CHALMERS   #
 ##                                                                        ##
 ############################################################################
 
data_global
 
_audit_creation_method                'Xtal3.6 + some modification'
_audit_creation_date                   99-12-03
_audit_update_record                  '00-03-30 Stefan Norberg'

#==============================================================================
#   (Publishing Staff Use Only)

_journal_date_recd_electronic          ?
_journal_date_to_coeditor              ?
_journal_date_from_coeditor            ?
_journal_date_accepted                 ?
_journal_date_printers_first           ?
_journal_date_printers_final           ?
_journal_date_proofs_out               ?
_journal_date_proofs_in                ?
_journal_coeditor_name                 ?
_journal_coeditor_code                 OS0060
_journal_coeditor_notes
;  ?
;
_journal_techeditor_code               ?
_iucr_compatibility_tag       ACTA95
_journal_techeditor_notes
;  ?
;
_journal_coden_ASTM                    ?
_journal_name_full                     ?
_journal_year                          ?
_journal_volume                        ?
_journal_issue                         ?
_journal_page_first                    ?
_journal_page_last                     ?
_journal_suppl_publ_number             ?
_journal_suppl_publ_pages              ?
#==============================================================================


#------------------------------------------------------------------------------
# SUBMISSION DETAILS
#------------------------------------------------------------------------------
 
_publ_contact_author_name             'STEFAN T. NORBERG'
_publ_contact_author_address
;
Department of Inorganic Chemistry
Chalmers University of Technology
SE-412 96 Göteborg
Sweden
;

_publ_contact_author_email            'stn@inoc.chalmers.se'
_publ_contact_author_fax              '+46 (0)31 7722846'
_publ_contact_author_phone            '+46 (0)31 7722881'
 
_publ_contact_letter
 'OS60'
 
_publ_requested_journal               'Acta Crystallographica Section B'
_publ_requested_category              'Research Paper'

_publ_section_title
;
Dopant positions in strontium/chromium and barium doped KTP, determined with
synchrotron X-radiation
;

_publ_section_title_footnote           ?
 
loop_
_publ_author_name
_publ_author_footnote
_publ_author_address
 'STEFAN T. NORBERG'
  ?
;
Department of Inorganic Chemistry
Chalmers University of Technology
S-412 96 Göteborg
Sweden
;
 'VICTOR A. STRELTSOV'
  ? 
;
Crystallography Centre
University of Western Australia
Nedlands 6907
Australia
;
 'GÖRAN SVENSSON'
  ?
;
Department of Inorganic Chemistry
Chalmers University of Technology
S-412 96 Göteborg
Sweden
;
 'JÖRGEN ALBERTSSON'
  ?
;
Department of Inorganic Chemistry
Chalmers University of Technology
S-412 96 Göteborg
Sweden
;


#------------------------------------------------------------------------------
# TEXT and TABLES
#------------------------------------------------------------------------------
 
_publ_section_synopsis
;  ?
;
_publ_section_abstract
;  ?
;
_publ_section_comment
;  ?
;
_publ_section_exptl_prep
;  ?
;
_publ_section_exptl_refinement
;  ?
;
_publ_section_acknowledgements
;  ?
;
_publ_section_references
;  ?
;
_publ_section_figure_captions
;  ?
;


#==============================================================================
#  One data block for each single structure in the paper
#==============================================================================
 
data_SrCrKTP

 
#------------------------------------------------------------------------------
# A1. CRYSTAL DATA for the SrCrKTP structure
#------------------------------------------------------------------------------

_chemical_formula_sum                 'Cr0.05 K0.87 O5 P Sr0.06 Ti0.95'
_chemical_formula_moiety              'Sr0.06 K0.87 Cr0.05 Ti0.95 O P O4'
_chemical_formula_weight               198.13
_chemical_melting_point               'not measured'
 
_symmetry_cell_setting                 orthorhombic
_symmetry_space_group_name_H-M        'P n a 21'
_symmetry_space_group_name_Hall       'p 2c -2n'
 
loop_
_symmetry_equiv_pos_as_xyz
  +x,+y,+z  -x,-y,1/2+z  1/2-x,1/2+y,1/2+z  1/2+x,1/2-y,+z

_cell_special_details
;
Reflections used for the determination of the unit cell:
  (0 12 0), (0 -12 0), (20 0 0), (-20 0 0),
  (8 0 16), (8 0 -16), (-8 0 16), (-8 0 -16),
  (0 4 16), (0 4 -16), (0 -4 16), (0 -4 -16).
;
 
_cell_length_a                         12.786(2)
_cell_length_b                         6.3927(8)
_cell_length_c                         10.5585(9)
_cell_angle_alpha                      90
_cell_angle_beta                       90
_cell_angle_gamma                      90
_cell_volume                           863.03(19)
_cell_formula_units_Z                  8
_cell_measurement_reflns_used          12
_cell_measurement_theta_min            35.9
_cell_measurement_theta_max            44.8
_cell_measurement_temperature          293(1)
_cell_measurement_radiation            ?
_cell_measurement_wavelength           ?
  
_exptl_crystal_density_diffrn          3.050
_exptl_crystal_density_meas           'not measured'
_exptl_crystal_density_method          ?

_exptl_crystal_description             Rectangular

_exptl_crystal_size_max                0.058
_exptl_crystal_size_mid                0.054
_exptl_crystal_size_min                0.040
_exptl_crystal_size_rad                ?
_exptl_crystal_colour                 'light brown'

_exptl_crystal_F_000                   766.57
_exptl_absorpt_coefficient_mu          4.107 
_exptl_absorpt_correction_type         analytical
_exptl_absorpt_process_details
;
Alcock, N. W. 1974. Absorption and Extinction Corrections: Calculation
Methods and Standard Tests. Acta Cryst. A30, 332-335
;
_exptl_absorpt_correction_T_min        .8054
_exptl_absorpt_correction_T_max        .8577


#------------------------------------------------------------------------------
# A2. EXPERIMENTAL DATA for the SrCrKTP structure
#------------------------------------------------------------------------------

_exptl_special_details
;  ?
;

_diffrn_special_details
;  ?
;

_diffrn_radiation_type                'synchrotron x-ray vertical wiggler'
_diffrn_radiation_wavelength           .75000(9)
_diffrn_radiation_source              'photon factory bl14a'
_diffrn_ambient_temperature            293(1)
_diffrn_ambient_environment            ?
 
_diffrn_measurement_device_type       'bl14a 4-circle'
_diffrn_measurement_method             ω-2θ   
_diffrn_radiation_monochromator        si(111)  
_diffrn_radiation_detector            'avalanche photo diode'

_diffrn_detector_area_resol_mean       ?
_diffrn_measured_fraction_theta_max    ?
_diffrn_measured_fraction_theta_full   ?

_diffrn_reflns_number                  40331

_diffrn_reflns_theta_min               3.36
_diffrn_reflns_theta_max               64.91
_diffrn_reflns_theta_full              ?
_diffrn_reflns_av_R_equivalents        .060
_diffrn_reflns_av_unetI/netI           .022
_diffrn_reflns_limit_h_min             -28
_diffrn_reflns_limit_h_max             28
_diffrn_reflns_limit_k_min             -14
_diffrn_reflns_limit_k_max             14
_diffrn_reflns_limit_l_min             -25
_diffrn_reflns_limit_l_max             23
_diffrn_reflns_reduction_process      'equatorial monochr Lp'

_diffrn_standards_number               6
_diffrn_standards_interval_count       200
_diffrn_standards_interval_time        ?
_diffrn_standards_decay_%              23

loop_
_diffrn_standard_refln_index_h
_diffrn_standard_refln_index_k
_diffrn_standard_refln_index_l
   12   0   0
  -12   0   0
    4  10   0
   -4 -10   0
    0   0  16
    0   0 -16


#------------------------------------------------------------------------------
# A3. REFINEMENT DATA for the SrCrKTP structure
#------------------------------------------------------------------------------

_refine_special_details
;
Two constraints used during the refinement of the population:
    constr pop(Cr1)=1.0-1.0*pop(Ti1)
    constr pop(Cr2)=1.0-1.0*pop(Ti2)

No restraints used.
;

_reflns_number_total                   10124
_reflns_number_gt                      10124
_reflns_Friedel_coverage               1.012
_reflns_threshold_expression           F>2σ(F)
 
_reflns_limit_h_min                    0
_reflns_limit_h_max                    28
_reflns_limit_k_min                    0
_reflns_limit_k_max                    14
_reflns_limit_l_min                   -25
_reflns_limit_l_max                    23
_reflns_d_resolution_high              .414
_reflns_d_resolution_low               6.385
 
_refine_ls_structure_factor_coef       F
_refine_ls_matrix_type                 full
_refine_ls_R_factor_all                .028
_refine_ls_R_factor_gt                 .028
_refine_ls_wR_factor_all               .032
_refine_ls_wR_factor_ref               .032
_refine_ls_goodness_of_fit_all         2.493
_refine_ls_goodness_of_fit_ref         2.493
_refine_ls_number_reflns               10124
_refine_ls_number_parameters           194
_refine_ls_weighting_scheme            calc
_refine_ls_weighting_details           w=1/σ²(F)
_refine_ls_number_restraints           0
_refine_ls_number_constraints          2
_refine_ls_hydrogen_treatment          none
_refine_ls_shift/su_max                .019
_refine_ls_shift/su_mean               .001
_refine_diff_density_min               -1.454
_refine_diff_density_max               1.199
 
_refine_ls_extinction_method          'Gaussian (Zachariasen, 1967)'
_refine_ls_extinction_expression      'Eq22 p292 "Cryst. Comp." Munksgaard 1970'
_refine_ls_extinction_coef             .000
_refine_ls_abs_structure_details      'Flack xabs refined'
_refine_ls_abs_structure_Flack         0.465(10)
 

#------------------------------------------------------------------------------
# A4. COMPUTING METHODS for the SrCrKTP structure
#------------------------------------------------------------------------------
 
_computing_data_collection            'BL14A (Tsukuba, Japan)'
_computing_cell_refinement            'BL14A (Tsukuba, Japan)'
_computing_data_reduction
 'Xtal3.6 (Hall et al., 1999) DIFDAT ADDREF ABSORB SORTRF'
_computing_structure_refinement       'Xtal3.6 (Hall et al., 1999) CRYLSQ'
_computing_molecular_graphics
;
ORTEPIII (Burnett & Johnson, 1996) and Xtal3.6 (Hall et al., 1999) FOURR SLANT
CONTRS
;
_computing_publication_material
 'Xtal3.6 (Hall et al., 1999) BONDLA ATABLE CIFIO'


#------------------------------------------------------------------------------
# A5. SCATERING FACTORS AND ATOM DATA for the SrCrKTP structure
#------------------------------------------------------------------------------
 
loop_
_atom_type_symbol
_atom_type_description
_atom_type_oxidation_number
_atom_type_number_in_cell
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
  K   ?  0 '6.956'   .1958   .2781 'Int Tables Vol IV Tables 2.2B and 2.3.1'
  Sr  ?  0 '0.464' -2.8958  3.5793 'Int Tables Vol IV Tables 2.2B and 2.3.1'
  Ti  ?  0 '7.612'   .2647   .4951 'Int Tables Vol IV Tables 2.2B and 2.3.1'
  Cr  ?  0 '0.388'   .2983   .6914 'Int Tables Vol IV Tables 2.2B and 2.3.1'
  P   ?  0  8        .1003   .1055 'Int Tables Vol IV Tables 2.2B and 2.3.1'
  O   ?  0 40        .0093   .0689 'Int Tables Vol IV Tables 2.2B and 2.3.1'

# S.Sasaki (1989) Numerical Tables of Anomalous Scattering Factors
# Calculated by the Cromer and Liberman's Method, KEK Report, 88-14, 1-136.
# Are used for anomalous dispersion correction.
 
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_calc_attached_atom
_atom_site_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
  K1    .37755(5)   .22053(9)  .30331(8)  .01901(18) Uani  ?  ?   .857(2)  ?  ?
  Sr1a  .3898(6)    .2116(9)   .3398(8)   .019(2)    Uani  ?  ?   .040(1)  ?  ?
  Sr1b  .3945(9)    .2022(17)  .4372(12)  .026(4)    Uani  ?  ?   .023(1)  ?  ?
  K2    .10548(4)   .30046(11) .05796(8)  .0204(2)   Uani  ?  ?   .882(2)  ?  ?
  Sr2a  .1047(6)    .3032(11)  .0968(8)   .016(2)    Uani  ?  ?   .033(1)  ?  ?
  Sr2b  .1219(10)   .2783(13)  .1953(11)  .025(4)    Uani  ?  ?   .020(1)  ?  ?
  Ti1   .372899(17) .49998(3) -.00666(6)  .00705(6)  Uani  ?  ?   .955(1)  ?  ?
  Cr1   .3874(5)    .5069(7)   .0214(6)   .0096(7)   Uiso  ?  ?   .045(1)  ?  ?
  Ti2   .246829(14) .73301(4)  .24415(7)  .00664(6)  Uani  ?  ?   .948(1)  ?  ?
  Cr2   .2450(3)    .7862(6)   .2666(5)   .0096(13)  Uani  ?  ?   .052(1)  ?  ?
  P1    .498123(18) .66508(4)  .25210(9)  .00661(7)  Uani  ?  ?  1.000     ?  ?
  P2    .18034(2)   .49796(4)  .50376(6)  .00665(9)  Uani  ?  ?  1.000     ?  ?
  O1    .48594(9)   .51487(18) .14126(12) .0111(3)   Uani  ?  ?  1.000     ?  ?
  O2    .50963(8)   .5347(2)   .37442(11) .0110(3)   Uani  ?  ?  1.000     ?  ?
  O3    .40048(6)   .80241(15) .27093(10) .0098(3)   Uani  ?  ?  1.000     ?  ?
  O4    .59383(6)   .80702(15) .23196(10) .0101(3)   Uani  ?  ?  1.000     ?  ?
  O11   .27536(8)   .53370(16) .13381(11) .0105(3)   Uani  ?  ?  1.000     ?  ?
  O12   .22366(8)   .9591(2)   .38055(12) .0113(3)   Uani  ?  ?  1.000     ?  ?
  O5    .11202(9)   .68890(17) .53274(11) .0097(3)   Uani  ?  ?  1.000     ?  ?
  O6    .11110(9)   .30816(16) .47780(11) .0109(3)   Uani  ?  ?  1.000     ?  ?
  O7    .25287(8)   .4608(2)   .61869(12) .0111(3)   Uani  ?  ?  1.000     ?  ?
  O8    .25264(8)   .53903(18) .390(2)    .0111(3)   Uani  ?  ?  1.000     ?  ?

 
 
#------------------------------------------------------------------------------
# A6. MOLECULAR GEOMETRY for the SrCrKTP structure
#------------------------------------------------------------------------------

_geom_special_details
;  ?
;
 
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
  K1    Sr1a   .        .        .420(8)    no
  K1    Sr1b   .        .       1.435(13)   no
  K1    K2     .        .       4.3674(11)  no
  K1    Sr2a   .        .       4.148(8)    no
  K1    Sr2b   .        .       3.481(13)   no
  K1    Ti1    .        .       3.7291(10)  no
  K1    Cr1    .        .       3.497(6)    no
  K1    Ti2    .       '1 545'  3.5913(7)   no
  K1    Cr2    .       '1 545'  3.276(4)    no
  K1    P1     .        .       3.2780(7)   no
  K1    P2     .       '3 544'  3.5463(10)  no
  K1    O1     .        .       2.8963(14)  no
  K1    O2     .        .       2.7294(13)  no
  K1    O3     .       '1 545'  2.7106(12)  no
  K1    O11    .        .       2.9863(13)  no
  K1    O12    .       '1 545'  2.7073(13)  no
  K1    O5     .       '3 544'  2.8671(14)  no
  K1    O7     .       '3 544'  3.0557(14)  no
  K1    O8     .        .       2.746(8)    no
  K1    Ti2    .        .       3.7305(8)   no
  K1    K2     .       '3 545'  3.8063(11)  no
  K1    Sr2a   .       '3 545'  4.095(8)    no
  K1    K2     .        3       4.5848(11)  no
  K1    K2     .        4       3.9016(11)  no
  K1    Sr2a   .        4       3.635(8)    no
  K1    Sr2b   .        4       3.326(13)   no
  Sr1a  Sr1b   .        .       1.031(15)   no
  Sr1a  K2     .        .       4.732(8)    no
  Sr1a  Sr2a   .        .       4.496(11)   no
  Sr1a  Sr2b   .        .       3.774(14)   no
  Sr1a  Ti2    .       '1 545'  3.704(6)    no
  Sr1a  Cr2    .       '1 545'  3.379(8)    no
  Sr1a  P1     .        .       3.344(6)    no
  Sr1a  O1     .        .       3.109(7)    no
  Sr1a  O2     .        .       2.598(6)    no
  Sr1a  O3     .       '1 545'  2.718(6)    no
  Sr1a  O12    .       '1 545'  2.702(7)    no
  Sr1a  O6     .        4       3.185(7)    no
  Sr1a  O8     .        .       2.782(8)    no
  Sr1a  K2     .       '3 545'  3.495(7)    no
  Sr1a  Sr2a   .       '3 545'  3.766(11)   no
  Sr1a  Sr2b   .       '3 545'  4.667(13)   no
  Sr1a  K2     .        3       4.414(7)    no
  Sr1a  Sr2a   .        3       4.655(10)   no
  Sr1a  K2     .        4       4.058(8)    no
  Sr1a  Sr2a   .        4       3.761(11)   no
  Sr1a  Sr2b   .        4       3.338(14)   no
  Sr1b  Sr2b   .        .       4.348(17)   no
  Sr1b  O2     .        .       2.669(11)   no
  Sr1b  O3     .       '1 545'  3.102(11)   no
  Sr1b  O4     .       '2 665'  3.116(13)   no
  Sr1b  O12    .       '1 545'  2.747(11)   no
  Sr1b  O6     .        4       2.803(11)   no
  Sr1b  O8     .        .       2.858(12)   no
  Sr1b  Ti1    .       '2 665'  3.581(11)   no
  Sr1b  Cr1    .       '2 665'  3.467(13)   no
  Sr1b  O1     .       '2 665'  3.202(12)   no
  Sr1b  K2     .       '3 545'  2.868(11)   no
  Sr1b  Sr2a   .       '3 545'  3.057(14)   no
  Sr1b  Sr2b   .       '3 545'  3.849(15)   no
  Sr1b  Ti1    .       '3 545'  3.703(11)   no
  Sr1b  O11    .       '3 545'  3.192(12)   no
  Sr1b  K2     .        3       4.031(11)   no
  Sr1b  Sr2a   .        3       4.195(13)   no
  Sr1b  Sr2b   .        3       4.586(15)   no
  Sr1b  Ti2    .       '3 545'  3.716(12)   no
  Sr1b  P2     .        .       3.401(11)   no
  Sr1b  O7     .        .       3.112(12)   no
  Sr1b  Sr2a   .        4       4.488(15)   no
  Sr1b  Sr2b   .        4       3.872(17)   no
  K2    Sr2a   .        .        .410(9)    no
  K2    Sr2b   .        .       1.472(11)   no
  K2    Ti1    .        .       3.7127(8)   no
  K2    P2     .       '3 544'  3.4011(8)   no
  K2    O11    .        .       2.7537(12)  no
  K2    O7     .       '3 544'  2.8994(14)  no
  K2    Ti2    .        .       3.8441(9)   no
  K2    P1     .       '3 544'  3.5963(12)  no
  K2    O2     .       '3 544'  2.9678(14)  no
  K2    O8     .       '3 544'  3.036(13)   no
  K2    Ti2    .       '3 544'  3.8381(11)  no
  K2    Cr2    .       '3 544'  3.624(5)    no
  K2    O3     .       '3 544'  3.0315(14)  no
  K2    O4     .       '4 465'  3.1134(13)  no
  K2    O12    .       '3 544'  3.0513(14)  no
  K2    Ti1    .       '4 455'  3.6052(7)   no
  K2    Cr1    .       '4 455'  3.432(6)    no
  K2    O1     .       '4 455'  2.6783(13)  no
  K2    O5     .       '2 564'  2.7944(13)  no
  Sr2a  Sr2b   .        .       1.075(14)   no
  Sr2a  Ti1    .        .       3.813(7)    no
  Sr2a  P2     .       '3 544'  3.511(7)    no
  Sr2a  O11    .        .       2.662(7)    no
  Sr2a  O7     .       '3 544'  2.857(7)    no
  Sr2a  Ti2    .        .       3.643(7)    no
  Sr2a  O4     .       '4 465'  2.875(8)    no
  Sr2a  Ti1    .       '4 455'  3.706(7)    no
  Sr2a  Cr1    .       '4 455'  3.504(9)    no
  Sr2a  O1     .       '4 455'  2.581(7)    no
  Sr2a  O5     .       '2 564'  2.852(7)    no
  Sr2b  Cr2    .       '1 545'  3.597(10)   no
  Sr2b  O11    .        .       2.634(11)   no
  Sr2b  O12    .       '1 545'  3.112(10)   no
  Sr2b  O7     .       '3 544'  2.709(10)   no
  Sr2b  O8     .        .       3.132(19)   no
  Sr2b  Ti2    .        .       3.357(10)   no
  Sr2b  Ti1    .       '3 545'  3.616(11)   no
  Sr2b  O4     .       '4 465'  2.703(8)    no
  Sr2b  P1     .       '4 455'  3.301(10)   no
  Sr2b  O1     .       '4 455'  2.619(11)   no
  Sr2b  O2     .       '4 455'  3.105(11)   no
  Sr2b  O6     .        .       2.992(11)   no
  Ti1   Cr1    .        .        .352(7)    no
  Ti1   O1     .        .       2.1301(13)  no
  Ti1   O11    .        .       1.9498(12)  no
  Ti1   O5     .       '3 544'  2.0408(11)  no
  Ti1   O2     .       '2 664'  1.9702(12)  no
  Ti1   O6     .       '3 554'  1.9875(11)  no
  Ti1   O12    .       '3 544'  1.7352(13)  no
  Cr1   O1     .        .       1.786(7)    no
  Cr1   O11    .        .       1.869(7)    no
  Cr1   O5     .       '3 544'  2.036(5)    no
  Cr1   O2     .       '2 664'  2.052(7)    no
  Cr1   O6     .       '3 554'  1.980(5)    no
  Cr1   O12    .       '3 544'  2.079(7)    no
  Ti2   Cr2   '1 545'  '1 545'   .415(4)    no
  Ti2   O3    '1 545'  '1 545'  2.0339(9)   no
  Ti2   O12   '1 545'  '1 545'  2.0618(14)  no
  Ti2   O7    '1 545'  '3 544'  1.9686(14)  no
  Ti2   O11   '1 545'  '1 545'  1.7646(12)  no
  Ti2   O8    '1 545'  '1 545'  1.981(18)   no
  Ti2   O4    '1 545'  '4 455'  1.9771(9)   no
  Cr2   O3    '1 545'  '1 545'  1.992(4)    no
  Cr2   O12   '1 545'  '1 545'  1.656(5)    no
  Cr2   O7    '1 545'  '3 544'  1.919(5)    no
  Cr2   O8    '1 545'  '1 545'  2.053(15)   no
  Cr2   O4    '1 545'  '4 455'  2.055(4)    no
  P1    O1     .        .       1.5218(14)  no
  P1    O2     .        .       1.5441(15)  no
  P1    O3     .        .       1.5392(9)   no
  P1    O4     .        .       1.5382(9)   no
  P2    O5    '3 544'  '3 544'  1.5319(11)  no
  P2    O7    '3 544'  '3 544'  1.5457(13)  no
  P2    O6    '3 544'  '3 544'  1.5268(11)  no
  P2    O8    '3 544'  '3 544'  1.536(18)   no
 
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
  Sr1a  K1    Sr1b   .        .        .        13.7(11)    no
  Sr1a  K1    K2     .        .        .       149.0(10)    no
  Sr1a  K1    Sr2a   .        .        .       144.4(10)    no
  Sr1a  K1    Sr2b   .        .        .       131.7(10)    no
  Sr1a  K1    Ti1    .        .        .       151.3(9)     no
  Sr1a  K1    Cr1    .        .        .       147.1(9)     no
  Sr1a  K1    Ti2    .        .       '1 545'  102.4(8)     no
  Sr1a  K1    Cr2    .        .       '1 545'  100.7(8)     no
  Sr1a  K1    P1     .        .        .        95.4(8)     no
  Sr1a  K1    P2     .        .       '3 544'  147.3(8)     no
  Sr1a  K1    O1     .        .        .       116.9(9)     no
  Sr1a  K1    O2     .        .        .        67.5(8)     no
  Sr1a  K1    O3     .        .       '1 545'   86.6(8)     no
  Sr1a  K1    O11    .        .        .       143.6(8)     no
  Sr1a  K1    O12    .        .       '1 545'   84.8(9)     no
  Sr1a  K1    O5     .        .       '3 544'  152.6(10)    no
  Sr1a  K1    O7     .        .       '3 544'  135.6(8)     no
  Sr1a  K1    O8     .        .        .        90.6(10)    no
  Sr1a  K1    Ti2    .        .        .       116.1(8)     no
  Sr1a  K1    K2     .        .       '3 545'   40.0(8)     no
  Sr1a  K1    Sr2a   .        .       '3 545'   36.5(8)     no
  Sr1a  K1    K2     .        .        3        63.5(8)     no
  Sr1a  K1    K2     .        .        4       109.1(10)    no
  Sr1a  K1    Sr2a   .        .        4       104.3(10)    no
  Sr1a  K1    Sr2b   .        .        4        88.0(10)    no
  Sr1b  K1    K2     .        .        .       135.6(4)     no
  Sr1b  K1    Sr2a   .        .        .       130.9(5)     no
  Sr1b  K1    Sr2b   .        .        .       118.2(5)     no
  Sr1b  K1    Ti1    .        .        .       155.0(4)     no
  Sr1b  K1    Cr1    .        .        .       151.1(4)     no
  Sr1b  K1    Ti2    .        .       '1 545'   99.8(4)     no
  Sr1b  K1    Cr2    .        .       '1 545'   97.2(4)     no
  Sr1b  K1    P1     .        .        .        99.3(4)     no
  Sr1b  K1    P2     .        .       '3 544'  151.3(4)     no
  Sr1b  K1    O1     .        .        .       124.2(4)     no
  Sr1b  K1    O2     .        .        .        72.3(4)     no
  Sr1b  K1    O3     .        .       '1 545'   91.6(4)     no
  Sr1b  K1    O11    .        .        .       135.3(4)     no
  Sr1b  K1    O12    .        .       '1 545'   76.3(4)     no
  Sr1b  K1    O5     .        .       '3 544'  165.7(4)     no
  Sr1b  K1    O7     .        .       '3 544'  131.8(4)     no
  Sr1b  K1    O8     .        .        .        79.6(6)     no
  Sr1b  K1    Ti2    .        .        .       107.7(4)     no
  Sr1b  K1    K2     .        .       '3 545'   40.4(4)     no
  Sr1b  K1    Sr2a   .        .       '3 545'   36.2(4)     no
  Sr1b  K1    K2     .        .        3        58.7(4)     no
  Sr1b  K1    K2     .        .        4       122.6(4)     no
  Sr1b  K1    Sr2a   .        .        4       117.8(5)     no
  Sr1b  K1    Sr2b   .        .        4       101.3(5)     no
  K2    K1    Sr2a   .        .        .         4.67(11)   no
  K2    K1    Sr2b   .        .        .        17.34(19)   no
  K2    K1    Ti1    .        .        .        53.891(15)  no
  K2    K1    Cr1    .        .        .        57.50(10)   no
  K2    K1    Ti2    .        .       '1 545'   68.138(18)  no
  K2    K1    Cr2    .        .       '1 545'   67.46(8)    no
  K2    K1    P1     .        .        .       100.10(2)    no
  K2    K1    P2     .        .       '3 544'   49.584(15)  no
  K2    K1    O1     .        .        .        87.41(3)    no
  K2    K1    O2     .        .        .       124.75(3)    no
  K2    K1    O3     .        .       '1 545'   97.28(3)    no
  K2    K1    O11    .        .        .        38.52(2)    no
  K2    K1    O12    .        .       '1 545'   70.85(3)    no
  K2    K1    O5     .        .       '3 544'   56.93(3)    no
  K2    K1    O7     .        .       '3 544'   41.45(3)    no
  K2    K1    O8     .        .        .        69.4(4)     no
  K2    K1    Ti2    .        .        .        56.017(16)  no
  K2    K1    K2     .        .       '3 545'  123.16(2)    no
  K2    K1    Sr2a   .        .       '3 545'  124.70(10)   no
  K2    K1    K2     .        .        3       106.916(18)  no
  K2    K1    K2     .        .        4       101.84(3)    no
  K2    K1    Sr2a   .        .        4       106.59(13)   no
  K2    K1    Sr2b   .        .        4       123.0(2)     no
  Sr2a  K1    Sr2b   .        .        .        12.7(2)     no
  Sr2a  K1    Ti1    .        .        .        57.60(11)   no
  Sr2a  K1    Cr1    .        .        .        61.07(15)   no
  Sr2a  K1    Ti2    .        .       '1 545'   68.14(10)   no
  Sr2a  K1    Cr2    .        .       '1 545'   67.08(12)   no
  Sr2a  K1    P1     .        .        .       101.44(10)   no
  Sr2a  K1    P2     .        .       '3 544'   53.61(11)   no
  Sr2a  K1    O1     .        .        .        90.52(11)   no
  Sr2a  K1    O2     .        .        .       124.84(10)   no
  Sr2a  K1    O3     .        .       '1 545'   98.65(10)   no
  Sr2a  K1    O11    .        .        .        39.78(10)   no
  Sr2a  K1    O12    .        .       '1 545'   68.02(11)   no
  Sr2a  K1    O5     .        .       '3 544'   61.60(12)   no
  Sr2a  K1    O7     .        .       '3 544'   43.52(10)   no
  Sr2a  K1    O8     .        .        .        65.9(4)     no
  Sr2a  K1    Ti2    .        .        .        54.77(10)   no
  Sr2a  K1    K2     .        .       '3 545'  120.61(11)   no
  Sr2a  K1    Sr2a   .        .       '3 545'  121.84(15)   no
  Sr2a  K1    K2     .        .        3       104.18(10)   no
  Sr2a  K1    K2     .        .        4       106.47(12)   no
  Sr2a  K1    Sr2a   .        .        4       111.22(17)   no
  Sr2a  K1    Sr2b   .        .        4       127.6(2)     no
  Sr2b  K1    Ti1    .        .        .        69.31(18)   no
  Sr2b  K1    Cr1    .        .        .        72.5(2)     no
  Sr2b  K1    Ti2    .        .       '1 545'   66.30(14)   no
  Sr2b  K1    Cr2    .        .       '1 545'   64.23(16)   no
  Sr2b  K1    P1     .        .        .       107.19(14)   no
  Sr2b  K1    P2     .        .       '3 544'   63.54(18)   no
  Sr2b  K1    O1     .        .        .       100.77(17)   no
  Sr2b  K1    O2     .        .        .       126.37(14)   no
  Sr2b  K1    O3     .        .       '1 545'   99.49(14)   no
  Sr2b  K1    O11    .        .        .        47.30(16)   no
  Sr2b  K1    O12    .        .       '1 545'   58.79(16)   no
  Sr2b  K1    O5     .        .       '3 544'   74.0(2)     no
  Sr2b  K1    O7     .        .       '3 544'   48.42(16)   no
  Sr2b  K1    O8     .        .        .        59.0(3)     no
  Sr2b  K1    Ti2    .        .        .        55.34(14)   no
  Sr2b  K1    K2     .        .       '3 545'  111.09(17)   no
  Sr2b  K1    Sr2a   .        .       '3 545'  111.7(2)     no
  Sr2b  K1    K2     .        .        3        98.68(15)   no
  Sr2b  K1    K2     .        .        4       119.2(2)     no
  Sr2b  K1    Sr2a   .        .        4       123.9(2)     no
  Sr2b  K1    Sr2b   .        .        4       140.3(3)     no
  Ti1   K1    Cr1    .        .        .         4.21(10)   no
  Ti1   K1    Ti2    .        .       '1 545'  104.81(2)    no
  Ti1   K1    Cr2    .        .       '1 545'  107.09(9)    no
  Ti1   K1    P1     .        .        .        56.46(2)    no
  Ti1   K1    P2     .        .       '3 544'   53.566(16)  no
  Ti1   K1    O1     .        .        .        34.71(3)    no
  Ti1   K1    O2     .        .        .        84.19(3)    no
  Ti1   K1    O3     .        .       '1 545'  111.31(3)    no
  Ti1   K1    O11    .        .        .        31.34(2)    no
  Ti1   K1    O12    .        .       '1 545'  123.26(4)    no
  Ti1   K1    O5     .        .       '3 544'   32.86(2)    no
  Ti1   K1    O7     .        .       '3 544'   72.04(3)    no
  Ti1   K1    O8     .        .        .        85.9(4)     no
  Ti1   K1    Ti2    .        .        .        54.915(16)  no
  Ti1   K1    K2     .        .       '3 545'  163.50(2)    no
  Ti1   K1    Sr2a   .        .       '3 545'  167.70(11)   no
  Ti1   K1    K2     .        .        3        97.359(19)  no
  Ti1   K1    K2     .        .        4        56.333(17)  no
  Ti1   K1    Sr2a   .        .        4        60.41(12)   no
  Ti1   K1    Sr2b   .        .        4        73.32(19)   no
  Cr1   K1    Ti2    .        .       '1 545'  108.85(9)    no
  Cr1   K1    Cr2    .        .       '1 545'  111.20(13)   no
  Cr1   K1    P1     .        .        .        52.32(9)    no
  Cr1   K1    P2     .        .       '3 544'   57.20(9)    no
  Cr1   K1    O1     .        .        .        30.65(10)   no
  Cr1   K1    O2     .        .        .        80.01(10)   no
  Cr1   K1    O3     .        .       '1 545'  113.89(9)    no
  Cr1   K1    O11    .        .        .        32.30(10)   no
  Cr1   K1    O12    .        .       '1 545'  127.29(11)   no
  Cr1   K1    O5     .        .       '3 544'   35.61(9)    no
  Cr1   K1    O7     .        .       '3 544'   76.18(10)   no
  Cr1   K1    O8     .        .        .        85.3(4)     no
  Cr1   K1    Ti2    .        .        .        54.12(9)    no
  Cr1   K1    K2     .        .       '3 545'  165.60(9)    no
  Cr1   K1    Sr2a   .        .       '3 545'  169.46(14)   no
  Cr1   K1    K2     .        .        3        94.26(9)    no
  Cr1   K1    K2     .        .        4        54.95(10)   no
  Cr1   K1    Sr2a   .        .        4        58.82(16)   no
  Cr1   K1    Sr2b   .        .        4        70.9(2)     no
  Ti2   K1    Cr2   '1 545'   .       '1 545'    4.52(8)    no
  Ti2   K1    P1    '1 545'   .        .       160.49(3)    no
  Ti2   K1    P2    '1 545'   .       '3 544'   53.097(18)  no
  Ti2   K1    O1    '1 545'   .        .       133.14(4)    no
  Ti2   K1    O2    '1 545'   .        .       167.01(4)    no
  Ti2   K1    O3    '1 545'   .       '1 545'   34.17(2)    no
  Ti2   K1    O11   '1 545'   .        .       105.90(3)    no
  Ti2   K1    O12   '1 545'   .       '1 545'   34.76(3)    no
  Ti2   K1    O5    '1 545'   .       '3 544'   77.71(3)    no
  Ti2   K1    O7    '1 545'   .       '3 544'   33.23(3)    no
  Ti2   K1    O8    '1 545'   .        .       115.53(4)    no
  Ti2   K1    Ti2   '1 545'   .        .       121.63(2)    no
  Ti2   K1    K2    '1 545'   .       '3 545'   62.43(2)    no
  Ti2   K1    Sr2a  '1 545'   .       '3 545'   65.93(11)   no
  Ti2   K1    K2    '1 545'   .        3       145.67(2)    no
  Ti2   K1    K2    '1 545'   .        4       101.67(2)    no
  Ti2   K1    Sr2a  '1 545'   .        4       103.37(12)   no
  Ti2   K1    Sr2b  '1 545'   .        4       112.30(15)   no
  Cr2   K1    P1    '1 545'   .        .       163.45(9)    no
  Cr2   K1    P2    '1 545'   .       '3 544'   56.38(8)    no
  Cr2   K1    O1    '1 545'   .        .       136.74(9)    no
  Cr2   K1    O2    '1 545'   .        .       167.52(9)    no
  Cr2   K1    O3    '1 545'   .       '1 545'   37.38(8)    no
  Cr2   K1    O11   '1 545'   .        .       105.71(8)    no
  Cr2   K1    O12   '1 545'   .       '1 545'   30.28(8)    no
  Cr2   K1    O5    '1 545'   .       '3 544'   81.16(9)    no
  Cr2   K1    O7    '1 545'   .       '3 544'   35.07(9)    no
  Cr2   K1    O8    '1 545'   .        .       111.53(8)    no
  Cr2   K1    Ti2   '1 545'   .        .       119.51(8)    no
  Cr2   K1    K2    '1 545'   .       '3 545'   61.00(8)    no
  Cr2   K1    Sr2a  '1 545'   .       '3 545'   64.29(13)   no
  Cr2   K1    K2    '1 545'   .        3       141.19(8)    no
  Cr2   K1    K2    '1 545'   .        4       106.19(8)    no
  Cr2   K1    Sr2a  '1 545'   .        4       107.88(14)   no
  Cr2   K1    Sr2b  '1 545'   .        4       116.58(17)   no
  P1    K1    P2     .        .       '3 544'  107.39(3)    no
  P1    K1    O1     .        .        .        27.66(3)    no
  P1    K1    O2     .        .        .        27.92(3)    no
  P1    K1    O3     .        .       '1 545'  141.55(3)    no
  P1    K1    O11    .        .        .        61.69(3)    no
  P1    K1    O12    .        .       '1 545'  157.92(4)    no
  P1    K1    O5     .        .       '3 544'   82.81(3)    no
  P1    K1    O7     .        .       '3 544'  128.50(4)    no
  P1    K1    O8     .        .        .        71.69(14)   no
  P1    K1    Ti2    .        .        .        54.673(14)  no
  P1    K1    K2     .        .       '3 545'  134.54(3)    no
  P1    K1    Sr2a   .        .       '3 545'  131.57(11)   no
  P1    K1    K2     .        .        3        51.20(2)    no
  P1    K1    K2     .        .        4        64.47(2)    no
  P1    K1    Sr2a   .        .        4        63.99(11)   no
  P1    K1    Sr2b   .        .        4        59.98(14)   no
  P2    K1    O1    '3 544'   .        .        80.42(3)    no
  P2    K1    O2    '3 544'   .        .       132.04(4)    no
  P2    K1    O3    '3 544'   .       '1 545'   60.95(3)    no
  P2    K1    O11   '3 544'   .        .        69.09(3)    no
  P2    K1    O12   '3 544'   .       '1 545'   82.49(3)    no
  P2    K1    O5    '3 544'   .       '3 544'   24.87(2)    no
  P2    K1    O7    '3 544'   .       '3 544'   25.73(2)    no
  P2    K1    O8    '3 544'   .        .       118.3(4)     no
  P2    K1    Ti2   '3 544'   .        .        96.29(2)    no
  P2    K1    K2    '3 544'   .       '3 545'  111.03(2)    no
  P2    K1    Sr2a  '3 544'   .       '3 545'  115.16(11)   no
  P2    K1    K2    '3 544'   .        3       149.02(2)    no
  P2    K1    K2    '3 544'   .        4        63.25(2)    no
  P2    K1    Sr2a  '3 544'   .        4        67.35(13)   no
  P2    K1    Sr2b  '3 544'   .        4        83.7(2)     no
  O1    K1    O2     .        .        .        52.29(4)    no
  O1    K1    O3     .        .       '1 545'  120.95(4)    no
  O1    K1    O11    .        .        .        54.54(3)    no
  O1    K1    O12    .        .       '1 545'  157.93(5)    no
  O1    K1    O5     .        .       '3 544'   55.59(4)    no
  O1    K1    O7     .        .       '3 544'  103.73(4)    no
  O1    K1    O8     .        .        .        89.7(3)     no
  O1    K1    Ti2    .        .        .        62.93(3)    no
  O1    K1    K2     .        .       '3 545'  148.03(3)    no
  O1    K1    Sr2a   .        .       '3 545'  147.53(11)   no
  O1    K1    K2     .        .        3        78.37(3)    no
  O1    K1    K2     .        .        4        43.34(3)    no
  O1    K1    Sr2a   .        .        4        44.80(12)   no
  O1    K1    Sr2b   .        .        4        49.19(16)   no
  O2    K1    O3     .        .       '1 545'  133.90(4)    no
  O2    K1    O11    .        .        .        86.69(4)    no
  O2    K1    O12    .        .       '1 545'  145.19(5)    no
  O2    K1    O5     .        .       '3 544'  107.29(4)    no
  O2    K1    O7     .        .       '3 544'  155.92(5)    no
  O2    K1    O8     .        .        .        73.88(10)   no
  O2    K1    Ti2    .        .        .        71.16(3)    no
  O2    K1    K2     .        .       '3 545'  106.83(4)    no
  O2    K1    Sr2a   .        .       '3 545'  103.70(11)   no
  O2    K1    K2     .        .        3        38.22(3)    no
  O2    K1    K2     .        .        4        75.27(3)    no
  O2    K1    Sr2a   .        .        4        72.63(12)   no
  O2    K1    Sr2b   .        .        4        60.75(16)   no
  O3    K1    O11   '1 545'   .        .       129.26(4)    no
  O3    K1    O12   '1 545'   .       '1 545'   60.52(3)    no
  O3    K1    O5    '1 545'   .       '3 544'   78.45(4)    no
  O3    K1    O7    '1 545'   .       '3 544'   56.14(3)    no
  O3    K1    O8    '1 545'   .        .       146.75(14)   no
  O3    K1    Ti2   '1 545'   .        .       153.29(3)    no
  O3    K1    K2    '1 545'   .       '3 545'   52.21(3)    no
  O3    K1    Sr2a  '1 545'   .       '3 545'   56.43(11)   no
  O3    K1    K2    '1 545'   .        3       150.02(4)    no
  O3    K1    K2    '1 545'   .        4        78.55(3)    no
  O3    K1    Sr2a  '1 545'   .        4        78.27(11)   no
  O3    K1    Sr2b  '1 545'   .        4        81.80(14)   no
  O11   K1    O12    .        .       '1 545'  106.04(4)    no
  O11   K1    O5     .        .       '3 544'   58.03(3)    no
  O11   K1    O7     .        .       '3 544'   75.12(4)    no
  O11   K1    O8     .        .        .        56.6(4)     no
  O11   K1    Ti2    .        .        .        27.73(2)    no
  O11   K1    K2     .        .       '3 545'  157.11(3)    no
  O11   K1    Sr2a   .        .       '3 545'  156.13(11)   no
  O11   K1    K2     .        .        3        80.22(3)    no
  O11   K1    K2     .        .        4        87.25(3)    no
  O11   K1    Sr2a   .        .        4        91.04(12)   no
  O11   K1    Sr2b   .        .        4       101.77(18)   no
  O12   K1    O5    '1 545'   .       '3 544'  106.88(4)    no
  O12   K1    O7    '1 545'   .       '3 544'   57.32(4)    no
  O12   K1    O8    '1 545'   .        .        86.23(14)   no
  O12   K1    Ti2   '1 545'   .        .       105.48(3)    no
  O12   K1    K2    '1 545'   .       '3 545'   52.64(3)    no
  O12   K1    Sr2a  '1 545'   .       '3 545'   53.86(11)   no
  O12   K1    K2    '1 545'   .        3       110.91(4)    no
  O12   K1    K2    '1 545'   .        4       136.19(4)    no
  O12   K1    Sr2a  '1 545'   .        4       137.35(12)   no
  O12   K1    Sr2b  '1 545'   .        4       141.94(15)   no
  O5    K1    O7    '3 544'   .       '3 544'   49.57(3)    no
  O5    K1    O8    '3 544'   .        .       114.4(4)     no
  O5    K1    Ti2   '3 544'   .        .        85.18(3)    no
  O5    K1    K2    '3 544'   .       '3 545'  130.65(3)    no
  O5    K1    Sr2a  '3 544'   .       '3 545'  134.86(11)   no
  O5    K1    K2    '3 544'   .        3       129.73(3)    no
  O5    K1    K2    '3 544'   .        4        45.67(3)    no
  O5    K1    Sr2a  '3 544'   .        4        50.36(13)   no
  O5    K1    Sr2b  '3 544'   .        4        67.3(2)     no
  O7    K1    O8    '3 544'   .        .       107.4(3)     no
  O7    K1    Ti2   '3 544'   .        .        97.23(3)    no
  O7    K1    K2    '3 544'   .       '3 545'   95.65(3)    no
  O7    K1    Sr2a  '3 544'   .       '3 545'   99.15(11)   no
  O7    K1    K2    '3 544'   .        3       147.07(3)    no
  O7    K1    K2    '3 544'   .        4        88.01(3)    no
  O7    K1    Sr2a  '3 544'   .        4        91.75(13)   no
  O7    K1    Sr2b  '3 544'   .        4       107.16(19)   no
  O8    K1    Ti2    .        .        .        31.2(4)     no
  O8    K1    K2     .        .       '3 545'  108.7(4)     no
  O8    K1    Sr2a   .        .       '3 545'  105.2(4)     no
  O8    K1    K2     .        .        3        39.8(2)     no
  O8    K1    K2     .        .        4       133.0(3)     no
  O8    K1    Sr2a   .        .        4       134.1(3)     no
  O8    K1    Sr2b   .        .        4       131.25(17)   no
  Ti2   K1    K2     .        .       '3 545'  139.77(3)    no
  Ti2   K1    Sr2a   .        .       '3 545'  136.36(11)   no
  Ti2   K1    K2     .        .        3        53.794(17)  no
  Ti2   K1    K2     .        .        4       104.70(2)    no
  Ti2   K1    Sr2a   .        .        4       107.11(12)   no
  Ti2   K1    Sr2b   .        .        4       111.19(15)   no
  K2    K1    Sr2a  '3 545'   .       '3 545'    4.23(11)   no
  K2    K1    K2    '3 545'   .        3        98.83(2)    no
  K2    K1    K2    '3 545'   .        4       113.71(2)    no
  K2    K1    Sr2a  '3 545'   .        4       110.41(12)   no
  K2    K1    Sr2b  '3 545'   .        4       100.97(17)   no
  Sr2a  K1    K2    '3 545'   .        3        94.61(11)   no
  Sr2a  K1    K2    '3 545'   .        4       116.01(11)   no
  Sr2a  K1    Sr2a  '3 545'   .        4       112.48(16)   no
  Sr2a  K1    Sr2b  '3 545'   .        4       102.1(2)     no
  K2    K1    K2     3        .        4       112.45(2)    no
  K2    K1    Sr2a   3        .        4       110.35(12)   no
  K2    K1    Sr2b   3        .        4        98.91(16)   no
  K2    K1    Sr2a   4        .        4         4.75(13)   no
  K2    K1    Sr2b   4        .        4        21.7(2)     no
  Sr2a  K1    Sr2b   4        .        4        17.0(2)     no
  K1    Sr1a  Sr1b   .        .        .       160.8(15)    no
  K1    Sr1a  K2     .        .        .        28.4(9)     no
  K1    Sr1a  Sr2a   .        .        .        32.5(9)     no
  K1    Sr1a  Sr2b   .        .        .        43.6(9)     no
  K1    Sr1a  Ti2    .        .       '1 545'   71.3(8)     no
  K1    Sr1a  Cr2    .        .       '1 545'   72.3(8)     no
  K1    Sr1a  P1     .        .        .        77.4(8)     no
  K1    Sr1a  O1     .        .        .        56.2(9)     no
  K1    Sr1a  O2     .        .        .       103.9(9)     no
  K1    Sr1a  O3     .        .       '1 545'   84.5(8)     no
  K1    Sr1a  O12    .        .       '1 545'   86.3(9)     no
  K1    Sr1a  O6     .        .        4       139.1(11)    no
  K1    Sr1a  O8     .        .        .        80.7(10)    no
  K1    Sr1a  K2     .        .       '3 545'  135.6(9)     no
  K1    Sr1a  Sr2a   .        .       '3 545'  139.7(9)     no
  K1    Sr1a  Sr2b   .        .       '3 545'  143.8(9)     no
  K1    Sr1a  K2     .        .        3       111.6(8)     no
  K1    Sr1a  Sr2a   .        .        3       115.5(9)     no
  K1    Sr1a  K2     .        .        4        65.3(10)    no
  K1    Sr1a  Sr2a   .        .        4        69.5(10)    no
  K1    Sr1a  Sr2b   .        .        4        84.8(10)    no
  Sr1b  Sr1a  K2     .        .        .       132.7(8)     no
  Sr1b  Sr1a  Sr2a   .        .        .       128.6(8)     no
  Sr1b  Sr1a  Sr2b   .        .        .       117.6(8)     no
  Sr1b  Sr1a  Ti2    .        .       '1 545'  104.6(7)     no
  Sr1b  Sr1a  Cr2    .        .       '1 545'  102.3(7)     no
  Sr1b  Sr1a  P1     .        .        .       107.6(7)     no
  Sr1b  Sr1a  O1     .        .        .       133.2(7)     no
  Sr1b  Sr1a  O2     .        .        .        82.6(7)     no
  Sr1b  Sr1a  O3     .        .       '1 545'  102.0(7)     no
  Sr1b  Sr1a  O12    .        .       '1 545'   81.5(7)     no
  Sr1b  Sr1a  O6     .        .        4        59.3(7)     no
  Sr1b  Sr1a  O8     .        .        .        83.7(9)     no
  Sr1b  Sr1a  K2     .        .       '3 545'   45.5(7)     no
  Sr1b  Sr1a  Sr2a   .        .       '3 545'   40.6(7)     no
  Sr1b  Sr1a  Sr2b   .        .       '3 545'   33.5(7)     no
  Sr1b  Sr1a  K2     .        .        3        61.9(7)     no
  Sr1b  Sr1a  Sr2a   .        .        3        57.7(7)     no
  Sr1b  Sr1a  K2     .        .        4       133.6(8)     no
  Sr1b  Sr1a  Sr2a   .        .        4       129.5(8)     no
  Sr1b  Sr1a  Sr2b   .        .        4       113.9(8)     no
  K2    Sr1a  Sr2a   .        .        .         4.17(11)   no
  K2    Sr1a  Sr2b   .        .        .        15.19(18)   no
  K2    Sr1a  Ti2    .        .       '1 545'   63.17(11)   no
  K2    Sr1a  Cr2    .        .       '1 545'   62.08(14)   no
  K2    Sr1a  P1     .        .        .        92.29(16)   no
  K2    Sr1a  O1     .        .        .        78.74(16)   no
  K2    Sr1a  O2     .        .        .       116.5(2)     no
  K2    Sr1a  O3     .        .       '1 545'   89.19(18)   no
  K2    Sr1a  O12    .        .       '1 545'   64.40(15)   no
  K2    Sr1a  O6     .        .        4       167.1(2)     no
  K2    Sr1a  O8     .        .        .        63.0(4)     no
  K2    Sr1a  K2     .        .       '3 545'  121.20(16)   no
  K2    Sr1a  Sr2a   .        .       '3 545'  123.4(2)     no
  K2    Sr1a  Sr2b   .        .       '3 545'  123.5(2)     no
  K2    Sr1a  K2     .        .        3       103.67(13)   no
  K2    Sr1a  Sr2a   .        .        3       106.30(16)   no
  K2    Sr1a  K2     .        .        4        93.62(16)   no
  K2    Sr1a  Sr2a   .        .        4        97.8(2)     no
  K2    Sr1a  Sr2b   .        .        4       113.2(3)     no
  Sr2a  Sr1a  Sr2b   .        .        .       11.1(2)      no
  Sr2a  Sr1a  Ti2    .        .       '1 545'   63.38(14)   no
  Sr2a  Sr1a  Cr2    .        .       '1 545'   61.97(16)   no
  Sr2a  Sr1a  P1     .        .        .        93.71(18)   no
  Sr2a  Sr1a  O1     .        .        .        81.63(19)   no
  Sr2a  Sr1a  O2     .        .        .       117.1(2)     no
  Sr2a  Sr1a  O3     .        .       '1 545'   90.8(2)     no
  Sr2a  Sr1a  O12    .        .       '1 545'   62.06(17)   no
  Sr2a  Sr1a  O6     .        .        4       170.6(2)     no
  Sr2a  Sr1a  O8     .        .        .        60.0(4)     no
  Sr2a  Sr1a  K2     .        .       '3 545'  119.2(2)     no
  Sr2a  Sr1a  Sr2a   .        .       '3 545'  121.1(2)     no
  Sr2a  Sr1a  Sr2b   .        .       '3 545'  120.7(2)     no
  Sr2a  Sr1a  K2     .        .        3       101.41(16)   no
  Sr2a  Sr1a  Sr2a   .        .        3       103.83(18)   no
  Sr2a  Sr1a  K2     .        .        4        97.8(2)     no
  Sr2a  Sr1a  Sr2a   .        .        4       101.9(2)     no
  Sr2a  Sr1a  Sr2b   .        .        4       117.2(3)     no
  Sr2b  Sr1a  Ti2    .        .       '1 545'   62.30(17)   no
  Sr2b  Sr1a  Cr2    .        .       '1 545'   60.07(18)   no
  Sr2b  Sr1a  P1     .        .        .        99.6(2)     no
  Sr2b  Sr1a  O1     .        .        .        90.9(2)     no
  Sr2b  Sr1a  O2     .        .        .       120.2(2)     no
  Sr2b  Sr1a  O3     .        .       '1 545'   92.6(2)     no
  Sr2b  Sr1a  O12    .        .       '1 545'   54.4(2)     no
  Sr2b  Sr1a  O6     .        .        4       174.7(3)     no
  Sr2b  Sr1a  O8     .        .        .        54.6(4)     no
  Sr2b  Sr1a  K2     .        .       '3 545'  111.5(2)     no
  Sr2b  Sr1a  Sr2a   .        .       '3 545'  112.8(3)     no
  Sr2b  Sr1a  Sr2b   .        .       '3 545'  111.3(3)     no
  Sr2b  Sr1a  K2     .        .        3        97.3(2)     no
  Sr2b  Sr1a  Sr2a   .        .        3        99.1(2)     no
  Sr2b  Sr1a  K2     .        .        4       108.8(3)     no
  Sr2b  Sr1a  Sr2a   .        .        4       113.0(3)     no
  Sr2b  Sr1a  Sr2b   .        .        4       128.3(4)     no
  Ti2   Sr1a  Cr2   '1 545'   .       '1 545'    4.19(8)    no
  Ti2   Sr1a  P1    '1 545'   .        .       147.7(3)     no
  Ti2   Sr1a  O1    '1 545'   .        .       121.8(2)     no
  Ti2   Sr1a  O2    '1 545'   .        .       170.5(3)     no
  Ti2   Sr1a  O3    '1 545'   .       '1 545'   32.56(8)    no
  Ti2   Sr1a  O12   '1 545'   .       '1 545'   33.09(8)    no
  Ti2   Sr1a  O6    '1 545'   .        4       122.03(18)   no
  Ti2   Sr1a  O8    '1 545'   .        .       111.3(2)     no
  Ti2   Sr1a  K2    '1 545'   .       '3 545'   64.36(10)   no
  Ti2   Sr1a  Sr2a  '1 545'   .       '3 545'   68.48(16)   no
  Ti2   Sr1a  Sr2b  '1 545'   .       '3 545'   73.34(17)   no
  Ti2   Sr1a  K2    '1 545'   .        3       148.6(2)     no
  Ti2   Sr1a  Sr2a  '1 545'   .        3       146.9(2)     no
  Ti2   Sr1a  K2    '1 545'   .        4        96.87(16)   no
  Ti2   Sr1a  Sr2a  '1 545'   .        4        98.8(2)     no
  Ti2   Sr1a  Sr2b  '1 545'   .        4       109.3(2)     no
  Cr2   Sr1a  P1    '1 545'   .        .       149.4(3)     no
  Cr2   Sr1a  O1    '1 545'   .        .       124.3(3)     no
  Cr2   Sr1a  O2    '1 545'   .        .       174.4(3)     no
  Cr2   Sr1a  O3    '1 545'   .       '1 545'   36.11(11)   no
  Cr2   Sr1a  O12   '1 545'   .       '1 545'   28.97(10)   no
  Cr2   Sr1a  O6    '1 545'   .        4       124.0(2)     no
  Cr2   Sr1a  O8    '1 545'   .        .       107.7(2)     no
  Cr2   Sr1a  K2    '1 545'   .       '3 545'   63.60(13)   no
  Cr2   Sr1a  Sr2a  '1 545'   .       '3 545'   67.51(18)   no
  Cr2   Sr1a  Sr2b  '1 545'   .       '3 545'   71.9(2)     no
  Cr2   Sr1a  K2    '1 545'   .        3       144.4(2)     no
  Cr2   Sr1a  Sr2a  '1 545'   .        3       142.7(2)     no
  Cr2   Sr1a  K2    '1 545'   .        4       100.9(2)     no
  Cr2   Sr1a  Sr2a  '1 545'   .        4       102.9(2)     no
  Cr2   Sr1a  Sr2b  '1 545'   .        4       113.5(3)     no
  P1    Sr1a  O1     .        .        .        26.96(6)    no
  P1    Sr1a  O2     .        .        .        26.52(7)    no
  P1    Sr1a  O3     .        .       '1 545'  137.7(3)     no
  P1    Sr1a  O12    .        .       '1 545'  152.6(3)     no
  P1    Sr1a  O6     .        .        4        78.05(15)   no
  P1    Sr1a  O8     .        .        .        70.2(2)     no
  P1    Sr1a  K2     .        .       '3 545'  145.8(2)     no
  P1    Sr1a  Sr2a   .        .       '3 545'  142.4(3)     no
  P1    Sr1a  Sr2b   .        .       '3 545'  138.6(3)     no
  P1    Sr1a  K2     .        .        3        53.09(9)    no
  P1    Sr1a  Sr2a   .        .        3        56.68(14)   no
  P1    Sr1a  K2     .        .        4        62.08(12)   no
  P1    Sr1a  Sr2a   .        .        4        61.98(16)   no
  P1    Sr1a  Sr2b   .        .        4        59.21(18)   no
  O1    Sr1a  O2     .        .        .        50.63(12)   no
  O1    Sr1a  O3     .        .       '1 545'  113.6(3)     no
  O1    Sr1a  O12    .        .       '1 545'  142.2(3)     no
  O1    Sr1a  O6     .        .        4        88.96(18)   no
  O1    Sr1a  O8     .        .        .        84.8(4)     no
  O1    Sr1a  K2     .        .       '3 545'  155.0(2)     no
  O1    Sr1a  Sr2a   .        .       '3 545'  155.6(3)     no
  O1    Sr1a  Sr2b   .        .       '3 545'  157.7(3)     no
  O1    Sr1a  K2     .        .        3        79.31(12)   no
  O1    Sr1a  Sr2a   .        .        3        83.12(16)   no
  O1    Sr1a  K2     .        .        4        41.28(10)   no
  O1    Sr1a  Sr2a   .        .        4        42.83(15)   no
  O1    Sr1a  Sr2b   .        .        4        47.8(2)     no
  O2    Sr1a  O3     .        .       '1 545'  140.6(3)     no
  O2    Sr1a  O12    .        .       '1 545'  156.4(3)     no
  O2    Sr1a  O6     .        .        4        56.16(14)   no
  O2    Sr1a  O8     .        .        .        75.32(17)   no
  O2    Sr1a  K2     .        .       '3 545'  119.7(3)     no
  O2    Sr1a  Sr2a   .        .       '3 545'  116.0(3)     no
  O2    Sr1a  Sr2b   .        .       '3 545'  112.2(3)     no
  O2    Sr1a  K2     .        .        3        40.56(11)   no
  O2    Sr1a  Sr2a   .        .        3        42.53(15)   no
  O2    Sr1a  K2     .        .        4        73.58(17)   no
  O2    Sr1a  Sr2a   .        .        4        71.6(2)     no
  O2    Sr1a  Sr2b   .        .        4        61.6(2)     no
  O3    Sr1a  O12   '1 545'   .       '1 545'   60.49(13)   no
  O3    Sr1a  O6    '1 545'   .        4        92.27(19)   no
  O3    Sr1a  O8    '1 545'   .        .       143.8(3)     no
  O3    Sr1a  K2    '1 545'   .       '3 545'   56.76(12)   no
  O3    Sr1a  Sr2a  '1 545'   .       '3 545'   61.63(17)   no
  O3    Sr1a  Sr2b  '1 545'   .       '3 545'   69.25(18)   no
  O3    Sr1a  K2    '1 545'   .        3       163.7(3)     no
  O3    Sr1a  Sr2a  '1 545'   .        3       159.5(3)     no
  O3    Sr1a  K2    '1 545'   .        4        75.60(17)   no
  O3    Sr1a  Sr2a  '1 545'   .        4        75.9(2)     no
  O3    Sr1a  Sr2b  '1 545'   .        4        81.5(2)     no
  O12   Sr1a  O6    '1 545'   .        4       127.0(3)     no
  O12   Sr1a  O8    '1 545'   .        .        85.6(2)     no
  O12   Sr1a  K2    '1 545'   .       '3 545'   57.29(13)   no
  O12   Sr1a  Sr2a  '1 545'   .       '3 545'   59.08(17)   no
  O12   Sr1a  Sr2b  '1 545'   .       '3 545'   59.5(2)     no
  O12   Sr1a  K2    '1 545'   .        3       115.9(2)     no
  O12   Sr1a  Sr2a  '1 545'   .        3       113.9(2)     no
  O12   Sr1a  K2    '1 545'   .        4       129.8(2)     no
  O12   Sr1a  Sr2a  '1 545'   .        4       131.9(3)     no
  O12   Sr1a  Sr2b  '1 545'   .        4       141.6(3)     no
  O6    Sr1a  O8     4        .        .       120.1(4)     no
  O6    Sr1a  K2     4        .       '3 545'   69.72(15)   no
  O6    Sr1a  Sr2a   4        .       '3 545'   68.06(18)   no
  O6    Sr1a  Sr2b   4        .       '3 545'   68.7(2)     no
  O6    Sr1a  K2     4        .        3        77.46(14)   no
  O6    Sr1a  Sr2a   4        .        3        75.65(17)   no
  O6    Sr1a  K2     4        .        4        74.39(14)   no
  O6    Sr1a  Sr2a   4        .        4        70.24(19)   no
  O6    Sr1a  Sr2b   4        .        4        54.5(2)     no
  O8    Sr1a  K2     .        .       '3 545'  116.8(5)     no
  O8    Sr1a  Sr2a   .        .       '3 545'  113.3(5)     no
  O8    Sr1a  Sr2b   .        .       '3 545'  105.8(5)     no
  O8    Sr1a  K2     .        .        3        42.9(3)     no
  O8    Sr1a  Sr2a   .        .        3        44.5(3)     no
  O8    Sr1a  K2     .        .        4       125.7(4)     no
  O8    Sr1a  Sr2a   .        .        4       127.6(4)     no
  O8    Sr1a  Sr2b   .        .        4       129.3(3)     no
  K2    Sr1a  Sr2a  '3 545'   .       '3 545'    4.88(12)   no
  K2    Sr1a  Sr2b  '3 545'   .       '3 545'   12.66(13)   no
  K2    Sr1a  K2    '3 545'   .        3       107.3(2)     no
  K2    Sr1a  Sr2a  '3 545'   .        3       103.1(2)     no
  K2    Sr1a  K2    '3 545'   .        4       117.21(17)   no
  K2    Sr1a  Sr2a  '3 545'   .        4       114.7(2)     no
  K2    Sr1a  Sr2b  '3 545'   .        4       107.5(2)     no
  Sr2a  Sr1a  Sr2b  '3 545'   .       '3 545'    8.01(17)   no
  Sr2a  Sr1a  K2    '3 545'   .        3       102.4(2)     no
  Sr2a  Sr1a  Sr2a  '3 545'   .        3        98.2(2)     no
  Sr2a  Sr1a  K2    '3 545'   .        4       120.2(2)     no
  Sr2a  Sr1a  Sr2a  '3 545'   .        4       117.4(2)     no
  Sr2a  Sr1a  Sr2b  '3 545'   .        4       109.0(3)     no
  Sr2b  Sr1a  K2    '3 545'   .        3        95.0(2)     no
  Sr2b  Sr1a  Sr2a  '3 545'   .        3        90.8(2)     no
  Sr2b  Sr1a  K2    '3 545'   .        4       126.9(2)     no
  Sr2b  Sr1a  Sr2a  '3 545'   .        4       123.9(2)     no
  Sr2b  Sr1a  Sr2b  '3 545'   .        4       114.1(3)     no
  K2    Sr1a  Sr2a   3        .        3         4.19(10)   no
  K2    Sr1a  K2     3        .        4       112.92(15)   no
  K2    Sr1a  Sr2a   3        .        4       111.56(19)   no
  K2    Sr1a  Sr2b   3        .        4       102.1(2)     no
  Sr2a  Sr1a  K2     3        .        4       115.62(17)   no
  Sr2a  Sr1a  Sr2a   3        .        4       114.0(2)     no
  Sr2a  Sr1a  Sr2b   3        .        4       103.7(2)     no
  K2    Sr1a  Sr2a   4        .        4         4.15(12)   no
  K2    Sr1a  Sr2b   4        .        4        20.1(2)     no
  Sr2a  Sr1a  Sr2b   4        .        4        16.0(2)     no
  K1    Sr1b  Sr1a   .        .        .         5.5(4)     no
  K1    Sr1b  Sr2b   .        .        .        44.9(4)     no
  K1    Sr1b  O2     .        .        .        76.9(5)     no
  K1    Sr1b  O3     .        .       '1 545'   60.9(4)     no
  K1    Sr1b  O4     .        .       '2 665'  173.0(6)     no
  K1    Sr1b  O12    .        .       '1 545'   73.2(4)     no
  K1    Sr1b  O6     .        .        4       107.6(6)     no
  K1    Sr1b  O8     .        .        .        70.9(6)     no
  K1    Sr1b  Ti1    .        .       '2 665'  104.2(5)     no
  K1    Sr1b  Cr1    .        .       '2 665'  109.3(5)     no
  K1    Sr1b  O1     .        .       '2 665'  133.6(6)     no
  K1    Sr1b  K2     .        .       '3 545'  120.7(6)     no
  K1    Sr1b  Sr2a   .        .       '3 545'  127.7(6)     no
  K1    Sr1b  Sr2b   .        .       '3 545'  138.3(6)     no
  K1    Sr1b  Ti1    .        .       '3 545'   92.7(5)     no
  K1    Sr1b  O11    .        .       '3 545'  124.4(6)     no
  K1    Sr1b  K2     .        .        3       103.6(5)     no
  K1    Sr1b  Sr2a   .        .        3       108.7(5)     no
  K1    Sr1b  Sr2b   .        .        3       120.9(5)     no
  K1    Sr1b  Ti2    .        .       '3 545'  141.4(6)     no
  K1    Sr1b  P2     .        .        .        92.1(5)     no
  K1    Sr1b  O7     .        .        .       118.4(6)     no
  K1    Sr1b  Sr2a   .        .        4        45.7(4)     no
  K1    Sr1b  Sr2b   .        .        4        57.4(4)     no
  Sr1a  Sr1b  Sr2b   .        .        .        50.3(7)     no
  Sr1a  Sr1b  O2     .        .        .        74.9(7)     no
  Sr1a  Sr1b  O3     .        .       '1 545'   59.0(6)     no
  Sr1a  Sr1b  O4     .        .       '2 665'  177.7(9)     no
  Sr1a  Sr1b  O12    .        .       '1 545'   76.7(7)     no
  Sr1a  Sr1b  O6     .        .        4       102.2(8)     no
  Sr1a  Sr1b  O8     .        .        .        75.3(8)     no
  Sr1a  Sr1b  Ti1    .        .       '2 665'  100.5(8)     no
  Sr1a  Sr1b  Cr1    .        .       '2 665'  105.7(8)     no
  Sr1a  Sr1b  O1     .        .       '2 665'  131.8(8)     no
  Sr1a  Sr1b  K2     .        .       '3 545'  119.7(8)     no
  Sr1a  Sr1b  Sr2a   .        .       '3 545'  126.7(8)     no
  Sr1a  Sr1b  Sr2b   .        .       '3 545'  138.0(8)     no
  Sr1a  Sr1b  Ti1    .        .       '3 545'   97.2(8)     no
  Sr1a  Sr1b  O11    .        .       '3 545'  128.9(8)     no
  Sr1a  Sr1b  K2     .        .        3       105.1(7)     no
  Sr1a  Sr1b  Sr2a   .        .        3       110.3(7)     no
  Sr1a  Sr1b  Sr2b   .        .        3       122.9(8)     no
  Sr1a  Sr1b  Ti2    .        .       '3 545'  146.9(9)     no
  Sr1a  Sr1b  P2     .        .        .        97.3(8)     no
  Sr1a  Sr1b  O7     .        .        .       123.3(8)     no
  Sr1a  Sr1b  Sr2a   .        .        4        40.3(7)     no
  Sr1a  Sr1b  Sr2b   .        .        4        52.0(7)     no
  Sr2b  Sr1b  O2     .        .        .       102.0(3)     no
  Sr2b  Sr1b  O3     .        .       '1 545'   77.3(3)     no
  Sr2b  Sr1b  O4     .        .       '2 665'  128.8(4)     no
  Sr2b  Sr1b  O12    .        .       '1 545'   45.4(2)     no
  Sr2b  Sr1b  O6     .        .        4       152.2(4)     no
  Sr2b  Sr1b  O8     .        .        .        46.0(4)     no
  Sr2b  Sr1b  Ti1    .        .       '2 665'  134.7(3)     no
  Sr2b  Sr1b  Cr1    .        .       '2 665'  137.3(3)     no
  Sr2b  Sr1b  O1     .        .       '2 665'  135.6(3)     no
  Sr2b  Sr1b  K2     .        .       '3 545'  111.2(3)     no
  Sr2b  Sr1b  Sr2a   .        .       '3 545'  114.8(3)     no
  Sr2b  Sr1b  Sr2b   .        .       '3 545'  116.8(3)     no
  Sr2b  Sr1b  Ti1    .        .       '3 545'   52.6(2)     no
  Sr2b  Sr1b  O11    .        .       '3 545'   82.8(3)     no
  Sr2b  Sr1b  K2     .        .        3        94.6(2)     no
  Sr2b  Sr1b  Sr2a   .        .        3        97.8(3)     no
  Sr2b  Sr1b  Sr2b   .        .        3       102.9(3)     no
  Sr2b  Sr1b  Ti2    .        .       '3 545'   96.7(3)     no
  Sr2b  Sr1b  P2     .        .        .        54.1(2)     no
  Sr2b  Sr1b  O7     .        .        .        80.6(3)     no
  Sr2b  Sr1b  Sr2a   .        .        4        90.6(3)     no
  Sr2b  Sr1b  Sr2b   .        .        4       102.2(4)     no
  O2    Sr1b  O3     .        .       '1 545'  120.1(4)     no
  O2    Sr1b  O4     .        .       '2 665'  103.7(4)     no
  O2    Sr1b  O12    .        .       '1 545'  146.6(5)     no
  O2    Sr1b  O6     .        .        4        60.8(2)     no
  O2    Sr1b  O8     .        .        .        73.0(3)     no
  O2    Sr1b  Ti1    .        .       '2 665'   32.82(13)   no
  O2    Sr1b  Cr1    .        .       '2 665'   36.20(17)   no
  O2    Sr1b  O1     .        .       '2 665'   56.9(2)     no
  O2    Sr1b  K2     .        .       '3 545'  145.4(4)     no
  O2    Sr1b  Sr2a   .        .       '3 545'  143.1(5)     no
  O2    Sr1b  Sr2b   .        .       '3 545'  140.0(4)     no
  O2    Sr1b  Ti1    .        .       '3 545'  145.8(4)     no
  O2    Sr1b  O11    .        .       '3 545'  143.7(4)     no
  O2    Sr1b  K2     .        .        3        47.40(17)   no
  O2    Sr1b  Sr2a   .        .        3        50.9(2)     no
  O2    Sr1b  Sr2b   .        .        3        62.2(3)     no
  O2    Sr1b  Ti2    .        .       '3 545'  116.3(4)     no
  O2    Sr1b  P2     .        .        .        93.0(3)     no
  O2    Sr1b  O7     .        .        .        92.9(3)     no
  O2    Sr1b  Sr2a   .        .        4        58.5(2)     no
  O2    Sr1b  Sr2b   .        .        4        52.9(2)     no
  O3    Sr1b  O4    '1 545'   .       '2 665'  123.3(4)     no
  O3    Sr1b  O12   '1 545'   .       '1 545'   55.3(2)     no
  O3    Sr1b  O6    '1 545'   .        4        92.4(3)     no
  O3    Sr1b  O8    '1 545'   .        .       122.6(5)     no
  O3    Sr1b  Ti1   '1 545'   .       '2 665'  120.7(3)     no
  O3    Sr1b  Cr1   '1 545'   .       '2 665'  124.6(4)     no
  O3    Sr1b  O1    '1 545'   .       '2 665'  146.6(4)     no
  O3    Sr1b  K2    '1 545'   .       '3 545'   60.9(2)     no
  O3    Sr1b  Sr2a  '1 545'   .       '3 545'   67.9(3)     no
  O3    Sr1b  Sr2b  '1 545'   .       '3 545'   79.7(3)     no
  O3    Sr1b  Ti1   '1 545'   .       '3 545'   80.0(2)     no
  O3    Sr1b  O11   '1 545'   .       '3 545'   96.1(3)     no
  O3    Sr1b  K2    '1 545'   .        3       163.9(4)     no
  O3    Sr1b  Sr2a  '1 545'   .        3       169.1(4)     no
  O3    Sr1b  Sr2b  '1 545'   .        3       177.6(4)     no
  O3    Sr1b  Ti2   '1 545'   .       '3 545'  123.3(3)     no
  O3    Sr1b  P2    '1 545'   .        .       126.5(4)     no
  O3    Sr1b  O7    '1 545'   .        .       143.2(4)     no
  O3    Sr1b  Sr2a  '1 545'   .        4        61.7(2)     no
  O3    Sr1b  Sr2b  '1 545'   .        4        68.6(3)     no
  O4    Sr1b  O12   '2 665'   .       '1 545'  104.2(4)     no
  O4    Sr1b  O6    '2 665'   .        4        78.4(3)     no
  O4    Sr1b  O8    '2 665'   .        .       102.6(6)     no
  O4    Sr1b  Ti1   '2 665'   .       '2 665'   78.8(3)     no
  O4    Sr1b  Cr1   '2 665'   .       '2 665'   73.5(3)     no
  O4    Sr1b  O1    '2 665'   .       '2 665'   46.82(18)   no
  O4    Sr1b  K2    '2 665'   .       '3 545'   62.5(2)     no
  O4    Sr1b  Sr2a  '2 665'   .       '3 545'   55.5(3)     no
  O4    Sr1b  Sr2b  '2 665'   .       '3 545'   44.1(2)     no
  O4    Sr1b  Ti1   '2 665'   .       '3 545'   83.0(3)     no
  O4    Sr1b  O11   '2 665'   .       '3 545'   51.4(2)     no
  O4    Sr1b  K2    '2 665'   .        3        72.7(2)     no
  O4    Sr1b  Sr2a  '2 665'   .        3        67.4(2)     no
  O4    Sr1b  Sr2b  '2 665'   .        3        54.8(2)     no
  O4    Sr1b  Ti2   '2 665'   .       '3 545'   32.14(12)   no
  O4    Sr1b  P2    '2 665'   .        .        81.0(3)     no
  O4    Sr1b  O7    '2 665'   .        .        54.8(2)     no
  O4    Sr1b  Sr2a  '2 665'   .        4       140.4(3)     no
  O4    Sr1b  Sr2b  '2 665'   .        4       128.6(4)     no
  O12   Sr1b  O6    '1 545'   .        4       143.7(4)     no
  O12   Sr1b  O8    '1 545'   .        .        83.3(3)     no
  O12   Sr1b  Ti1   '1 545'   .       '2 665'  175.9(4)     no
  O12   Sr1b  Cr1   '1 545'   .       '2 665'  177.2(5)     no
  O12   Sr1b  O1    '1 545'   .       '2 665'  147.8(5)     no
  O12   Sr1b  K2    '1 545'   .       '3 545'   65.8(2)     no
  O12   Sr1b  Sr2a  '1 545'   .       '3 545'   69.6(3)     no
  O12   Sr1b  Sr2b  '1 545'   .       '3 545'   73.3(3)     no
  O12   Sr1b  Ti1   '1 545'   .       '3 545'   26.24(11)   no
  O12   Sr1b  O11   '1 545'   .       '3 545'   53.8(2)     no
  O12   Sr1b  K2    '1 545'   .        3       127.3(3)     no
  O12   Sr1b  Sr2a  '1 545'   .        3       127.4(4)     no
  O12   Sr1b  Sr2b  '1 545'   .        3       123.2(4)     no
  O12   Sr1b  Ti2   '1 545'   .       '3 545'   80.4(3)     no
  O12   Sr1b  P2    '1 545'   .        .        73.7(3)     no
  O12   Sr1b  O7    '1 545'   .        .        88.4(3)     no
  O12   Sr1b  Sr2a  '1 545'   .        4       107.3(4)     no
  O12   Sr1b  Sr2b  '1 545'   .        4       118.1(4)     no
  O6    Sr1b  O8     4        .        .       132.2(4)     no
  O6    Sr1b  Ti1    4        .       '2 665'   33.56(13)   no
  O6    Sr1b  Cr1    4        .       '2 665'   34.82(16)   no
  O6    Sr1b  O1     4        .       '2 665'   55.9(2)     no
  O6    Sr1b  K2     4        .       '3 545'   84.9(3)     no
  O6    Sr1b  Sr2a   4        .       '3 545'   83.8(3)     no
  O6    Sr1b  Sr2b   4        .       '3 545'   85.9(3)     no
  O6    Sr1b  Ti1    4        .       '3 545'  151.6(4)     no
  O6    Sr1b  O11    4        .       '3 545'  124.4(4)     no
  O6    Sr1b  K2     4        .        3        88.5(3)     no
  O6    Sr1b  Sr2a   4        .        3        87.6(3)     no
  O6    Sr1b  Sr2b   4        .        3        88.5(3)     no
  O6    Sr1b  Ti2    4        .       '3 545'  110.4(4)     no
  O6    Sr1b  P2     4        .        .       141.0(4)     no
  O6    Sr1b  O7     4        .        .       119.6(4)     no
  O6    Sr1b  Sr2a   4        .        4        62.0(2)     no
  O6    Sr1b  Sr2b   4        .        4        50.2(3)     no
  O8    Sr1b  Ti1    .        .       '2 665'   98.9(3)     no
  O8    Sr1b  Cr1    .        .       '2 665'   98.7(3)     no
  O8    Sr1b  O1     .        .       '2 665'   89.7(4)     no
  O8    Sr1b  K2     .        .       '3 545'  138.7(5)     no
  O8    Sr1b  Sr2a   .        .       '3 545'  136.6(5)     no
  O8    Sr1b  Sr2b   .        .       '3 545'  128.2(5)     no
  O8    Sr1b  Ti1    .        .       '3 545'   72.8(3)     no
  O8    Sr1b  O11    .        .       '3 545'   86.3(4)     no
  O8    Sr1b  K2     .        .        3        48.7(3)     no
  O8    Sr1b  Sr2a   .        .        3        51.8(4)     no
  O8    Sr1b  Sr2b   .        .        3        57.9(4)     no
  O8    Sr1b  Ti2    .        .       '3 545'   78.6(5)     no
  O8    Sr1b  P2     .        .        .        26.6(4)     no
  O8    Sr1b  O7     .        .        .        48.5(5)     no
  O8    Sr1b  Sr2a   .        .        4       104.3(5)     no
  O8    Sr1b  Sr2b   .        .        4       109.8(5)     no
  Ti1   Sr1b  Cr1   '2 665'   .       '2 665'    5.43(11)   no
  Ti1   Sr1b  O1    '2 665'   .       '2 665'   36.06(12)   no
  Ti1   Sr1b  K2    '2 665'   .       '3 545'  113.7(3)     no
  Ti1   Sr1b  Sr2a  '2 665'   .       '3 545'  110.5(4)     no
  Ti1   Sr1b  Sr2b  '2 665'   .       '3 545'  107.6(4)     no
  Ti1   Sr1b  Ti1   '2 665'   .       '3 545'  157.8(4)     no
  Ti1   Sr1b  O11   '2 665'   .       '3 545'  129.6(4)     no
  Ti1   Sr1b  K2    '2 665'   .        3        56.16(16)   no
  Ti1   Sr1b  Sr2a  '2 665'   .        3        56.26(19)   no
  Ti1   Sr1b  Sr2b  '2 665'   .        3        60.8(2)     no
  Ti1   Sr1b  Ti2   '2 665'   .       '3 545'  103.4(3)     no
  Ti1   Sr1b  P2    '2 665'   .        .       109.8(3)     no
  Ti1   Sr1b  O7    '2 665'   .        .        95.7(3)     no
  Ti1   Sr1b  Sr2a  '2 665'   .        4        68.9(2)     no
  Ti1   Sr1b  Sr2b  '2 665'   .        4        57.9(2)     no
  Cr1   Sr1b  O1    '2 665'   .       '2 665'   30.74(15)   no
  Cr1   Sr1b  K2    '2 665'   .       '3 545'  111.5(4)     no
  Cr1   Sr1b  Sr2a  '2 665'   .       '3 545'  107.7(4)     no
  Cr1   Sr1b  Sr2b  '2 665'   .       '3 545'  103.9(4)     no
  Cr1   Sr1b  Ti1   '2 665'   .       '3 545'  152.7(4)     no
  Cr1   Sr1b  O11   '2 665'   .       '3 545'  124.2(4)     no
  Cr1   Sr1b  K2    '2 665'   .        3        53.85(18)   no
  Cr1   Sr1b  Sr2a  '2 665'   .        3        53.4(2)     no
  Cr1   Sr1b  Sr2b  '2 665'   .        3        56.9(2)     no
  Cr1   Sr1b  Ti2   '2 665'   .       '3 545'   98.0(3)     no
  Cr1   Sr1b  P2    '2 665'   .        .       107.2(3)     no
  Cr1   Sr1b  O7    '2 665'   .        .        91.4(3)     no
  Cr1   Sr1b  Sr2a  '2 665'   .        4        74.2(3)     no
  Cr1   Sr1b  Sr2b  '2 665'   .        4        63.1(3)     no
  O1    Sr1b  K2    '2 665'   .       '3 545'  101.9(4)     no
  O1    Sr1b  Sr2a  '2 665'   .       '3 545'   95.7(4)     no
  O1    Sr1b  Sr2b  '2 665'   .       '3 545'   87.0(3)     no
  O1    Sr1b  Ti1   '2 665'   .       '3 545'  122.0(4)     no
  O1    Sr1b  O11   '2 665'   .       '3 545'   94.5(3)     no
  O1    Sr1b  K2    '2 665'   .        3        41.52(13)   no
  O1    Sr1b  Sr2a  '2 665'   .        3        37.93(16)   no
  O1    Sr1b  Sr2b  '2 665'   .        3        33.7(2)     no
  O1    Sr1b  Ti2   '2 665'   .       '3 545'   67.4(2)     no
  O1    Sr1b  P2    '2 665'   .        .        86.1(3)     no
  O1    Sr1b  O7    '2 665'   .        .        64.1(2)     no
  O1    Sr1b  Sr2a  '2 665'   .        4       104.9(3)     no
  O1    Sr1b  Sr2b  '2 665'   .        4        93.8(3)     no
  K2    Sr1b  Sr2a  '3 545'   .       '3 545'   7.05(16)    no
  K2    Sr1b  Sr2b  '3 545'   .       '3 545'  19.00(18)    no
  K2    Sr1b  Ti1   '3 545'   .       '3 545'   67.4(2)     no
  K2    Sr1b  O11   '3 545'   .       '3 545'   53.7(2)     no
  K2    Sr1b  K2    '3 545'   .        3       135.2(4)     no
  K2    Sr1b  Sr2a  '3 545'   .        3       129.9(4)     no
  K2    Sr1b  Sr2b  '3 545'   .        3       117.1(4)     no
  K2    Sr1b  Ti2   '3 545'   .       '3 545'   70.1(3)     no
  K2    Sr1b  P2    '3 545'   .        .       114.0(4)     no
  K2    Sr1b  O7    '3 545'   .        .       101.7(4)     no
  K2    Sr1b  Sr2a  '3 545'   .        4       110.4(3)     no
  K2    Sr1b  Sr2b  '3 545'   .        4       108.8(3)     no
  Sr2a  Sr1b  Sr2b  '3 545'   .       '3 545'   12.2(2)     no
  Sr2a  Sr1b  Ti1   '3 545'   .       '3 545'   67.9(3)     no
  Sr2a  Sr1b  O11   '3 545'   .       '3 545'   50.4(2)     no
  Sr2a  Sr1b  K2    '3 545'   .        3       128.1(4)     no
  Sr2a  Sr1b  Sr2a  '3 545'   .        3       122.9(4)     no
  Sr2a  Sr1b  Sr2b  '3 545'   .        3       110.0(4)     no
  Sr2a  Sr1b  Ti2   '3 545'   .       '3 545'   64.2(3)     no
  Sr2a  Sr1b  P2    '3 545'   .        .       110.7(4)     no
  Sr2a  Sr1b  O7    '3 545'   .        .        96.1(4)     no
  Sr2a  Sr1b  Sr2a  '3 545'   .        4       115.6(3)     no
  Sr2a  Sr1b  Sr2b  '3 545'   .        4       112.8(4)     no
  Sr2b  Sr1b  Ti1   '3 545'   .       '3 545'   65.8(3)     no
  Sr2b  Sr1b  O11   '3 545'   .       '3 545'   42.7(2)     no
  Sr2b  Sr1b  K2    '3 545'   .        3       116.4(3)     no
  Sr2b  Sr1b  Sr2a  '3 545'   .        3       111.1(4)     no
  Sr2b  Sr1b  Sr2b  '3 545'   .        3        98.2(3)     no
  Sr2b  Sr1b  Ti2   '3 545'   .       '3 545'   52.6(2)     no
  Sr2b  Sr1b  P2    '3 545'   .        .       101.6(3)     no
  Sr2b  Sr1b  O7    '3 545'   .        .        84.6(3)     no
  Sr2b  Sr1b  Sr2a  '3 545'   .        4       126.5(3)     no
  Sr2b  Sr1b  Sr2b  '3 545'   .        4       122.0(4)     no
  Ti1   Sr1b  O11   '3 545'   .       '3 545'   31.76(11)   no
  Ti1   Sr1b  K2    '3 545'   .        3       106.3(3)     no
  Ti1   Sr1b  Sr2a  '3 545'   .        3       104.9(3)     no
  Ti1   Sr1b  Sr2b  '3 545'   .        3        98.2(3)     no
  Ti1   Sr1b  Ti2   '3 545'   .       '3 545'   55.24(17)   no
  Ti1   Sr1b  P2    '3 545'   .        .        54.38(17)   no
  Ti1   Sr1b  O7    '3 545'   .        .        63.2(2)     no
  Ti1   Sr1b  Sr2a  '3 545'   .        4       132.7(3)     no
  Ti1   Sr1b  Sr2b  '3 545'   .        4       144.1(4)     no
  O11   Sr1b  K2    '3 545'   .        3        96.6(3)     no
  O11   Sr1b  Sr2a  '3 545'   .        3        92.8(3)     no
  O11   Sr1b  Sr2b  '3 545'   .        3        81.6(3)     no
  O11   Sr1b  Ti2   '3 545'   .       '3 545'   28.32(11)   no
  O11   Sr1b  P2    '3 545'   .        .        60.4(2)     no
  O11   Sr1b  O7    '3 545'   .        .        51.9(2)     no
  O11   Sr1b  Sr2a  '3 545'   .        4       157.8(3)     no
  O11   Sr1b  Sr2b  '3 545'   .        4       162.0(4)     no
  K2    Sr1b  Sr2a   3        .        3         5.24(12)   no
  K2    Sr1b  Sr2b   3        .        3        18.25(14)   no
  K2    Sr1b  Ti2    3        .       '3 545'   71.0(2)     no
  K2    Sr1b  P2     3        .        .        53.66(16)   no
  K2    Sr1b  O7     3        .        .        45.68(15)   no
  K2    Sr1b  Sr2a   3        .        4       105.1(3)     no
  K2    Sr1b  Sr2b   3        .        4       100.3(3)     no
  Sr2a  Sr1b  Sr2b   3        .        3        13.11(18)   no
  Sr2a  Sr1b  Ti2    3        .       '3 545'   66.6(2)     no
  Sr2a  Sr1b  P2     3        .        .        53.84(18)   no
  Sr2a  Sr1b  O7     3        .        .        42.92(17)   no
  Sr2a  Sr1b  Sr2a   3        .        4       109.1(3)     no
  Sr2a  Sr1b  Sr2b   3        .        4       103.5(3)     no
  Sr2b  Sr1b  Ti2    3        .       '3 545'   54.3(2)     no
  Sr2b  Sr1b  P2     3        .        .        52.7(2)     no
  Sr2b  Sr1b  O7     3        .        .        35.0(2)     no
  Sr2b  Sr1b  Sr2a   3        .        4       120.6(3)     no
  Sr2b  Sr1b  Sr2b   3        .        4       113.6(3)     no
  Ti2   Sr1b  P2    '3 545'   .        .        53.04(17)   no
  Ti2   Sr1b  O7    '3 545'   .        .        31.98(12)   no
  Ti2   Sr1b  Sr2a  '3 545'   .        4       171.9(3)     no
  Ti2   Sr1b  Sr2b  '3 545'   .        4       159.8(4)     no
  P2    Sr1b  O7     .        .        .        26.99(10)   no
  P2    Sr1b  Sr2a   .        .        4       130.7(3)     no
  P2    Sr1b  Sr2b   .        .        4       136.3(4)     no
  O7    Sr1b  Sr2a   .        .        4       147.8(3)     no
  O7    Sr1b  Sr2b   .        .        4       145.7(4)     no
  Sr2a  Sr1b  Sr2b   4        .        4        12.1(2)     no
  K1    K2    Sr1a   .        .        .         2.62(10)   no
  K1    K2    Sr2a   .        .        .        55.4(10)    no
  K1    K2    Sr2b   .        .        .        44.8(5)     no
  K1    K2    Ti1    .        .        .        54.240(16)  no
  K1    K2    P2     .        .       '3 544'   52.548(18)  no
  K1    K2    O11    .        .        .        42.48(3)    no
  K1    K2    O7     .        .       '3 544'   44.24(3)    no
  K1    K2    Ti2    .        .        .        53.581(14)  no
  K1    K2    K1     .        .       '3 544'  102.448(18)  no
  K1    K2    Sr1a   .        .       '3 544'  101.47(10)   no
  K1    K2    Sr1b   .        .       '3 544'   94.39(17)   no
  K1    K2    P1     .        .       '3 544'  142.93(2)    no
  K1    K2    O2     .        .       '3 544'  135.67(3)    no
  K1    K2    O8     .        .       '3 544'   78.8(3)     no
  K1    K2    K1     .        .       '3 554'  117.14(2)    no
  K1    K2    Sr1a   .        .       '3 554'  117.71(12)   no
  K1    K2    Sr1b   .        .       '3 554'  111.6(2)     no
  K1    K2    Ti2    .        .       '3 544'   96.14(2)    no
  K1    K2    Cr2    .        .       '3 544'   94.61(7)    no
  K1    K2    O3     .        .       '3 544'  127.84(3)    no
  K1    K2    O4     .        .       '4 465'   77.43(2)    no
  K1    K2    O12    .        .       '3 544'   80.37(3)    no
  K1    K2    K1     .        .       '4 455'  101.37(3)    no
  K1    K2    Sr1a   .        .       '4 455'   95.98(11)   no
  K1    K2    Ti1    .        .       '4 455'  134.99(2)    no
  K1    K2    Cr1    .        .       '4 455'  130.30(10)   no
  K1    K2    O1     .        .       '4 455'   99.89(3)    no
  K1    K2    O5     .        .       '2 564'  148.43(4)    no
  Sr1a  K2    Sr2a   .        .        .        52.8(10)    no
  Sr1a  K2    Sr2b   .        .        .        42.2(5)     no
  Sr1a  K2    Ti1    .        .        .        56.59(9)    no
  Sr1a  K2    P2     .        .       '3 544'   54.48(9)    no
  Sr1a  K2    O11    .        .        .        43.63(8)    no
  Sr1a  K2    O7     .        .       '3 544'   44.86(8)    no
  Sr1a  K2    Ti2    .        .        .        53.39(7)    no
  Sr1a  K2    K1     .        .       '3 544'  103.61(8)    no
  Sr1a  K2    Sr1a   .        .       '3 544'  102.43(12)   no
  Sr1a  K2    Sr1b   .        .       '3 544'   94.87(18)   no
  Sr1a  K2    P1     .        .       '3 544'  144.96(9)    no
  Sr1a  K2    O2     .        .       '3 544'  136.29(8)    no
  Sr1a  K2    O8     .        .       '3 544'   80.9(3)     no
  Sr1a  K2    K1     .        .       '3 554'  119.02(8)    no
  Sr1a  K2    Sr1a   .        .       '3 554'  119.43(14)   no
  Sr1a  K2    Sr1b   .        .       '3 554'  112.8(2)     no
  Sr1a  K2    Ti2    .        .       '3 544'   98.71(10)   no
  Sr1a  K2    Cr2    .        .       '3 544'   97.21(12)   no
  Sr1a  K2    O3     .        .       '3 544'  130.43(10)   no
  Sr1a  K2    O4     .        .       '4 465'   76.26(8)    no
  Sr1a  K2    O12    .        .       '3 544'   82.88(10)   no
  Sr1a  K2    K1     .        .       '4 455'   98.75(10)   no
  Sr1a  K2    Sr1a   .        .       '4 455'   93.36(14)   no
  Sr1a  K2    Ti1    .        .       '4 455'  133.52(8)    no
  Sr1a  K2    Cr1    .        .       '4 455'  128.75(13)   no
  Sr1a  K2    O1     .        .       '4 455'   98.13(9)    no
  Sr1a  K2    O5     .        .       '2 564'  145.82(10)   no
  Sr2a  K2    Sr2b   .        .        .        12.6(11)    no
  Sr2a  K2    Ti1    .        .        .       101.0(10)    no
  Sr2a  K2    P2     .        .       '3 544'  102.3(10)    no
  Sr2a  K2    O11    .        .        .        72.9(10)    no
  Sr2a  K2    O7     .        .       '3 544'   80.0(10)    no
  Sr2a  K2    Ti2    .        .        .        58.0(10)    no
  Sr2a  K2    K1     .        .       '3 544'  128.5(10)    no
  Sr2a  K2    Sr1a   .        .       '3 544'  124.0(10)    no
  Sr2a  K2    Sr1b   .        .       '3 544'  110.9(10)    no
  Sr2a  K2    P1     .        .       '3 544'  153.9(10)    no
  Sr2a  K2    O2     .        .       '3 544'  131.7(10)    no
  Sr2a  K2    O8     .        .       '3 544'  128.4(11)    no
  Sr2a  K2    K1     .        .       '3 554'  132.6(10)    no
  Sr2a  K2    Sr1a   .        .       '3 554'  128.8(10)    no
  Sr2a  K2    Sr1b   .        .       '3 554'  113.9(10)    no
  Sr2a  K2    Ti2    .        .       '3 544'  151.6(10)    no
  Sr2a  K2    Cr2    .        .       '3 544'  149.6(10)    no
  Sr2a  K2    O3     .        .       '3 544'  176.1(10)    no
  Sr2a  K2    O4     .        .       '4 465'   51.3(10)    no
  Sr2a  K2    O12    .        .       '3 544'  128.1(10)    no
  Sr2a  K2    K1     .        .       '4 455'   47.1(10)    no
  Sr2a  K2    Sr1a   .        .       '4 455'   41.5(10)    no
  Sr2a  K2    Ti1    .        .       '4 455'  101.1(10)    no
  Sr2a  K2    Cr1    .        .       '4 455'   96.7(10)    no
  Sr2a  K2    O1     .        .       '4 455'   72.0(10)    no
  Sr2a  K2    O5     .        .       '2 564'   94.0(10)    no
  Sr2b  K2    Ti1    .        .        .        94.7(5)     no
  Sr2b  K2    P2     .        .       '3 544'   89.8(4)     no
  Sr2b  K2    O11    .        .        .        69.7(4)     no
  Sr2b  K2    O7     .        .       '3 544'   67.7(4)     no
  Sr2b  K2    Ti2    .        .        .        59.9(4)     no
  Sr2b  K2    K1     .        .       '3 544'  119.5(3)     no
  Sr2b  K2    Sr1a   .        .       '3 544'  115.5(3)     no
  Sr2b  K2    Sr1b   .        .       '3 544'  102.7(4)     no
  Sr2b  K2    P1     .        .       '3 544'  156.1(4)     no
  Sr2b  K2    O2     .        .       '3 544'  131.2(4)     no
  Sr2b  K2    O8     .        .       '3 544'  115.9(6)     no
  Sr2b  K2    K1     .        .       '3 554'  139.1(3)     no
  Sr2b  K2    Sr1a   .        .       '3 554'  136.0(4)     no
  Sr2b  K2    Sr1b   .        .       '3 554'  121.6(4)     no
  Sr2b  K2    Ti2    .        .       '3 544'  140.3(5)     no
  Sr2b  K2    Cr2    .        .       '3 544'  139.3(5)     no
  Sr2b  K2    O3     .        .       '3 544'  171.4(4)     no
  Sr2b  K2    O4     .        .       '4 465'   60.2(3)     no
  Sr2b  K2    O12    .        .       '3 544'  122.3(5)     no
  Sr2b  K2    K1     .        .       '4 455'   56.6(5)     no
  Sr2b  K2    Sr1a   .        .       '4 455'   51.2(5)     no
  Sr2b  K2    Ti1    .        .       '4 455'  104.7(4)     no
  Sr2b  K2    Cr1    .        .       '4 455'   99.9(5)     no
  Sr2b  K2    O1     .        .       '4 455'   71.7(4)     no
  Sr2b  K2    O5     .        .       '2 564'  103.8(5)     no
  Ti1   K2    P2     .        .       '3 544'   54.746(14)  no
  Ti1   K2    O11    .        .        .        30.79(3)    no
  Ti1   K2    O7     .        .       '3 544'   73.89(3)    no
  Ti1   K2    Ti2    .        .        .        54.117(14)  no
  Ti1   K2    K1     .        .       '3 544'   97.26(2)    no
  Ti1   K2    Sr1a   .        .       '3 544'  100.63(9)    no
  Ti1   K2    Sr1b   .        .       '3 544'  105.52(16)   no
  Ti1   K2    P1     .        .       '3 544'  104.89(2)    no
  Ti1   K2    O2     .        .       '3 544'  122.23(3)    no
  Ti1   K2    O8     .        .       '3 544'   62.07(5)    no
  Ti1   K2    K1     .        .       '3 554'   64.868(17)  no
  Ti1   K2    Sr1a   .        .       '3 554'   66.71(12)   no
  Ti1   K2    Sr1b   .        .       '3 554'   67.1(2)     no
  Ti1   K2    Ti2    .        .       '3 544'   55.025(15)  no
  Ti1   K2    Cr2    .        .       '3 544'   50.70(7)    no
  Ti1   K2    O3     .        .       '3 544'   80.68(3)    no
  Ti1   K2    O4     .        .       '4 465'   82.86(2)    no
  Ti1   K2    O12    .        .       '3 544'   27.57(2)    no
  Ti1   K2    K1     .        .       '4 455'  145.26(3)    no
  Ti1   K2    Sr1a   .        .       '4 455'  140.10(10)   no
  Ti1   K2    Ti1    .        .       '4 455'  155.22(3)    no
  Ti1   K2    Cr1    .        .       '4 455'  157.52(11)   no
  Ti1   K2    O1     .        .       '4 455'  147.62(3)    no
  Ti1   K2    O5     .        .       '2 564'  152.95(4)    no
  P2    K2    O11   '3 544'   .        .        73.84(3)    no
  P2    K2    O7    '3 544'   .       '3 544'   26.92(3)    no
  P2    K2    Ti2   '3 544'   .        .        96.688(18)  no
  P2    K2    K1    '3 544'   .       '3 544'   53.376(16)  no
  P2    K2    Sr1a  '3 544'   .       '3 544'   54.28(9)    no
  P2    K2    Sr1b  '3 544'   .       '3 544'   53.65(16)   no
  P2    K2    P1    '3 544'   .       '3 544'   90.50(2)    no
  P2    K2    O2    '3 544'   .       '3 544'   87.93(3)    no
  P2    K2    O8    '3 544'   .       '3 544'   26.8(3)     no
  P2    K2    K1    '3 544'   .       '3 554'  103.67(2)    no
  P2    K2    Sr1a  '3 544'   .       '3 554'  107.62(12)   no
  P2    K2    Sr1b  '3 544'   .       '3 554'  115.7(2)     no
  P2    K2    Ti2   '3 544'   .       '3 544'   52.745(17)  no
  P2    K2    Cr2   '3 544'   .       '3 544'   54.40(7)    no
  P2    K2    O3    '3 544'   .       '3 544'   81.63(3)    no
  P2    K2    O4    '3 544'   .       '4 465'  126.59(3)    no
  P2    K2    O12   '3 544'   .       '3 544'   60.60(3)    no
  P2    K2    K1    '3 544'   .       '4 455'  133.92(3)    no
  P2    K2    Sr1a  '3 544'   .       '4 455'  131.29(10)   no
  P2    K2    Ti1   '3 544'   .       '4 455'  109.24(2)    no
  P2    K2    Cr1   '3 544'   .       '4 455'  108.04(9)    no
  P2    K2    O1    '3 544'   .       '4 455'   94.98(3)    no
  P2    K2    O5    '3 544'   .       '2 564'  143.05(3)    no
  O11   K2    O7     .        .       '3 544'   81.28(4)    no
  O11   K2    Ti2    .        .        .        24.62(2)    no
  O11   K2    K1     .        .       '3 544'  124.82(3)    no
  O11   K2    Sr1a   .        .       '3 544'  127.07(10)   no
  O11   K2    Sr1b   .        .       '3 544'  127.27(16)   no
  O11   K2    P1     .        .       '3 544'  133.00(4)    no
  O11   K2    O2     .        .       '3 544'  153.01(4)    no
  O11   K2    O8     .        .       '3 544'   89.79(13)   no
  O11   K2    K1     .        .       '3 554'   77.20(3)    no
  O11   K2    Sr1a   .        .       '3 554'   76.75(12)   no
  O11   K2    Sr1b   .        .       '3 554'   69.2(2)     no
  O11   K2    Ti2    .        .       '3 544'   85.63(3)    no
  O11   K2    Cr2    .        .       '3 544'   81.04(7)    no
  O11   K2    O3     .        .       '3 544'  107.96(4)    no
  O11   K2    O4     .        .       '4 465'   55.23(3)    no
  O11   K2    O12    .        .       '3 544'   55.51(4)    no
  O11   K2    K1     .        .       '4 455'  114.50(4)    no
  O11   K2    Sr1a   .        .       '4 455'  109.45(11)   no
  O11   K2    Ti1    .        .       '4 455'  173.80(4)    no
  O11   K2    Cr1    .        .       '4 455'  169.53(12)   no
  O11   K2    O1     .        .       '4 455'  139.66(5)    no
  O11   K2    O5     .        .       '2 564'  143.08(4)    no
  O7    K2    Ti2   '3 544'   .        .        97.58(3)    no
  O7    K2    K1    '3 544'   .       '3 544'   59.64(3)    no
  O7    K2    Sr1a  '3 544'   .       '3 544'   57.86(10)   no
  O7    K2    Sr1b  '3 544'   .       '3 544'   50.17(17)   no
  O7    K2    P1    '3 544'   .       '3 544'  104.39(3)    no
  O7    K2    O2    '3 544'   .       '3 544'   91.46(4)    no
  O7    K2    O8    '3 544'   .       '3 544'   49.0(3)     no
  O7    K2    K1    '3 544'   .       '3 554'  130.46(3)    no
  O7    K2    Sr1a  '3 544'   .       '3 554'  134.27(12)   no
  O7    K2    Sr1b  '3 544'   .       '3 554'  140.3(2)     no
  O7    K2    Ti2   '3 544'   .       '3 544'   78.43(3)    no
  O7    K2    Cr2   '3 544'   .       '3 544'   80.75(7)    no
  O7    K2    O3    '3 544'   .       '3 544'  103.88(4)    no
  O7    K2    O4    '3 544'   .       '4 465'  120.20(4)    no
  O7    K2    O12   '3 544'   .       '3 544'   86.41(4)    no
  O7    K2    K1    '3 544'   .       '4 455'  107.10(3)    no
  O7    K2    Sr1a  '3 544'   .       '4 455'  104.37(10)   no
  O7    K2    Ti1   '3 544'   .       '4 455'   99.10(3)    no
  O7    K2    Cr1   '3 544'   .       '4 455'   95.95(9)    no
  O7    K2    O1    '3 544'   .       '4 455'   73.75(4)    no
  O7    K2    O5    '3 544'   .       '2 564'  131.37(4)    no
  Ti2   K2    K1     .        .       '3 544'  149.238(18)  no
  Ti2   K2    Sr1a   .        .       '3 544'  150.92(9)    no
  Ti2   K2    Sr1b   .        .       '3 544'  147.58(16)   no
  Ti2   K2    P1     .        .       '3 544'  143.66(3)    no
  Ti2   K2    O2     .        .       '3 544'  168.20(4)    no
  Ti2   K2    O8     .        .       '3 544'  114.41(13)   no
  Ti2   K2    K1     .        .       '3 554'   80.03(2)    no
  Ti2   K2    Sr1a   .        .       '3 554'   77.76(12)   no
  Ti2   K2    Sr1b   .        .       '3 554'   65.4(2)     no
  Ti2   K2    Ti2    .        .       '3 544'  106.92(2)    no
  Ti2   K2    Cr2    .        .       '3 544'  101.78(7)    no
  Ti2   K2    O3     .        .       '3 544'  121.34(3)    no
  Ti2   K2    O4     .        .       '4 465'   30.796(17)  no
  Ti2   K2    O12    .        .       '3 544'   74.83(3)    no
  Ti2   K2    K1     .        .       '4 455'   92.08(2)    no
  Ti2   K2    Sr1a   .        .       '4 455'   87.60(10)   no
  Ti2   K2    Ti1    .        .       '4 455'  150.20(2)    no
  Ti2   K2    Cr1    .        .       '4 455'  148.34(11)   no
  Ti2   K2    O1     .        .       '4 455'  129.92(4)    no
  Ti2   K2    O5     .        .       '2 564'  119.94(3)    no
  K1    K2    Sr1a  '3 544'   .       '3 544'   4.89(10)    no
  K1    K2    Sr1b  '3 544'   .       '3 544'  17.71(18)    no
  K1    K2    P1    '3 544'   .       '3 544'   45.269(14)  no
  K1    K2    O2    '3 544'   .       '3 544'   34.68(3)    no
  K1    K2    O8    '3 544'   .       '3 544'   35.38(9)    no
  K1    K2    K1    '3 544'   .       '3 554'   98.83(2)    no
  K1    K2    Sr1a  '3 544'   .       '3 554'  102.75(12)   no
  K1    K2    Sr1b  '3 544'   .       '3 554'  117.6(2)     no
  K1    K2    Ti2   '3 544'   .       '3 544'   51.654(14)  no
  K1    K2    Cr2   '3 544'   .       '3 544'   57.10(6)    no
  K1    K2    O3    '3 544'   .       '3 544'   54.43(2)    no
  K1    K2    O4    '3 544'   .       '4 465'  179.74(7)    no
  K1    K2    O12   '3 544'   .       '3 544'   82.81(3)    no
  K1    K2    K1    '3 544'   .       '4 455'  113.39(2)    no
  K1    K2    Sr1a  '3 544'   .       '4 455'  116.55(9)    no
  K1    K2    Ti1   '3 544'   .       '4 455'   59.821(16)  no
  K1    K2    Cr1   '3 544'   .       '4 455'   60.63(10)   no
  K1    K2    O1    '3 544'   .       '4 455'   67.11(3)    no
  K1    K2    O5    '3 544'   .       '2 564'   90.63(3)    no
  Sr1a  K2    Sr1b  '3 544'   .       '3 544'   13.0(2)     no
  Sr1a  K2    P1    '3 544'   .       '3 544'   48.03(10)   no
  Sr1a  K2    O2    '3 544'   .       '3 544'   34.70(10)   no
  Sr1a  K2    O8    '3 544'   .       '3 544'   38.56(11)   no
  Sr1a  K2    K1    '3 544'   .       '3 554'  103.44(10)   no
  Sr1a  K2    Sr1a  '3 544'   .       '3 554'  107.29(16)   no
  Sr1a  K2    Sr1b  '3 544'   .       '3 554'  122.1(3)     no
  Sr1a  K2    Ti2   '3 544'   .       '3 544'   56.42(10)   no
  Sr1a  K2    Cr2   '3 544'   .       '3 544'   61.86(12)   no
  Sr1a  K2    O3    '3 544'   .       '3 544'   58.82(10)   no
  Sr1a  K2    O4    '3 544'   .       '4 465'  174.86(10)   no
  Sr1a  K2    O12   '3 544'   .       '3 544'   87.32(10)   no
  Sr1a  K2    K1    '3 544'   .       '4 455'  109.11(10)   no
  Sr1a  K2    Sr1a  '3 544'   .       '4 455'  112.08(13)   no
  Sr1a  K2    Ti1   '3 544'   .       '4 455'   57.19(9)    no
  Sr1a  K2    Cr1   '3 544'   .       '4 455'   57.60(13)   no
  Sr1a  K2    O1    '3 544'   .       '4 455'   62.44(10)   no
  Sr1a  K2    O5    '3 544'   .       '2 564'   89.13(10)   no
  Sr1b  K2    P1    '3 544'   .       '3 544'   59.18(18)   no
  Sr1b  K2    O2    '3 544'   .       '3 544'   41.45(17)   no
  Sr1b  K2    O8    '3 544'   .       '3 544'   45.03(18)   no
  Sr1b  K2    K1    '3 544'   .       '3 554'  116.48(18)   no
  Sr1b  K2    Sr1a  '3 544'   .       '3 554'  120.3(2)     no
  Sr1b  K2    Sr1b  '3 544'   .       '3 554'  135.2(3)     no
  Sr1b  K2    Ti2   '3 544'   .       '3 544'   67.68(17)   no
  Sr1b  K2    Cr2   '3 544'   .       '3 544'   73.00(18)   no
  Sr1b  K2    O3    '3 544'   .       '3 544'   71.80(18)   no
  Sr1b  K2    O4    '3 544'   .       '4 465'  162.03(18)   no
  Sr1b  K2    O12   '3 544'   .       '3 544'   96.95(17)   no
  Sr1b  K2    K1    '3 544'   .       '4 455'  100.22(17)   no
  Sr1b  K2    Sr1a  '3 544'   .       '4 455'  102.36(19)   no
  Sr1b  K2    Ti1   '3 544'   .       '4 455'   55.59(16)   no
  Sr1b  K2    Cr1   '3 544'   .       '4 455'   54.65(18)   no
  Sr1b  K2    O1    '3 544'   .       '4 455'   52.41(17)   no
  Sr1b  K2    O5    '3 544'   .       '2 564'   89.60(16)   no
  P1    K2    O2    '3 544'   .       '3 544'   24.93(3)    no
  P1    K2    O8    '3 544'   .       '3 544'   64.1(3)     no
  P1    K2    K1    '3 544'   .       '3 554'   63.67(2)    no
  P1    K2    Sr1a  '3 544'   .       '3 554'   66.15(12)   no
  P1    K2    Sr1b  '3 544'   .       '3 554'   79.4(2)     no
  P1    K2    Ti2   '3 544'   .       '3 544'   51.608(16)  no
  P1    K2    Cr2   '3 544'   .       '3 544'   54.96(7)    no
  P1    K2    O3    '3 544'   .       '3 544'   25.04(2)    no
  P1    K2    O4    '3 544'   .       '4 465'  134.93(3)    no
  P1    K2    O12   '3 544'   .       '3 544'   78.02(3)    no
  P1    K2    K1    '3 544'   .       '4 455'  108.23(2)    no
  P1    K2    Sr1a  '3 544'   .       '4 455'  113.81(11)   no
  P1    K2    Ti1   '3 544'   .       '4 455'   52.988(16)  no
  P1    K2    Cr1   '3 544'   .       '4 455'   57.45(11)   no
  P1    K2    O1    '3 544'   .       '4 455'   84.47(3)    no
  P1    K2    O5    '3 544'   .       '2 564'   63.50(3)    no
  O2    K2    O8    '3 544'   .       '3 544'   66.4(2)     no
  O2    K2    K1    '3 544'   .       '3 554'   88.33(3)    no
  O2    K2    Sr1a  '3 544'   .       '3 554'   90.50(12)   no
  O2    K2    Sr1b  '3 544'   .       '3 554'  102.9(2)     no
  O2    K2    Ti2   '3 544'   .       '3 544'   67.42(3)    no
  O2    K2    Cr2   '3 544'   .       '3 544'   72.12(7)    no
  O2    K2    O3    '3 544'   .       '3 544'   48.48(3)    no
  O2    K2    O4    '3 544'   .       '4 465'  145.38(3)    no
  O2    K2    O12   '3 544'   .       '3 544'   98.31(4)    no
  O2    K2    K1    '3 544'   .       '4 455'   92.49(3)    no
  O2    K2    Sr1a  '3 544'   .       '4 455'   97.53(10)   no
  O2    K2    Ti1   '3 544'   .       '4 455'   33.11(2)    no
  O2    K2    Cr1   '3 544'   .       '4 455'   36.49(11)   no
  O2    K2    O1    '3 544'   .       '4 455'   60.04(4)    no
  O2    K2    O5    '3 544'   .       '2 564'   57.20(3)    no
  O8    K2    K1    '3 544'   .       '3 554'   86.7(3)     no
  O8    K2    Sr1a  '3 544'   .       '3 554'   91.1(3)     no
  O8    K2    Sr1b  '3 544'   .       '3 554'  103.5(4)     no
  O8    K2    Ti2   '3 544'   .       '3 544'   30.8(3)     no
  O8    K2    Cr2   '3 544'   .       '3 544'   34.5(3)     no
  O8    K2    O3    '3 544'   .       '3 544'   55.6(3)     no
  O8    K2    O4    '3 544'   .       '4 465'  144.71(9)    no
  O8    K2    O12   '3 544'   .       '3 544'   52.93(14)   no
  O8    K2    K1    '3 544'   .       '4 455'  144.54(14)   no
  O8    K2    Sr1a  '3 544'   .       '4 455'  145.4(2)     no
  O8    K2    Ti1   '3 544'   .       '4 455'   95.12(11)   no
  O8    K2    Cr1   '3 544'   .       '4 455'   96.00(13)   no
  O8    K2    O1    '3 544'   .       '4 455'   96.79(12)   no
  O8    K2    O5    '3 544'   .       '2 564'  123.5(2)     no
  K1    K2    Sr1a  '3 554'   .       '3 554'    4.43(12)   no
  K1    K2    Sr1b  '3 554'   .       '3 554'   18.9(2)     no
  K1    K2    Ti2   '3 554'   .       '3 544'   56.040(17)  no
  K1    K2    Cr2   '3 554'   .       '3 544'   52.26(6)    no
  K1    K2    O3    '3 554'   .       '3 544'   44.96(2)    no
  K1    K2    O4    '3 554'   .       '4 465'   81.43(3)    no
  K1    K2    O12   '3 554'   .       '3 544'   44.85(3)    no
  K1    K2    K1    '3 554'   .       '4 455'  122.40(2)    no
  K1    K2    Sr1a  '3 554'   .       '4 455'  124.76(9)    no
  K1    K2    Ti1   '3 554'   .       '4 455'  106.81(2)    no
  K1    K2    Cr1   '3 554'   .       '4 455'  111.76(11)   no
  K1    K2    O1    '3 554'   .       '4 455'  142.71(4)    no
  K1    K2    O5    '3 554'   .       '2 564'   88.41(3)    no
  Sr1a  K2    Sr1b  '3 554'   .       '3 554'   14.9(3)     no
  Sr1a  K2    Ti2   '3 554'   .       '3 544'   60.46(12)   no
  Sr1a  K2    Cr2   '3 554'   .       '3 544'   56.65(13)   no
  Sr1a  K2    O3    '3 554'   .       '3 544'   48.59(12)   no
  Sr1a  K2    O4    '3 554'   .       '4 465'   77.50(12)   no
  Sr1a  K2    O12   '3 554'   .       '3 544'   48.17(12)   no
  Sr1a  K2    K1    '3 554'   .       '4 455'  118.45(12)   no
  Sr1a  K2    Sr1a  '3 554'   .       '4 455'  120.62(15)   no
  Sr1a  K2    Ti1   '3 554'   .       '4 455'  106.87(12)   no
  Sr1a  K2    Cr1   '3 554'   .       '4 455'  111.74(16)   no
  Sr1a  K2    O1    '3 554'   .       '4 455'  142.40(12)   no
  Sr1a  K2    O5    '3 554'   .       '2 564'   86.34(12)   no
  Sr1b  K2    Ti2   '3 554'   .       '3 544'   73.5(2)     no
  Sr1b  K2    Cr2   '3 554'   .       '3 544'   69.2(2)     no
  Sr1b  K2    O3    '3 554'   .       '3 544'   63.4(2)     no
  Sr1b  K2    O4    '3 554'   .       '4 465'   62.6(2)     no
  Sr1b  K2    O12   '3 554'   .       '3 544'   55.2(2)     no
  Sr1b  K2    K1    '3 554'   .       '4 455'  109.0(2)     no
  Sr1b  K2    Sr1a  '3 554'   .       '4 455'  110.1(2)     no
  Sr1b  K2    Ti1   '3 554'   .       '4 455'  113.2(2)     no
  Sr1b  K2    Cr1   '3 554'   .       '4 455'  117.6(2)     no
  Sr1b  K2    O1    '3 554'   .       '4 455'  145.1(2)     no
  Sr1b  K2    O5    '3 554'   .       '2 564'   86.3(2)     no
  Ti2   K2    Cr2   '3 544'   .       '3 544'   5.47(6)     no
  Ti2   K2    O3    '3 544'   .       '3 544'   31.768(19)  no
  Ti2   K2    O4    '3 544'   .       '4 465'  128.57(3)    no
  Ti2   K2    O12   '3 544'   .       '3 544'   32.33(3)    no
  Ti2   K2    K1    '3 544'   .       '4 455'  159.53(2)    no
  Ti2   K2    Sr1a  '3 544'   .       '4 455'  164.87(10)   no
  Ti2   K2    Ti1   '3 544'   .       '4 455'  100.52(2)    no
  Ti2   K2    Cr1   '3 544'   .       '4 455'  103.78(11)   no
  Ti2   K2    O1    '3 544'   .       '4 455'  118.67(3)    no
  Ti2   K2    O5    '3 544'   .       '2 564'  114.21(4)    no
  Cr2   K2    O3    '3 544'   .       '3 544'   33.34(7)    no
  Cr2   K2    O4    '3 544'   .       '4 465'  123.12(7)    no
  Cr2   K2    O12   '3 544'   .       '3 544'  27.03(7)     no
  Cr2   K2    K1    '3 544'   .       '4 455'  163.15(7)    no
  Cr2   K2    Sr1a  '3 544'   .       '4 455'  168.76(13)   no
  Cr2   K2    Ti1   '3 544'   .       '4 455'  105.14(7)    no
  Cr2   K2    Cr1   '3 544'   .       '4 455'  108.59(13)   no
  Cr2   K2    O1    '3 544'   .       '4 455'  124.13(7)    no
  Cr2   K2    O5    '3 544'   .       '2 564'  116.42(8)    no
  O3    K2    O4    '3 544'   .       '4 465'  125.83(3)    no
  O3    K2    O12   '3 544'   .       '3 544'   53.34(3)    no
  O3    K2    K1    '3 544'   .       '4 455'  130.18(3)    no
  O3    K2    Sr1a  '3 544'   .       '4 455'  135.73(11)   no
  O3    K2    Ti1   '3 544'   .       '4 455'   78.01(3)    no
  O3    K2    Cr1   '3 544'   .       '4 455'   82.50(11)   no
  O3    K2    O1    '3 544'   .       '4 455'  108.49(4)    no
  O3    K2    O5    '3 544'   .       '2 564'   83.09(3)    no
  O4    K2    O12   '4 465'   .       '3 544'   97.39(3)    no
  O4    K2    K1    '4 465'   .       '4 455'   66.43(2)    no
  O4    K2    Sr1a  '4 465'   .       '4 455'   63.26(9)    no
  O4    K2    Ti1   '4 465'   .       '4 455'  120.10(2)    no
  O4    K2    Cr1   '4 465'   .       '4 455'  119.27(10)   no
  O4    K2    O1    '4 465'   .       '4 455'  112.67(4)    no
  O4    K2    O5    '4 465'   .       '2 564'   89.37(3)    no
  O12   K2    K1    '3 544'   .       '4 455'  162.53(3)    no
  O12   K2    Sr1a  '3 544'   .       '4 455'  160.58(9)    no
  O12   K2    Ti1   '3 544'   .       '4 455'  130.65(4)    no
  O12   K2    Cr1   '3 544'   .       '4 455'  134.64(12)   no
  O12   K2    O1    '3 544'   .       '4 455'  149.36(4)    no
  O12   K2    O5    '3 544'   .       '2 564'  130.24(4)    no
  K1    K2    Sr1a  '4 455'   .       '4 455'   5.61(11)    no
  K1    K2    Ti1   '4 455'   .       '4 455'   59.416(18)  no
  K1    K2    Cr1   '4 455'   .       '4 455'   56.52(11)   no
  K1    K2    O1    '4 455'   .       '4 455'   47.92(3)    no
  K1    K2    O5    '4 455'   .       '2 564'   47.22(3)    no
  Sr1a  K2    Ti1   '4 455'   .       '4 455'   64.41(10)   no
  Sr1a  K2    Cr1   '4 455'   .       '4 455'   61.30(15)   no
  Sr1a  K2    O1    '4 455'   .       '4 455'   49.99(9)    no
  Sr1a  K2    O5    '4 455'   .       '2 564'   52.70(11)   no
  Ti1   K2    Cr1   '4 455'   .       '4 455'    5.00(11)   no
  Ti1   K2    O1    '4 455'   .       '4 455'   35.95(3)    no
  Ti1   K2    O5    '4 455'   .       '2 564'   34.32(2)    no
  Cr1   K2    O1    '4 455'   .       '4 455'   30.98(11)   no
  Cr1   K2    O5    '4 455'   .       '2 564'   36.39(9)    no
  O1    K2    O5    '4 455'   .       '2 564'   58.78(4)    no
  K1    Sr2a  Sr1a   .        .        .         3.12(10)   no
  K1    Sr2a  K2     .        .        .       119.9(11)    no
  K1    Sr2a  Sr2b   .        .        .        45.6(7)     no
  K1    Sr2a  Ti1    .        .        .        55.67(10)   no
  K1    Sr2a  P2     .        .       '3 544'   54.39(10)   no
  K1    Sr2a  O11    .        .        .        45.88(12)   no
  K1    Sr2a  O7     .        .       '3 544'   47.44(12)   no
  K1    Sr2a  Ti2    .        .        .        56.77(11)   no
  K1    Sr2a  Sr1a   .        .       '3 544'  100.95(17)   no
  K1    Sr2a  Sr1b   .        .       '3 544'   95.3(2)     no
  K1    Sr2a  K1     .        .       '3 554'  115.73(17)   no
  K1    Sr2a  Sr1a   .        .       '3 554'  116.8(2)     no
  K1    Sr2a  Sr1b   .        .       '3 554'  113.2(3)     no
  K1    Sr2a  O4     .        .       '4 465'   83.69(18)   no
  K1    Sr2a  K1     .        .       '4 455'  110.6(2)     no
  K1    Sr2a  Sr1a   .        .       '4 455'  104.6(2)     no
  K1    Sr2a  Sr1b   .        .       '4 455'   94.7(2)     no
  K1    Sr2a  Ti1    .        .       '4 455'  139.5(2)     no
  K1    Sr2a  Cr1    .        .       '4 455'  135.6(2)     no
  K1    Sr2a  O1     .        .       '4 455'  107.4(2)     no
  K1    Sr2a  O5     .        .       '2 564'  160.7(3)     no
  Sr1a  Sr2a  K2     .        .        .       123.0(11)    no
  Sr1a  Sr2a  Sr2b   .        .        .        42.5(8)     no
  Sr1a  Sr2a  Ti1    .        .        .        58.48(14)   no
  Sr1a  Sr2a  P2     .        .       '3 544'   56.81(14)   no
  Sr1a  Sr2a  O11    .        .        .        47.44(15)   no
  Sr1a  Sr2a  O7     .        .       '3 544'   48.48(14)   no
  Sr1a  Sr2a  Ti2    .        .        .        56.64(13)   no
  Sr1a  Sr2a  Sr1a   .        .       '3 544'  102.38(19)   no
  Sr1a  Sr2a  Sr1b   .        .       '3 544'   96.2(2)     no
  Sr1a  Sr2a  K1     .        .       '3 554'  118.15(19)   no
  Sr1a  Sr2a  Sr1a   .        .       '3 554'  119.1(2)     no
  Sr1a  Sr2a  Sr1b   .        .       '3 554'  114.9(3)     no
  Sr1a  Sr2a  O4     .        .       '4 465'   82.5(2)     no
  Sr1a  Sr2a  K1     .        .       '4 455'  107.5(2)     no
  Sr1a  Sr2a  Sr1a   .        .       '4 455'  101.5(2)     no
  Sr1a  Sr2a  Sr1b   .        .       '4 455'   91.6(2)     no
  Sr1a  Sr2a  Ti1    .        .       '4 455'  138.4(2)     no
  Sr1a  Sr2a  Cr1    .        .       '4 455'  134.3(2)     no
  Sr1a  Sr2a  O1     .        .       '4 455'  105.7(2)     no
  Sr1a  Sr2a  O5     .        .       '2 564'  157.7(3)     no
  K2    Sr2a  Sr2b   .        .        .       162.7(15)    no
  K2    Sr2a  Ti1    .        .        .        72.9(10)    no
  K2    Sr2a  P2     .        .       '3 544'   71.2(10)    no
  K2    Sr2a  O11    .        .        .        98.7(11)    no
  K2    Sr2a  O7     .        .       '3 544'   91.8(10)    no
  K2    Sr2a  Ti2    .        .        .       116.5(11)    no
  K2    Sr2a  Sr1a   .        .       '3 544'   51.9(9)     no
  K2    Sr2a  Sr1b   .        .       '3 544'   63.8(10)    no
  K2    Sr2a  K1     .        .       '3 554'   43.2(9)     no
  K2    Sr2a  Sr1a   .        .       '3 554'   46.4(9)     no
  K2    Sr2a  Sr1b   .        .       '3 554'   59.0(10)    no
  K2    Sr2a  O4     .        .       '4 465'  122.3(11)    no
  K2    Sr2a  K1     .        .       '4 455'  128.1(11)    no
  K2    Sr2a  Sr1a   .        .       '4 455'  134.3(11)    no
  K2    Sr2a  Sr1b   .        .       '4 455'  144.5(11)    no
  K2    Sr2a  Ti1    .        .       '4 455'   72.7(10)    no
  K2    Sr2a  Cr1    .        .       '4 455'   76.6(10)    no
  K2    Sr2a  O1     .        .       '4 455'   99.3(10)    no
  K2    Sr2a  O5     .        .       '2 564'   77.8(10)    no
  Sr2b  Sr2a  Ti1    .        .        .        98.1(8)     no
  Sr2b  Sr2a  P2     .        .       '3 544'   91.6(7)     no
  Sr2b  Sr2a  O11    .        .        .        76.8(7)     no
  Sr2b  Sr2a  O7     .        .       '3 544'   71.2(7)     no
  Sr2b  Sr2a  Ti2    .        .        .        66.2(6)     no
  Sr2b  Sr2a  Sr1a   .        .       '3 544'  116.1(6)     no
  Sr2b  Sr2a  Sr1b   .        .       '3 544'  104.6(6)     no
  Sr2b  Sr2a  K1     .        .       '3 554'  144.8(7)     no
  Sr2b  Sr2a  Sr1a   .        .       '3 554'  142.8(7)     no
  Sr2b  Sr2a  Sr1b   .        .       '3 554'  131.0(7)     no
  Sr2b  Sr2a  O4     .        .       '4 465'   70.0(6)     no
  Sr2b  Sr2a  K1     .        .       '4 455'   65.0(8)     no
  Sr2b  Sr2a  Sr1a   .        .       '4 455'   59.1(8)     no
  Sr2b  Sr2a  Sr1b   .        .       '4 455'   49.2(8)     no
  Sr2b  Sr2a  Ti1    .        .       '4 455'  111.8(7)     no
  Sr2b  Sr2a  Cr1    .        .       '4 455'  107.4(7)     no
  Sr2b  Sr2a  O1     .        .       '4 455'   80.1(7)     no
  Sr2b  Sr2a  O5     .        .       '2 564'  115.5(8)     no
  Ti1   Sr2a  P2     .        .       '3 544'   53.06(10)   no
  Ti1   Sr2a  O11    .        .        .        28.61(9)    no
  Ti1   Sr2a  O7     .        .       '3 544'   72.69(16)   no
  Ti1   Sr2a  Ti2    .        .        .        54.89(10)   no
  Ti1   Sr2a  Sr1a   .        .       '3 544'   95.01(18)   no
  Ti1   Sr2a  Sr1b   .        .       '3 544'  100.6(2)     no
  Ti1   Sr2a  K1     .        .       '3 554'   61.21(12)   no
  Ti1   Sr2a  Sr1a   .        .       '3 554'   63.13(16)   no
  Ti1   Sr2a  Sr1b   .        .       '3 554'   64.1(2)     no
  Ti1   Sr2a  O4     .        .       '4 465'   84.25(17)   no
  Ti1   Sr2a  K1     .        .       '4 455'  154.7(2)     no
  Ti1   Sr2a  Sr1a   .        .       '4 455'  149.4(3)     no
  Ti1   Sr2a  Sr1b   .        .       '4 455'  140.4(3)     no
  Ti1   Sr2a  Ti1    .        .       '4 455'  143.8(2)     no
  Ti1   Sr2a  Cr1    .        .       '4 455'  146.6(3)     no
  Ti1   Sr2a  O1     .        .       '4 455'  147.3(3)     no
  Ti1   Sr2a  O5     .        .       '2 564'  143.1(3)     no
  P2    Sr2a  O11   '3 544'   .        .        72.96(17)   no
  P2    Sr2a  O7    '3 544'   .       '3 544'   25.54(7)    no
  P2    Sr2a  Ti2   '3 544'   .        .        98.52(18)   no
  P2    Sr2a  Sr1a  '3 544'   .       '3 544'   51.21(13)   no
  P2    Sr2a  Sr1b  '3 544'   .       '3 544'   51.44(18)   no
  P2    Sr2a  K1    '3 544'   .       '3 554'   96.14(18)   no
  P2    Sr2a  Sr1a  '3 544'   .       '3 554'   99.7(2)     no
  P2    Sr2a  Sr1b  '3 544'   .       '3 554'  107.9(3)     no
  P2    Sr2a  O4    '3 544'   .       '4 465'  131.2(2)     no
  P2    Sr2a  K1    '3 544'   .       '4 455'  140.4(2)     no
  P2    Sr2a  Sr1a  '3 544'   .       '4 455'  138.5(2)     no
  P2    Sr2a  Sr1b  '3 544'   .       '4 455'  133.5(3)     no
  P2    Sr2a  Ti1   '3 544'   .       '4 455'  104.65(19)   no
  P2    Sr2a  Cr1   '3 544'   .       '4 455'  104.0(2)     no
  P2    Sr2a  O1    '3 544'   .       '4 455'   94.2(2)     no
  P2    Sr2a  O5    '3 544'   .       '2 564'  134.7(3)     no
  O11   Sr2a  O7     .        .       '3 544'   83.7(2)     no
  O11   Sr2a  Ti2    .        .        .        27.24(8)    no
  O11   Sr2a  Sr1a   .        .       '3 544'  121.5(2)     no
  O11   Sr2a  Sr1b   .        .       '3 544'  124.3(3)     no
  O11   Sr2a  K1     .        .       '3 554'   72.85(17)   no
  O11   Sr2a  Sr1a   .        .       '3 554'   72.9(2)     no
  O11   Sr2a  Sr1b   .        .       '3 554'   67.4(3)     no
  O11   Sr2a  O4     .        .       '4 465'   59.14(15)   no
  O11   Sr2a  K1     .        .       '4 455'  126.2(3)     no
  O11   Sr2a  Sr1a   .        .       '4 455'  120.8(3)     no
  O11   Sr2a  Sr1b   .        .       '4 455'  112.2(3)     no
  O11   Sr2a  Ti1    .        .       '4 455'  171.3(3)     no
  O11   Sr2a  Cr1    .        .       '4 455'  175.1(3)     no
  O11   Sr2a  O1     .        .       '4 455'  153.1(3)     no
  O11   Sr2a  O5     .        .       '2 564'  145.2(3)     no
  O7    Sr2a  Ti2   '3 544'   .        .       103.0(2)     no
  O7    Sr2a  Sr1a  '3 544'   .       '3 544'   54.19(15)   no
  O7    Sr2a  Sr1b  '3 544'   .       '3 544'   47.9(2)     no
  O7    Sr2a  K1    '3 544'   .       '3 554'  121.7(2)     no
  O7    Sr2a  Sr1a  '3 544'   .       '3 554'  125.3(3)     no
  O7    Sr2a  Sr1b  '3 544'   .       '3 554'  133.0(4)     no
  O7    Sr2a  O4    '3 544'   .       '4 465'  130.9(3)     no
  O7    Sr2a  K1    '3 544'   .       '4 455'  115.4(2)     no
  O7    Sr2a  Sr1a  '3 544'   .       '4 455'  113.0(3)     no
  O7    Sr2a  Sr1b  '3 544'   .       '4 455'  108.1(3)     no
  O7    Sr2a  Ti1   '3 544'   .       '4 455'   97.6(2)     no
  O7    Sr2a  Cr1   '3 544'   .       '4 455'   95.2(2)     no
  O7    Sr2a  O1    '3 544'   .       '4 455'   75.91(19)   no
  O7    Sr2a  O5    '3 544'   .       '2 564'  130.7(3)     no
  Ti2   Sr2a  Sr1a   .        .       '3 544'  148.7(2)     no
  Ti2   Sr2a  Sr1b   .        .       '3 544'  149.4(3)     no
  Ti2   Sr2a  K1     .        .       '3 554'   78.71(14)   no
  Ti2   Sr2a  Sr1a   .        .       '3 554'   77.03(18)   no
  Ti2   Sr2a  Sr1b   .        .       '3 554'   66.7(3)     no
  Ti2   Sr2a  O4     .        .       '4 465'   32.69(8)    no
  Ti2   Sr2a  K1     .        .       '4 455'  100.0(2)     no
  Ti2   Sr2a  Sr1a   .        .       '4 455'   95.3(2)     no
  Ti2   Sr2a  Sr1b   .        .       '4 455'   87.9(2)     no
  Ti2   Sr2a  Ti1    .        .       '4 455'  156.8(2)     no
  Ti2   Sr2a  Cr1    .        .       '4 455'  156.8(3)     no
  Ti2   Sr2a  O1     .        .       '4 455'  144.1(3)     no
  Ti2   Sr2a  O5     .        .       '2 564'  124.9(2)     no
  Sr1a  Sr2a  Sr1b  '3 544'   .       '3 544'  12.0(2)      no
  Sr1a  Sr2a  K1    '3 544'   .       '3 554'   95.02(19)   no
  Sr1a  Sr2a  Sr1a  '3 544'   .       '3 554'   98.2(2)     no
  Sr1a  Sr2a  Sr1b  '3 544'   .       '3 554'  110.9(3)     no
  Sr1a  Sr2a  O4    '3 544'   .       '4 465'  173.9(3)     no
  Sr1a  Sr2a  K1    '3 544'   .       '4 455'  109.14(19)   no
  Sr1a  Sr2a  Sr1a  '3 544'   .       '4 455'  112.8(2)     no
  Sr1a  Sr2a  Sr1b  '3 544'   .       '4 455'  118.0(2)     no
  Sr1a  Sr2a  Ti1   '3 544'   .       '4 455'   54.23(13)   no
  Sr1a  Sr2a  Cr1   '3 544'   .       '4 455'   54.55(17)   no
  Sr1a  Sr2a  O1    '3 544'   .       '4 455'   58.32(17)   no
  Sr1a  Sr2a  O5    '3 544'   .       '2 564'   83.7(2)     no
  Sr1b  Sr2a  K1    '3 544'   .       '3 554'  107.0(3)     no
  Sr1b  Sr2a  Sr1a  '3 544'   .       '3 554'  110.2(3)     no
  Sr1b  Sr2a  Sr1b  '3 544'   .       '3 554'  122.9(4)     no
  Sr1b  Sr2a  O4    '3 544'   .       '4 465'  173.3(3)     no
  Sr1b  Sr2a  K1    '3 544'   .       '4 455'  101.8(2)     no
  Sr1b  Sr2a  Sr1a  '3 544'   .       '4 455'  104.6(2)     no
  Sr1b  Sr2a  Sr1b  '3 544'   .       '4 455'  108.4(3)     no
  Sr1b  Sr2a  Ti1   '3 544'   .       '4 455'   53.46(18)   no
  Sr1b  Sr2a  Cr1   '3 544'   .       '4 455'   52.6(2)     no
  Sr1b  Sr2a  O1    '3 544'   .       '4 455'   49.7(2)     no
  Sr1b  Sr2a  O5    '3 544'   .       '2 564'   85.6(2)     no
  K1    Sr2a  Sr1a  '3 554'   .       '3 554'   3.80(11)    no
  K1    Sr2a  Sr1b  '3 554'   .       '3 554'   16.1(2)     no
  K1    Sr2a  O4    '3 554'   .       '4 465'   79.27(16)   no
  K1    Sr2a  K1    '3 554'   .       '4 455'  121.70(19)   no
  K1    Sr2a  Sr1a  '3 554'   .       '4 455'  125.0(2)     no
  K1    Sr2a  Sr1b  '3 554'   .       '4 455'  130.1(2)     no
  K1    Sr2a  Ti1   '3 554'   .       '4 455'   99.33(18)   no
  K1    Sr2a  Cr1   '3 554'   .       '4 455'  103.9(2)     no
  K1    Sr2a  O1    '3 554'   .       '4 455'  133.1(3)     no
  K1    Sr2a  O5    '3 554'   .       '2 564'   82.13(18)   no
  Sr1a  Sr2a  Sr1b  '3 554'   .       '3 554'   12.7(3)     no
  Sr1a  Sr2a  O4    '3 554'   .       '4 465'   76.0(2)     no
  Sr1a  Sr2a  K1    '3 554'   .       '4 455'  118.4(2)     no
  Sr1a  Sr2a  Sr1a  '3 554'   .       '4 455'  121.5(2)     no
  Sr1a  Sr2a  Sr1b  '3 554'   .       '4 455'  126.4(3)     no
  Sr1a  Sr2a  Ti1   '3 554'   .       '4 455'   99.5(2)     no
  Sr1a  Sr2a  Cr1   '3 554'   .       '4 455'  104.1(2)     no
  Sr1a  Sr2a  O1    '3 554'   .       '4 455'  133.5(3)     no
  Sr1a  Sr2a  O5    '3 554'   .       '2 564'   80.5(2)     no
  Sr1b  Sr2a  O4    '3 554'   .       '4 465'   63.3(3)     no
  Sr1b  Sr2a  K1    '3 554'   .       '4 455'  111.6(3)     no
  Sr1b  Sr2a  Sr1a  '3 554'   .       '4 455'  113.6(3)     no
  Sr1b  Sr2a  Sr1b  '3 554'   .       '4 455'  116.7(3)     no
  Sr1b  Sr2a  Ti1   '3 554'   .       '4 455'  106.1(3)     no
  Sr1b  Sr2a  Cr1   '3 554'   .       '4 455'  110.5(3)     no
  Sr1b  Sr2a  O1    '3 554'   .       '4 455'  139.4(4)     no
  Sr1b  Sr2a  O5    '3 554'   .       '2 564'   81.8(3)     no
  O4    Sr2a  K1    '4 465'   .       '4 455'   72.53(17)   no
  O4    Sr2a  Sr1a  '4 465'   .       '4 455'   69.38(19)   no
  O4    Sr2a  Sr1b  '4 465'   .       '4 455'   65.2(2)     no
  O4    Sr2a  Ti1   '4 465'   .       '4 455'  124.1(2)     no
  O4    Sr2a  Cr1   '4 465'   .       '4 455'  124.4(3)     no
  O4    Sr2a  O1    '4 465'   .       '4 455'  124.3(3)     no
  O4    Sr2a  O5    '4 465'   .       '2 564'   93.2(2)     no
  K1    Sr2a  Sr1a  '4 455'   .       '4 455'    6.21(12)   no
  K1    Sr2a  Sr1b  '4 455'   .       '4 455'   16.42(16)   no
  K1    Sr2a  Ti1   '4 455'   .       '4 455'   61.05(12)   no
  K1    Sr2a  Cr1   '4 455'   .       '4 455'   58.62(16)   no
  K1    Sr2a  O1    '4 455'   .       '4 455'   52.26(14)   no
  K1    Sr2a  O5    '4 455'   .       '2 564'   50.72(12)   no
  Sr1a  Sr2a  Sr1b  '4 455'   .       '4 455'   10.2(2)     no
  Sr1a  Sr2a  Ti1   '4 455'   .       '4 455'   66.65(17)   no
  Sr1a  Sr2a  Cr1   '4 455'   .       '4 455'   64.0(2)     no
  Sr1a  Sr2a  O1    '4 455'   .       '4 455'   54.98(17)   no
  Sr1a  Sr2a  O5    '4 455'   .       '2 564'   56.80(18)   no
  Sr1b  Sr2a  Ti1   '4 455'   .       '4 455'   75.7(2)     no
  Sr1b  Sr2a  Cr1   '4 455'   .       '4 455'   72.7(2)     no
  Sr1b  Sr2a  O1    '4 455'   .       '4 455'   59.7(2)     no
  Sr1b  Sr2a  O5    '4 455'   .       '2 564'   66.9(2)     no
  Ti1   Sr2a  Cr1   '4 455'   .       '4 455'    4.60(10)   no
  Ti1   Sr2a  O1    '4 455'   .       '4 455'   34.01(10)   no
  Ti1   Sr2a  O5    '4 455'   .       '2 564'   33.13(8)    no
  Cr1   Sr2a  O1    '4 455'   .       '4 455'   29.46(13)   no
  Cr1   Sr2a  O5    '4 455'   .       '2 564'   35.53(12)   no
  O1    Sr2a  O5    '4 455'   .       '2 564'   59.04(16)   no
  K1    Sr2b  Sr1a   .        .        .         4.77(13)   no
  K1    Sr2b  Sr1b   .        .        .        16.90(17)   no
  K1    Sr2b  K2     .        .        .       117.8(6)     no
  K1    Sr2b  Sr2a   .        .        .       121.7(9)     no
  K1    Sr2b  Cr2    .        .       '1 545'   55.11(18)   no
  K1    Sr2b  O11    .        .        .        56.4(2)     no
  K1    Sr2b  O12    .        .       '1 545'   48.09(17)   no
  K1    Sr2b  O7     .        .       '3 544'   57.6(2)     no
  K1    Sr2b  O8     .        .        .        48.71(19)   no
  K1    Sr2b  Ti2    .        .        .        66.1(2)     no
  K1    Sr2b  Sr1b   .        .       '3 544'   98.8(3)     no
  K1    Sr2b  Ti1    .        .       '3 545'   69.2(2)     no
  K1    Sr2b  Sr1a   .        .       '3 554'  110.9(3)     no
  K1    Sr2b  Sr1b   .        .       '3 554'  111.0(3)     no
  K1    Sr2b  O4     .        .       '4 465'  100.5(3)     no
  K1    Sr2b  K1     .        .       '4 455'  140.3(4)     no
  K1    Sr2b  Sr1a   .        .       '4 455'  133.4(4)     no
  K1    Sr2b  Sr1b   .        .       '4 455'  119.5(4)     no
  K1    Sr2b  P1     .        .       '4 455'  107.4(3)     no
  K1    Sr2b  O1     .        .       '4 455'  128.2(3)     no
  K1    Sr2b  O2     .        .       '4 455'   99.6(3)     no
  K1    Sr2b  O6     .        .        .        74.0(3)     no
  Sr1a  Sr2b  Sr1b   .        .        .        12.1(2)     no
  Sr1a  Sr2b  K2     .        .        .       122.6(6)     no
  Sr1a  Sr2b  Sr2a   .        .        .       126.5(9)     no
  Sr1a  Sr2b  Cr2    .        .       '1 545'   54.5(2)     no
  Sr1a  Sr2b  O11    .        .        .        59.6(3)     no
  Sr1a  Sr2b  O12    .        .       '1 545'   44.9(2)     no
  Sr1a  Sr2b  O7     .        .       '3 544'   60.0(3)     no
  Sr1a  Sr2b  O8     .        .        .        46.4(2)     no
  Sr1a  Sr2b  Ti2    .        .        .        66.7(2)     no
  Sr1a  Sr2b  Sr1b   .        .       '3 544'  101.0(3)     no
  Sr1a  Sr2b  Ti1    .        .       '3 545'   64.9(2)     no
  Sr1a  Sr2b  Sr1a   .        .       '3 554'  114.9(3)     no
  Sr1a  Sr2b  Sr1b   .        .       '3 554'  114.5(3)     no
  Sr1a  Sr2b  O4     .        .       '4 465'  100.0(3)     no
  Sr1a  Sr2b  K1     .        .       '4 455'  135.6(4)     no
  Sr1a  Sr2b  Sr1a   .        .       '4 455'  128.6(4)     no
  Sr1a  Sr2b  Sr1b   .        .       '4 455'  114.7(4)     no
  Sr1a  Sr2b  P1     .        .       '4 455'  105.3(3)     no
  Sr1a  Sr2b  O1     .        .       '4 455'  127.6(3)     no
  Sr1a  Sr2b  O2     .        .       '4 455'   95.8(3)     no
  Sr1a  Sr2b  O6     .        .        .        69.3(3)     no
  Sr1b  Sr2b  K2     .        .        .       134.7(6)     no
  Sr1b  Sr2b  Sr2a   .        .        .       138.5(9)     no
  Sr1b  Sr2b  Cr2    .        .       '1 545'   55.2(2)     no
  Sr1b  Sr2b  O11    .        .        .        67.5(3)     no
  Sr1b  Sr2b  O12    .        .       '1 545'   38.9(2)     no
  Sr1b  Sr2b  O7     .        .       '3 544'   67.5(3)     no
  Sr1b  Sr2b  O8     .        .        .        41.0(2)    no
  Sr1b  Sr2b  Ti2    .        .        .        68.0(3)     no
  Sr1b  Sr2b  Sr1b   .        .       '3 544'  107.2(3)     no
  Sr1b  Sr2b  Ti1    .        .       '3 545'   54.5(2)     no
  Sr1b  Sr2b  Sr1a   .        .       '3 554'  124.4(3)     no
  Sr1b  Sr2b  Sr1b   .        .       '3 554'  122.6(4)     no
  Sr1b  Sr2b  O4     .        .       '4 465'   97.6(3)     no
  Sr1b  Sr2b  K1     .        .       '4 455'  123.5(3)     no
  Sr1b  Sr2b  Sr1a   .        .       '4 455'  116.5(4)     no
  Sr1b  Sr2b  Sr1b   .        .       '4 455'  102.6(3)     no
  Sr1b  Sr2b  P1     .        .       '4 455'  100.5(3)     no
  Sr1b  Sr2b  O1     .        .       '4 455'  125.4(3)     no
  Sr1b  Sr2b  O2     .        .       '4 455'   86.6(3)     no
  Sr1b  Sr2b  O6     .        .        .        57.2(3)     no
  K2    Sr2b  Sr2a   .        .        .         4.8(4)     no
  K2    Sr2b  Cr2    .        .       '1 545'  110.7(5)     no
  K2    Sr2b  O11    .        .        .        78.7(4)     no
  K2    Sr2b  O12    .        .       '1 545'  137.9(5)     no
  K2    Sr2b  O7     .        .       '3 544'   82.1(4)     no
  K2    Sr2b  O8     .        .        .       132.3(6)     no
  K2    Sr2b  Ti2    .        .        .        97.8(4)     no
  K2    Sr2b  Sr1b   .        .       '3 544'   59.0(3)     no
  K2    Sr2b  Ti1    .        .       '3 545'  155.1(5)     no
  K2    Sr2b  Sr1a   .        .       '3 554'   31.4(3)     no
  K2    Sr2b  Sr1b   .        .       '3 554'   39.4(3)     no
  K2    Sr2b  O4     .        .       '4 465'   91.6(4)     no
  K2    Sr2b  K1     .        .       '4 455'  101.7(6)     no
  K2    Sr2b  Sr1a   .        .       '4 455'  108.7(6)     no
  K2    Sr2b  Sr1b   .        .       '4 455'  122.6(6)     no
  K2    Sr2b  P1     .        .       '4 455'  101.1(5)     no
  K2    Sr2b  O1     .        .       '4 455'   76.1(4)     no
  K2    Sr2b  O2     .        .       '4 455'  126.6(6)     no
  K2    Sr2b  O6     .        .        .       165.7(6)     no
  Sr2a  Sr2b  Cr2    .        .       '1 545'  115.0(7)     no
  Sr2a  Sr2b  O11    .        .        .        79.8(7)     no
  Sr2a  Sr2b  O12    .        .       '1 545'  142.3(8)     no
  Sr2a  Sr2b  O7     .        .       '3 544'   86.8(7)     no
  Sr2a  Sr2b  O8     .        .        .       131.8(8)     no
  Sr2a  Sr2b  Ti2    .        .        .        96.8(7)     no
  Sr2a  Sr2b  Sr1b   .        .       '3 544'   62.3(6)     no
  Sr2a  Sr2b  Ti1    .        .       '3 545'  156.8(7)     no
  Sr2a  Sr2b  Sr1a   .        .       '3 554'   29.2(5)     no
  Sr2a  Sr2b  Sr1b   .        .       '3 554'   36.8(5)     no
  Sr2a  Sr2b  O4     .        .       '4 465'   88.0(6)     no
  Sr2a  Sr2b  K1     .        .       '4 455'   98.0(8)     no
  Sr2a  Sr2b  Sr1a   .        .       '4 455'  104.9(9)     no
  Sr2a  Sr2b  Sr1b   .        .       '4 455'  118.6(9)     no
  Sr2a  Sr2b  P1     .        .       '4 455'  101.8(7)     no
  Sr2a  Sr2b  O1     .        .       '4 455'   76.1(7)     no
  Sr2a  Sr2b  O2     .        .       '4 455'  126.2(8)     no
  Sr2a  Sr2b  O6     .        .        .       161.0(9)     no
  Cr2   Sr2b  O11   '1 545'   .        .       105.5(4)     no
  Cr2   Sr2b  O12   '1 545'   .       '1 545'   27.38(11)   no
  Cr2   Sr2b  O7    '1 545'   .       '3 544'   31.64(13)   no
  Cr2   Sr2b  O8    '1 545'   .        .        95.4(3)     no
  Cr2   Sr2b  Ti2   '1 545'   .        .       121.1(4)     no
  Cr2   Sr2b  Sr1b  '1 545'   .       '3 544'   56.1(2)     no
  Cr2   Sr2b  Ti1   '1 545'   .       '3 545'   51.65(15)   no
  Cr2   Sr2b  Sr1a  '1 545'   .       '3 554'  134.5(3)     no
  Cr2   Sr2b  Sr1b  '1 545'   .       '3 554'  142.0(4)     no
  Cr2   Sr2b  O4    '1 545'   .       '4 465'  152.4(4)     no
  Cr2   Sr2b  K1    '1 545'   .       '4 455'  109.9(3)     no
  Cr2   Sr2b  Sr1a  '1 545'   .       '4 455'  108.1(3)     no
  Cr2   Sr2b  Sr1b  '1 545'   .       '4 455'  102.6(3)     no
  Cr2   Sr2b  P1    '1 545'   .       '4 455'   54.61(15)   no
  Cr2   Sr2b  O1    '1 545'   .       '4 455'   73.2(2)     no
  Cr2   Sr2b  O2    '1 545'   .       '4 455'   60.74(17)   no
  Cr2   Sr2b  O6    '1 545'   .        .        82.4(3)     no
  O11   Sr2b  O12    .        .       '1 545'  104.5(4)     no
  O11   Sr2b  O7     .        .       '3 544'   87.2(4)     no
  O11   Sr2b  O8     .        .        .        55.6(4)     no
  O11   Sr2b  Ti2    .        .        .        31.41(11)   no
  O11   Sr2b  Sr1b   .        .       '3 544'  112.7(4)     no
  O11   Sr2b  Ti1    .        .       '3 545'  120.4(4)     no
  O11   Sr2b  Sr1a   .        .       '3 554'   57.2(2)     no
  O11   Sr2b  Sr1b   .        .       '3 554'   55.2(2)     no
  O11   Sr2b  O4     .        .       '4 465'   61.7(2)     no
  O11   Sr2b  K1     .        .       '4 455'  141.5(3)     no
  O11   Sr2b  Sr1a   .        .       '4 455'  139.7(3)     no
  O11   Sr2b  Sr1b   .        .       '4 455'  134.6(4)     no
  O11   Sr2b  P1     .        .       '4 455'  159.1(4)     no
  O11   Sr2b  O1     .        .       '4 455'  152.2(5)     no
  O11   Sr2b  O2     .        .       '4 455'  153.4(5)     no
  O11   Sr2b  O6     .        .        .       103.9(4)     no
  O12   Sr2b  O7    '1 545'   .       '3 544'   56.6(2)     no
  O12   Sr2b  O8    '1 545'   .        .        73.3(3)     no
  O12   Sr2b  Ti2   '1 545'   .        .       105.8(3)     no
  O12   Sr2b  Sr1b  '1 545'   .       '3 544'   82.3(2)     no
  O12   Sr2b  Ti1   '1 545'   .       '3 545'   28.66(10)   no
  O12   Sr2b  Sr1a  '1 545'   .       '3 554'  155.3(4)     no
  O12   Sr2b  Sr1b  '1 545'   .       '3 554'  158.4(4)     no
  O12   Sr2b  O4    '1 545'   .       '4 465'  127.5(4)     no
  O12   Sr2b  K1    '1 545'   .       '4 455'  100.3(3)     no
  O12   Sr2b  Sr1a  '1 545'   .       '4 455'   95.6(3)     no
  O12   Sr2b  Sr1b  '1 545'   .       '4 455'   85.4(3)     no
  O12   Sr2b  P1    '1 545'   .       '4 455'   61.53(17)   no
  O12   Sr2b  O1    '1 545'   .       '4 455'   86.9(2)     no
  O12   Sr2b  O2    '1 545'   .       '4 455'   52.26(16)   no
  O12   Sr2b  O6    '1 545'   .        .        55.6(2)     no
  O7    Sr2b  O8    '3 544'   .        .       106.2(4)     no
  O7    Sr2b  Ti2   '3 544'   .        .       114.4(4)     no
  O7    Sr2b  Sr1b  '3 544'   .       '3 544'   41.2(2)     no
  O7    Sr2b  Ti1   '3 544'   .       '3 545'   83.1(2)     no
  O7    Sr2b  Sr1a  '3 544'   .       '3 554'  102.9(3)     no
  O7    Sr2b  Sr1b  '3 544'   .       '3 554'  110.4(4)     no
  O7    Sr2b  O4    '3 544'   .       '4 465'  148.9(5)     no
  O7    Sr2b  K1    '3 544'   .       '4 455'  131.2(3)     no
  O7    Sr2b  Sr1a  '3 544'   .       '4 455'  132.6(3)     no
  O7    Sr2b  Sr1b  '3 544'   .       '4 455'  131.7(3)     no
  O7    Sr2b  P1    '3 544'   .       '4 455'   72.20(19)   no
  O7    Sr2b  O1    '3 544'   .       '4 455'   77.9(2)     no
  O7    Sr2b  O2    '3 544'   .       '4 455'   88.4(2)     no
  O7    Sr2b  O6    '3 544'   .        .       111.9(4)     no
  O8    Sr2b  Ti2    .        .        .        35.3(3)     no
  O8    Sr2b  Sr1b   .        .       '3 544'  147.4(4)     no
  O8    Sr2b  Ti1    .        .       '3 545'   71.3(4)     no
  O8    Sr2b  Sr1a   .        .       '3 554'  103.3(4)     no
  O8    Sr2b  Sr1b   .        .       '3 554'   96.9(4)     no
  O8    Sr2b  O4     .        .       '4 465'   57.0(2)     no
  O8    Sr2b  K1     .        .       '4 455'  105.9(4)     no
  O8    Sr2b  Sr1a   .        .       '4 455'   99.4(4)     no
  O8    Sr2b  Sr1b   .        .       '4 455'   87.1(4)     no
  O8    Sr2b  P1     .        .       '4 455'  126.4(5)     no
  O8    Sr2b  O1     .        .       '4 455'  151.4(5)     no
  O8    Sr2b  O2     .        .       '4 455'  100.9(4)     no
  O8    Sr2b  O6     .        .        .        48.4(4)     no
  Ti2   Sr2b  Sr1b   .        .       '3 544'  144.0(4)     no
  Ti2   Sr2b  Ti1    .        .       '3 545'  106.5(3)     no
  Ti2   Sr2b  Sr1a   .        .       '3 554'   67.97(18)   no
  Ti2   Sr2b  Sr1b   .        .       '3 554'   61.6(2)     no
  Ti2   Sr2b  O4     .        .       '4 465'   36.09(12)   no
  Ti2   Sr2b  K1     .        .       '4 455'  113.1(3)     no
  Ti2   Sr2b  Sr1a   .        .       '4 455'  109.6(3)     no
  Ti2   Sr2b  Sr1b   .        .       '4 455'  103.2(3)     no
  Ti2   Sr2b  P1     .        .       '4 455'  160.7(4)     no
  Ti2   Sr2b  O1     .        .       '4 455'  165.7(4)     no
  Ti2   Sr2b  O2     .        .       '4 455'  133.2(4)     no
  Ti2   Sr2b  O6     .        .        .        79.3(2)     no
  Sr1b  Sr2b  Ti1   '3 544'   .       '3 545'   97.1(2)     no
  Sr1b  Sr2b  Sr1a  '3 544'   .       '3 554'   89.8(3)     no
  Sr1b  Sr2b  Sr1b  '3 544'   .       '3 554'   98.2(3)     no
  Sr1b  Sr2b  O4    '3 544'   .       '4 465'  150.1(4)     no
  Sr1b  Sr2b  K1    '3 544'   .       '4 455'   99.4(3)     no
  Sr1b  Sr2b  Sr1a  '3 544'   .       '4 455'  104.3(3)     no
  Sr1b  Sr2b  Sr1b  '3 544'   .       '4 455'  112.5(3)     no
  Sr1b  Sr2b  P1    '3 544'   .       '4 455'   52.9(2)     no
  Sr1b  Sr2b  O1    '3 544'   .       '4 455'   42.8(2)     no
  Sr1b  Sr2b  O2    '3 544'   .       '4 455'   79.8(2)     no
  Sr1b  Sr2b  O6    '3 544'   .        .       129.9(3)     no
  Ti1   Sr2b  Sr1a  '3 545'   .       '3 554'  173.0(3)     no
  Ti1   Sr2b  Sr1b  '3 545'   .       '3 554'  164.5(3)     no
  Ti1   Sr2b  O4    '3 545'   .       '4 465'  111.1(3)     no
  Ti1   Sr2b  K1    '3 545'   .       '4 455'   73.7(2)     no
  Ti1   Sr2b  Sr1a  '3 545'   .       '4 455'   68.2(2)     no
  Ti1   Sr2b  Sr1b  '3 545'   .       '4 455'   57.0(2)     no
  Ti1   Sr2b  P1    '3 545'   .       '4 455'   55.12(15)  no
  Ti1   Sr2b  O1    '3 545'   .       '4 455'   81.3(2)     no
  Ti1   Sr2b  O2    '3 545'   .       '4 455'   32.99(11)  no
  Ti1   Sr2b  O6    '3 545'   .        .        33.34(11)  no
  Sr1a  Sr2b  Sr1b  '3 554'   .       '3 554'    8.5(2)     no
  Sr1a  Sr2b  O4    '3 554'   .       '4 465'   61.9(2)     no
  Sr1a  Sr2b  K1    '3 554'   .       '4 455'  104.1(3)     no
  Sr1a  Sr2b  Sr1a  '3 554'   .       '4 455'  109.1(3)     no
  Sr1a  Sr2b  Sr1b  '3 554'   .       '4 455'  119.2(3)     no
  Sr1a  Sr2b  P1    '3 554'   .       '4 455'  129.8(3)     no
  Sr1a  Sr2b  O1    '3 554'   .       '4 455'  103.2(3)     no
  Sr1a  Sr2b  O2    '3 554'   .       '4 455'  149.0(4)     no
  Sr1a  Sr2b  O6    '3 554'   .        .       139.7(3)     no
  Sr1b  Sr2b  O4    '3 554'   .       '4 465'   53.4(2)     no
  Sr1b  Sr2b  K1    '3 554'   .       '4 455'  101.0(3)     no
  Sr1b  Sr2b  Sr1a  '3 554'   .       '4 455'  105.2(3)     no
  Sr1b  Sr2b  Sr1b  '3 554'   .       '4 455'  113.8(4)     no
  Sr1b  Sr2b  P1    '3 554'   .       '4 455'  135.0(4)     no
  Sr1b  Sr2b  O1    '3 554'   .       '4 455'  108.3(4)     no
  Sr1b  Sr2b  O2    '3 554'   .       '4 455'  149.3(4)     no
  Sr1b  Sr2b  O6    '3 554'   .        .       131.2(3)     no
  O4    Sr2b  K1    '4 465'   .       '4 455'   79.9(3)     no
  O4    Sr2b  Sr1a  '4 465'   .       '4 455'   78.3(3)     no
  O4    Sr2b  Sr1b  '4 465'   .       '4 455'   76.9(3)     no
  O4    Sr2b  P1    '4 465'   .       '4 455'  138.8(4)     no
  O4    Sr2b  O1    '4 465'   .       '4 455'  130.1(5)     no
  O4    Sr2b  O2    '4 465'   .       '4 455'  118.9(4)     no
  O4    Sr2b  O6    '4 465'   .        .        77.8(3)     no
  K1    Sr2b  Sr1a  '4 455'   .       '4 455'    7.22(14)   no
  K1    Sr2b  Sr1b  '4 455'   .       '4 455'   21.3(2)     no
  K1    Sr2b  P1    '4 455'   .       '4 455'   59.3(2)     no
  K1    Sr2b  O1    '4 455'   .       '4 455'   56.8(2)     no
  K1    Sr2b  O2    '4 455'   .       '4 455'   50.08(18)   no
  K1    Sr2b  O6    '4 455'   .        .        67.3(2)     no
  Sr1a  Sr2b  Sr1b  '4 455'   .       '4 455'   14.1(2)     no
  Sr1a  Sr2b  P1    '4 455'   .       '4 455'   60.5(2)     no
  Sr1a  Sr2b  O1    '4 455'   .       '4 455'   61.5(3)     no
  Sr1a  Sr2b  O2    '4 455'   .       '4 455'   47.4(2)     no
  Sr1a  Sr2b  O6    '4 455'   .        .        60.1(3)     no
  Sr1b  Sr2b  P1    '4 455'   .       '4 455'   63.1(3)     no
  Sr1b  Sr2b  O1    '4 455'   .       '4 455'   70.6(3)     no
  Sr1b  Sr2b  O2    '4 455'   .       '4 455'   43.3(2)     no
  Sr1b  Sr2b  O6    '4 455'   .        .        46.0(2)     no
  P1    Sr2b  O1    '4 455'   .       '4 455'   26.75(10)   no
  P1    Sr2b  O2    '4 455'   .       '4 455'   27.68(9)    no
  P1    Sr2b  O6    '4 455'   .        .        81.5(3)     no
  O1    Sr2b  O2    '4 455'   .       '4 455'   50.55(18)   no
  O1    Sr2b  O6    '4 455'   .        .       103.4(4)     no
  O2    Sr2b  O6    '4 455'   .        .        54.0(2)     no
  K1    Ti1   K2     .        .        .        71.869(19)  no
  K1    Ti1   Sr2a   .        .        .        66.73(12)   no
  K1    Ti1   Cr1    .        .        .        46.7(9)     no
  K1    Ti1   O1     .        .        .        50.73(4)    no
  K1    Ti1   O11    .        .        .        52.81(4)    no
  K1    Ti1   O5     .        .       '3 544'   49.67(4)    no
  K1    Ti1   Sr1b   .        .       '2 664'  112.8(2)     no
  K1    Ti1   O2     .        .       '2 664'  119.56(4)    no
  K1    Ti1   O6     .        .       '3 554'  123.07(4)    no
  K1    Ti1   Sr1b   .        .       '3 554'  108.8(2)     no
  K1    Ti1   Sr2b   .        .       '3 554'  177.9(2)     no
  K1    Ti1   O12    .        .       '3 544'  122.79(4)    no
  K1    Ti1   K2     .        .        4        64.250(19)  no
  K1    Ti1   Sr2a   .        .        4        58.54(13)   no
  K2    Ti1   Sr2a   .        .        .         6.06(13)   no
  K2    Ti1   Cr1    .        .        .       112.0(10)    no
  K2    Ti1   O1     .        .        .       120.36(4)    no
  K2    Ti1   O11    .        .        .        46.30(3)    no
  K2    Ti1   O5     .        .       '3 544'   73.43(4)    no
  K2    Ti1   Sr1b   .        .       '2 664'  167.98(17)   no
  K2    Ti1   O2     .        .       '2 664'  141.31(4)    no
  K2    Ti1   O6     .        .       '3 554'  116.78(4)    no
  K2    Ti1   Sr1b   .        .       '3 554'   45.50(17)   no
  K2    Ti1   Sr2b   .        .       '3 554'  110.2(2)     no
  K2    Ti1   O12    .        .       '3 544'   54.48(4)    no
  K2    Ti1   K2     .        .        4       122.812(18)  no
  K2    Ti1   Sr2a   .        .        4       120.18(12)   no
  Sr2a  Ti1   Cr1    .        .        .       106.0(10)    no
  Sr2a  Ti1   O1     .        .        .       114.52(13)   no
  Sr2a  Ti1   O11    .        .        .        40.82(13)   no
  Sr2a  Ti1   O5     .        .       '3 544'   72.85(11)   no
  Sr2a  Ti1   Sr1b   .        .       '2 664'  165.9(2)     no
  Sr2a  Ti1   O2     .        .       '2 664'  146.22(12)   no
  Sr2a  Ti1   O6     .        .       '3 554'  116.31(11)   no
  Sr2a  Ti1   Sr1b   .        .       '3 554'   48.0(2)     no
  Sr2a  Ti1   Sr2b   .        .       '3 554'  115.3(2)     no
  Sr2a  Ti1   O12    .        .       '3 544'   60.45(13)   no
  Sr2a  Ti1   K2     .        .        4       120.80(11)   no
  Sr2a  Ti1   Sr2a   .        .        4       117.54(16)   no
  Cr1   Ti1   O1     .        .        .        11.6(10)    no
  Cr1   Ti1   O11    .        .        .        71.6(10)    no
  Cr1   Ti1   O5     .        .       '3 544'   84.3(8)     no
  Cr1   Ti1   Sr1b   .        .       '2 664'   68.5(10)    no
  Cr1   Ti1   O2     .        .       '2 664'   98.5(10)    no
  Cr1   Ti1   O6     .        .       '3 554'   83.7(8)     no
  Cr1   Ti1   Sr1b   .        .       '3 554'  125.3(10)    no
  Cr1   Ti1   Sr2b   .        .       '3 554'  131.3(9)     no
  Cr1   Ti1   O12    .        .       '3 544'  166.2(10)    no
  Cr1   Ti1   K2     .        .        4        58.2(9)     no
  Cr1   Ti1   Sr2a   .        .        4        52.8(9)     no
  O1    Ti1   O11    .        .        .        82.61(5)    no
  O1    Ti1   O5     .        .       '3 544'   80.21(5)    no
  O1    Ti1   Sr1b   .        .       '2 664'   62.2(2)     no
  O1    Ti1   O2     .        .       '2 664'   87.42(5)    no
  O1    Ti1   O6     .        .       '3 554'   86.93(5)    no
  O1    Ti1   Sr1b   .        .       '3 554'  136.7(2)     no
  O1    Ti1   Sr2b   .        .       '3 554'  127.1(2)     no
  O1    Ti1   O12    .        .       '3 544'  173.10(5)    no
  O1    Ti1   K2     .        .        4        47.57(3)    no
  O1    Ti1   Sr2a   .        .        4        42.67(13)   no
  O11   Ti1   O5     .        .       '3 544'   90.75(5)    no
  O11   Ti1   Sr1b   .        .       '2 664'  126.8(2)     no
  O11   Ti1   O2     .        .       '2 664'  170.02(5)    no
  O11   Ti1   O6     .        .       '3 554'   91.09(5)    no
  O11   Ti1   Sr1b   .        .       '3 554'   59.5(2)     no
  O11   Ti1   Sr2b   .        .       '3 554'  128.27(19)   no
  O11   Ti1   O12    .        .       '3 544'   94.79(5)    no
  O11   Ti1   K2     .        .        4       116.27(4)    no
  O11   Ti1   Sr2a   .        .        4       110.19(13)   no
  O5    Ti1   Sr1b  '3 544'   .       '2 664'  118.25(18)   no
  O5    Ti1   O2    '3 544'   .       '2 664'   87.03(5)    no
  O5    Ti1   O6    '3 544'   .       '3 554'  166.66(5)    no
  O5    Ti1   Sr1b  '3 544'   .       '3 554'  117.40(17)   no
  O5    Ti1   Sr2b  '3 544'   .       '3 554'  130.93(15)   no
  O5    Ti1   O12   '3 544'   .       '3 544'   93.47(5)    no
  O5    Ti1   K2    '3 544'   .        4        50.53(3)    no
  O5    Ti1   Sr2a  '3 544'   .        4        49.81(12)   no
  Sr1b  Ti1   O2    '2 664'   .       '2 664'   47.2(2)     no
  Sr1b  Ti1   O6    '2 664'   .       '3 554'   51.23(18)   no
  Sr1b  Ti1   Sr1b  '2 664'   .       '3 554'  123.7(2)     no
  Sr1b  Ti1   Sr2b  '2 664'   .       '3 554'   65.1(3)     no
  Sr1b  Ti1   O12   '2 664'   .       '3 544'  123.9(2)     no
  Sr1b  Ti1   K2    '2 664'   .        4        68.25(18)   no
  Sr1b  Ti1   Sr2a  '2 664'   .        4        70.3(2)     no
  O2    Ti1   O6    '2 664'   .       '3 554'   88.88(5)    no
  O2    Ti1   Sr1b  '2 664'   .       '3 554'  129.9(2)     no
  O2    Ti1   Sr2b  '2 664'   .       '3 554'   59.1(2)     no
  O2    Ti1   O12   '2 664'   .       '3 544'   95.06(6)    no
  O2    Ti1   K2    '2 664'   .        4        55.38(4)    no
  O2    Ti1   Sr2a  '2 664'   .        4        61.27(13)   no
  O6    Ti1   Sr1b  '3 554'   .       '3 554'   74.67(17)   no
  O6    Ti1   Sr2b  '3 554'   .       '3 554'   55.84(15)   no
  O6    Ti1   O12   '3 554'   .       '3 544'   99.55(6)    no
  O6    Ti1   K2    '3 554'   .        4       117.31(4)    no
  O6    Ti1   Sr2a  '3 554'   .        4       117.42(12)   no
  Sr1b  Ti1   Sr2b  '3 554'   .       '3 554'   72.9(3)     no
  Sr1b  Ti1   O12   '3 554'   .       '3 544'   44.4(2)     no
  Sr1b  Ti1   K2    '3 554'   .        4       167.93(17)   no
  Sr1b  Ti1   Sr2a  '3 554'   .        4       165.5(2)     no
  Sr2b  Ti1   O12   '3 554'   .       '3 544'   59.3(2)     no
  Sr2b  Ti1   K2    '3 554'   .        4       114.3(2)     no
  Sr2b  Ti1   Sr2a  '3 554'   .        4       120.0(2)     no
  O12   Ti1   K2    '3 544'   .        4       129.54(4)    no
  O12   Ti1   Sr2a  '3 544'   .        4       133.83(13)   no
  K2    Ti1   Sr2a   4        .        4         6.24(13)   no
  K1    Cr1   Ti1    .        .        .       129.1(9)     no
  K1    Cr1   O1     .        .        .        55.75(17)   no
  K1    Cr1   O11    .        .        .        58.63(17)   no
  K1    Cr1   O5     .        .       '3 544'   55.07(15)   no
  K1    Cr1   Sr1b   .        .       '2 664'  121.9(3)     no
  K1    Cr1   O2     .        .       '2 664'  126.8(2)     no
  K1    Cr1   O6     .        .       '3 554'  135.0(3)     no
  K1    Cr1   O12    .        .       '3 544'  120.5(2)     no
  K1    Cr1   K2     .        .        4        68.53(11)   no
  K1    Cr1   Sr2a   .        .        4        62.56(17)   no
  Ti1   Cr1   O1     .        .        .       166.2(12)    no
  Ti1   Cr1   O11    .        .        .        98.1(11)    no
  Ti1   Cr1   O5     .        .       '3 544'   85.8(8)     no
  Ti1   Cr1   Sr1b   .        .       '2 664'  106.0(10)    no
  Ti1   Cr1   O2     .        .       '2 664'   71.8(10)    no
  Ti1   Cr1   O6     .        .       '3 554'   86.1(8)     no
  Ti1   Cr1   O12    .        .       '3 544'   11.5(9)     no
  Ti1   Cr1   K2     .        .        4       116.8(10)    no
  Ti1   Cr1   Sr2a   .        .        4       122.6(9)     no
  O1    Cr1   O11    .        .        .        95.0(3)     no
  O1    Cr1   O5     .        .       '3 544'   89.1(2)     no
  O1    Cr1   Sr1b   .        .       '2 664'   66.4(3)     no
  O1    Cr1   O2     .        .       '2 664'   95.0(3)     no
  O1    Cr1   O6     .        .       '3 554'   97.5(3)     no
  O1    Cr1   O12    .        .       '3 544'  173.1(3)     no
  O1    Cr1   K2     .        .        4        50.51(15)   no
  O1    Cr1   Sr2a   .        .        4        45.28(19)   no
  O11   Cr1   O5     .        .       '3 544'   93.3(2)     no
  O11   Cr1   Sr1b   .        .       '2 664'  136.9(3)     no
  O11   Cr1   O2     .        .       '2 664'  169.8(4)     no
  O11   Cr1   O6     .        .       '3 554'   93.8(2)     no
  O11   Cr1   O12    .        .       '3 544'   86.8(3)     no
  O11   Cr1   K2     .        .        4       127.1(3)     no
  O11   Cr1   Sr2a   .        .        4       121.0(3)     no
  O5    Cr1   Sr1b  '3 544'   .       '2 664'  123.2(3)     no
  O5    Cr1   O2    '3 544'   .       '2 664'   85.0(2)     no
  O5    Cr1   O6    '3 544'   .       '3 554'  169.9(4)     no
  O5    Cr1   O12   '3 544'   .       '3 544'   84.1(2)     no
  O5    Cr1   K2    '3 544'   .        4        54.49(14)   no
  O5    Cr1   Sr2a  '3 544'   .        4        54.49(18)   no
  Sr1b  Cr1   O2    '2 664'   .       '2 664'   50.2(2)     no
  Sr1b  Cr1   O6    '2 664'   .       '3 554'   53.9(2)     no
  Sr1b  Cr1   O12   '2 664'   .       '3 544'  116.4(3)     no
  Sr1b  Cr1   K2    '2 664'   .        4        71.5(2)     no
  Sr1b  Cr1   Sr2a  '2 664'   .        4        74.0(3)     no
  O2    Cr1   O6    '2 664'   .       '3 554'   86.8(2)     no
  O2    Cr1   O12   '2 664'   .       '3 544'   83.0(2)     no
  O2    Cr1   K2    '2 664'   .        4        59.34(15)   no
  O2    Cr1   Sr2a  '2 664'   .        4        65.8(2)     no
  O6    Cr1   O12   '3 554'   .       '3 544'   89.0(2)     no
  O6    Cr1   K2    '3 554'   .        4       125.1(3)     no
  O6    Cr1   Sr2a  '3 554'   .        4       126.6(3)     no
  O12   Cr1   K2    '3 544'   .        4       123.5(2)     no
  O12   Cr1   Sr2a  '3 544'   .        4       128.4(2)     no
  K2    Cr1   Sr2a   4        .        4        6.68(14)    no
  K1    Ti2   Sr1a   .       '1 545'   .        6.36(12)    no
  K1    Ti2   Cr2    .       '1 545'  '1 545'   38.4(6)     no
  K1    Ti2   O3     .       '1 545'  '1 545'   48.47(3)    no
  K1    Ti2   O12    .       '1 545'  '1 545'   48.47(3)    no
  K1    Ti2   O7     .       '1 545'  '3 544'   58.28(4)    no
  K1    Ti2   K1     .       '1 545'  '1 545'  121.63(2)    no
  K1    Ti2   K2     .       '1 545'  '1 545'  158.75(3)    no
  K1    Ti2   Sr2a   .       '1 545'  '1 545'  163.93(13)   no
  K1    Ti2   Sr2b   .       '1 545'  '1 545'  178.7(2)     no
  K1    Ti2   O11    .       '1 545'  '1 545'  130.18(4)    no
  K1    Ti2   O8     .       '1 545'  '1 545'  113.0(3)     no
  K1    Ti2   Sr1b   .       '1 545'  '3 544'  115.09(17)   no
  K1    Ti2   O4     .       '1 545'  '4 455'  125.74(3)    no
  K1    Ti2   K2     .       '1 545'  '3 545'   61.532(19)  no
  Sr1a  Ti2   Cr2    .       '1 545'  '1 545'   36.5(6)     no
  Sr1a  Ti2   O3     .       '1 545'  '1 545'   45.99(11)   no
  Sr1a  Ti2   O12    .       '1 545'  '1 545'   45.68(12)   no
  Sr1a  Ti2   O7     .       '1 545'  '3 544'   64.63(13)   no
  Sr1a  Ti2   K1     .       '1 545'  '1 545'  117.29(11)   no
  Sr1a  Ti2   K2     .       '1 545'  '1 545'  164.92(13)   no
  Sr1a  Ti2   Sr2a   .       '1 545'  '1 545'  170.23(18)   no
  Sr1a  Ti2   Sr2b   .       '1 545'  '1 545'  172.7(2)     no
  Sr1a  Ti2   O11    .       '1 545'  '1 545'  132.41(12)   no
  Sr1a  Ti2   O8     .       '1 545'  '1 545'  106.6(4)     no
  Sr1a  Ti2   Sr1b   .       '1 545'  '3 544'  121.4(2)     no
  Sr1a  Ti2   O4     .       '1 545'  '4 455'  127.80(11)   no
  Sr1a  Ti2   K2     .       '1 545'  '3 545'   55.18(12)   no
  Cr2   Ti2   O3    '1 545'  '1 545'  '1 545'   78.3(6)     no
  Cr2   Ti2   O12   '1 545'  '1 545'  '1 545'   11.2(6)     no
  Cr2   Ti2   O7    '1 545'  '1 545'  '3 544'   77.2(6)     no
  Cr2   Ti2   K1    '1 545'  '1 545'  '1 545'  130.5(6)     no
  Cr2   Ti2   K2    '1 545'  '1 545'  '1 545'  148.7(6)     no
  Cr2   Ti2   Sr2a  '1 545'  '1 545'  '1 545'  146.4(6)     no
  Cr2   Ti2   Sr2b  '1 545'  '1 545'  '1 545'  140.4(6)     no
  Cr2   Ti2   O11   '1 545'  '1 545'  '1 545'  168.5(6)     no
  Cr2   Ti2   O8    '1 545'  '1 545'  '1 545'   94.1(8)     no
  Cr2   Ti2   Sr1b  '1 545'  '1 545'  '3 544'  120.9(6)     no
  Cr2   Ti2   O4    '1 545'  '1 545'  '4 455'   95.0(6)     no
  Cr2   Ti2   K2    '1 545'  '1 545'  '3 545'   56.2(6)     no
  O3    Ti2   O12   '1 545'  '1 545'  '1 545'   83.61(5)    no
  O3    Ti2   O7    '1 545'  '1 545'  '3 544'   86.00(4)    no
  O3    Ti2   K1    '1 545'  '1 545'  '1 545'   74.66(3)    no
  O3    Ti2   K2    '1 545'  '1 545'  '1 545'  133.01(3)    no
  O3    Ti2   Sr2a  '1 545'  '1 545'  '1 545'  134.89(12)   no
  O3    Ti2   Sr2b  '1 545'  '1 545'  '1 545'  132.1(2)     no
  O3    Ti2   O11   '1 545'  '1 545'  '1 545'   92.84(5)    no
  O3    Ti2   O8    '1 545'  '1 545'  '1 545'   89.54(10)   no
  O3    Ti2   Sr1b  '1 545'  '1 545'  '3 544'  127.05(18)   no
  O3    Ti2   O4    '1 545'  '1 545'  '4 455'  173.24(5)    no
  O3    Ti2   K2    '1 545'  '1 545'  '3 545'   51.70(4)    no
  O12   Ti2   O7    '1 545'  '1 545'  '3 544'   87.23(5)    no
  O12   Ti2   K1    '1 545'  '1 545'  '1 545'  124.27(5)    no
  O12   Ti2   K2    '1 545'  '1 545'  '1 545'  142.56(3)    no
  O12   Ti2   Sr2a  '1 545'  '1 545'  '1 545'  139.06(13)   no
  O12   Ti2   Sr2b  '1 545'  '1 545'  '1 545'  130.3(2)     no
  O12   Ti2   O11   '1 545'  '1 545'  '1 545'  175.60(5)    no
  O12   Ti2   O8    '1 545'  '1 545'  '1 545'   84.3(4)     no
  O12   Ti2   Sr1b  '1 545'  '1 545'  '3 544'  125.21(17)   no
  O12   Ti2   O4    '1 545'  '1 545'  '4 455'   89.66(4)    no
  O12   Ti2   K2    '1 545'  '1 545'  '3 545'   52.33(4)    no
  O7    Ti2   K1    '3 544'  '1 545'  '1 545'  139.59(4)    no
  O7    Ti2   K2    '3 544'  '1 545'  '1 545'  100.89(4)    no
  O7    Ti2   Sr2a  '3 544'  '1 545'  '1 545'  105.75(14)   no
  O7    Ti2   Sr2b  '3 544'  '1 545'  '1 545'  122.6(2)     no
  O7    Ti2   O11   '3 544'  '1 545'  '1 545'   95.13(6)    no
  O7    Ti2   O8    '3 544'  '1 545'  '1 545'  170.8(4)     no
  O7    Ti2   Sr1b  '3 544'  '1 545'  '3 544'   56.85(17)   no
  O7    Ti2   O4    '3 544'  '1 545'  '4 455'   93.09(5)    no
  O7    Ti2   K2    '3 544'  '1 545'  '3 545'  119.79(4)    no
  K1    Ti2   K2    '1 545'  '1 545'  '1 545'   70.402(18)  no
  K1    Ti2   Sr2a  '1 545'  '1 545'  '1 545'   68.46(12)   no
  K1    Ti2   Sr2b  '1 545'  '1 545'  '1 545'   58.6(2)     no
  K1    Ti2   O11   '1 545'  '1 545'  '1 545'   51.96(4)    no
  K1    Ti2   O8    '1 545'  '1 545'  '1 545'   45.8(3)     no
  K1    Ti2   Sr1b  '1 545'  '1 545'  '3 544'  108.51(17)   no
  K1    Ti2   O4    '1 545'  '1 545'  '4 455'  109.91(3)    no
  K1    Ti2   K2    '1 545'  '1 545'  '3 545'   74.552(19)  no
  K2    Ti2   Sr2a  '1 545'  '1 545'  '1 545'    5.48(13)   no
  K2    Ti2   Sr2b  '1 545'  '1 545'  '1 545'   22.3(2)     no
  K2    Ti2   O11   '1 545'  '1 545'  '1 545'   40.55(4)    no
  K2    Ti2   O8    '1 545'  '1 545'  '1 545'   88.0(4)     no
  K2    Ti2   Sr1b  '1 545'  '1 545'  '3 544'   44.54(17)   no
  K2    Ti2   O4    '1 545'  '1 545'  '4 455'   53.73(3)    no
  K2    Ti2   K2    '1 545'  '1 545'  '3 545'  138.91(2)    no
  Sr2a  Ti2   Sr2b  '1 545'  '1 545'  '1 545'   17.0(2)     no
  Sr2a  Ti2   O11   '1 545'  '1 545'  '1 545'   43.67(12)   no
  Sr2a  Ti2   O8    '1 545'  '1 545'  '1 545'   83.1(4)     no
  Sr2a  Ti2   Sr1b  '1 545'  '1 545'  '3 544'   49.1(2)     no
  Sr2a  Ti2   O4    '1 545'  '1 545'  '4 455'   51.75(12)   no
  Sr2a  Ti2   K2    '1 545'  '1 545'  '3 545'  134.34(13)   no
  Sr2b  Ti2   O11   '1 545'  '1 545'  '1 545'   51.1(2)     no
  Sr2b  Ti2   O8    '1 545'  '1 545'  '1 545'   66.1(4)     no
  Sr2b  Ti2   Sr1b  '1 545'  '1 545'  '3 544'   65.7(3)     no
  Sr2b  Ti2   O4    '1 545'  '1 545'  '4 455'   53.6(2)     no
  Sr2b  Ti2   K2    '1 545'  '1 545'  '3 545'  117.7(2)     no
  O11   Ti2   O8    '1 545'  '1 545'  '1 545'   93.1(4)     no
  O11   Ti2   Sr1b  '1 545'  '1 545'  '3 544'   59.10(17)   no
  O11   Ti2   O4    '1 545'  '1 545'  '4 455'   93.91(5)    no
  O11   Ti2   K2    '1 545'  '1 545'  '3 545'  123.32(4)    no
  O8    Ti2   Sr1b  '1 545'  '1 545'  '3 544'  131.6(4)     no
  O8    Ti2   O4    '1 545'  '1 545'  '4 455'   90.39(6)    no
  O8    Ti2   K2    '1 545'  '1 545'  '3 545'   51.6(3)     no
  Sr1b  Ti2   O4    '3 544'  '1 545'  '4 455'   56.99(18)   no
  Sr1b  Ti2   K2    '3 544'  '1 545'  '3 545'  176.54(16)   no
  O4    Ti2   K2    '4 455'  '1 545'  '3 545'  123.89(4)    no
  K1    Cr2   Sr1a   .       '1 545'   .        7.01(13)    no
  K1    Cr2   Sr2b   .       '1 545'   .        60.7(2)     no
  K1    Cr2   Ti2    .       '1 545'  '1 545'  137.1(7)     no
  K1    Cr2   O3     .       '1 545'  '1 545'   55.71(10)   no
  K1    Cr2   O12    .       '1 545'  '1 545'   55.50(12)   no
  K1    Cr2   O7     .       '1 545'  '3 544'   66.18(12)   no
  K1    Cr2   O8     .       '1 545'  '1 545'  123.5(4)     no
  K1    Cr2   O4     .       '1 545'  '4 455'  138.89(17)   no
  K1    Cr2   K2     .       '1 545'  '3 545'   66.74(8)    no
  Sr1a  Cr2   Sr2b   .       '1 545'   .        65.4(2)     no
  Sr1a  Cr2   Ti2    .       '1 545'  '1 545'  139.3(7)     no
  Sr1a  Cr2   O3     .       '1 545'  '1 545'   53.55(15)   no
  Sr1a  Cr2   O12    .       '1 545'  '1 545'   52.19(18)   no
  Sr1a  Cr2   O7     .       '1 545'  '3 544'   73.17(18)   no
  Sr1a  Cr2   O8     .       '1 545'  '1 545'  116.6(4)     no
  Sr1a  Cr2   O4     .       '1 545'  '4 455'  142.1(2)     no
  Sr1a  Cr2   K2     .       '1 545'  '3 545'   59.76(15)   no
  Sr2b  Cr2   Ti2    .       '1 545'  '1 545'  128.5(7)     no
  Sr2b  Cr2   O3     .       '1 545'  '1 545'  113.3(2)     no
  Sr2b  Cr2   O12    .       '1 545'  '1 545'   59.8(2)     no
  Sr2b  Cr2   O7     .       '1 545'  '3 544'   47.7(2)     no
  Sr2b  Cr2   O8     .       '1 545'  '1 545'  145.8(4)     no
  Sr2b  Cr2   O4     .       '1 545'  '4 455'   78.8(2)     no
  Sr2b  Cr2   K2     .       '1 545'  '3 545'  112.7(2)     no
  Ti2   Cr2   O3    '1 545'  '1 545'  '1 545'   89.9(6)     no
  Ti2   Cr2   O12   '1 545'  '1 545'  '1 545'  166.0(8)     no
  Ti2   Cr2   O7    '1 545'  '1 545'  '3 544'   90.7(7)     no
  Ti2   Cr2   O8    '1 545'  '1 545'  '1 545'   74.3(8)     no
  Ti2   Cr2   O4    '1 545'  '1 545'  '4 455'   73.4(6)     no
  Ti2   Cr2   K2    '1 545'  '1 545'  '3 545'  118.3(6)     no
  O3    Cr2   O12   '1 545'  '1 545'  '1 545'   96.5(2)     no
  O3    Cr2   O7    '1 545'  '1 545'  '3 544'   88.52(18)   no
  O3    Cr2   O8    '1 545'  '1 545'  '1 545'   88.71(17)   no
  O3    Cr2   O4    '1 545'  '1 545'  '4 455'  163.3(2)     no
  O3    Cr2   K2    '1 545'  '1 545'  '3 545'   56.78(12)   no
  O12   Cr2   O7    '1 545'  '1 545'  '3 544'  101.9(2)     no
  O12   Cr2   O8    '1 545'  '1 545'  '1 545'   93.4(5)     no
  O12   Cr2   O4    '1 545'  '1 545'  '4 455'   99.7(2)     no
  O12   Cr2   K2    '1 545'  '1 545'  '3 545'   56.85(14)   no
  O7    Cr2   O8    '3 544'  '1 545'  '1 545'  164.7(5)     no
  O7    Cr2   O4    '3 544'  '1 545'  '4 455'   92.2(2)     no
  O7    Cr2   K2    '3 544'  '1 545'  '3 545'  131.95(18)   no
  O8    Cr2   O4    '1 545'  '1 545'  '4 455'   86.3(2)     no
  O8    Cr2   K2    '1 545'  '1 545'  '3 545'   56.9(4)     no
  O4    Cr2   K2    '4 455'  '1 545'  '3 545'  130.88(19)   no
  K1    P1    Sr1a   .        .        .         7.18(14)   no
  K1    P1    O1     .        .        .        62.07(5)    no
  K1    P1    O2     .        .        .        55.87(5)    no
  K1    P1    O3     .        .        .        95.26(4)    no
  K1    P1    O4     .        .        .       155.28(4)    no
  K1    P1    K2     .        .        3        83.53(3)    no
  K1    P1    Sr2b   .        .        4        60.7(2)     no
  Sr1a  P1    O1     .        .        .        67.89(14)   no
  Sr1a  P1    O2     .        .        .        48.69(14)   no
  Sr1a  P1    O3     .        .        .        97.05(12)   no
  Sr1a  P1    O4     .        .        .       151.56(13)   no
  Sr1a  P1    K2     .        .        3        78.89(13)   no
  Sr1a  P1    Sr2b   .        .        4        60.3(2)     no
  O1    P1    O2     .        .        .       108.20(7)    no
  O1    P1    O3     .        .        .       112.10(7)    no
  O1    P1    O4     .        .        .       110.33(8)    no
  O1    P1    K2     .        .        3       143.58(5)    no
  O1    P1    Sr2b   .        .        4        50.8(2)     no
  O2    P1    O3     .        .        .       106.09(7)    no
  O2    P1    O4     .        .        .       110.99(7)    no
  O2    P1    K2     .        .        3        54.12(5)    no
  O2    P1    Sr2b   .        .        4        69.1(2)     no
  O3    P1    O4     .        .        .       109.07(5)    no
  O3    P1    K2     .        .        3        56.49(5)    no
  O3    P1    Sr2b   .        .        4       154.4(2)     no
  O4    P1    K2     .        .        3       105.97(5)    no
  O4    P1    Sr2b   .        .        4        95.7(2)     no
  K2    P1    Sr2b   3        .        4       123.1(2)     no
  K1    P2    K2     .       '3 544'   .        77.87(2)    no
  K1    P2    Sr2a   .       '3 544'   .        71.99(14)   no
  K1    P2    O5     .       '3 544'  '3 544'   51.91(5)    no
  K1    P2    O7     .       '3 544'  '3 544'   59.11(5)    no
  K1    P2    O6     .       '3 544'  '3 544'  110.97(5)    no
  K1    P2    Sr1b   .       '3 544'  '3 544'  125.1(2)     no
  K1    P2    O8     .       '3 544'  '3 544'  138.8(4)     no
  K2    P2    Sr2a   .       '3 544'   .         6.56(14)   no
  K2    P2    O5     .       '3 544'  '3 544'   88.43(5)    no
  K2    P2    O7     .       '3 544'  '3 544'   58.14(5)    no
  K2    P2    O6     .       '3 544'  '3 544'  161.62(5)    no
  K2    P2    Sr1b   .       '3 544'  '3 544'   72.69(19)   no
  K2    P2    O8     .       '3 544'  '3 544'   63.2(5)     no
  Sr2a  P2    O5     .       '3 544'  '3 544'   87.00(13)   no
  Sr2a  P2    O7     .       '3 544'  '3 544'   52.85(14)   no
  Sr2a  P2    O6     .       '3 544'  '3 544'  161.05(13)   no
  Sr2a  P2    Sr1b   .       '3 544'  '3 544'   74.7(2)     no
  Sr2a  P2    O8     .       '3 544'  '3 544'   69.6(5)     no
  O5    P2    O7    '3 544'  '3 544'  '3 544'  107.92(7)    no
  O5    P2    O6    '3 544'  '3 544'  '3 544'  109.78(6)    no
  O5    P2    Sr1b  '3 544'  '3 544'  '3 544'  160.63(19)   no
  O5    P2    O8    '3 544'  '3 544'  '3 544'  111.28(10)   no
  O7    P2    O6    '3 544'  '3 544'  '3 544'  111.51(7)    no
  O7    P2    Sr1b  '3 544'  '3 544'  '3 544'   66.0(2)     no
  O7    P2    O8    '3 544'  '3 544'  '3 544'  106.1(5)     no
  O6    P2    Sr1b  '3 544'  '3 544'  '3 544'   89.31(19)   no
  O6    P2    O8    '3 544'  '3 544'  '3 544'  110.2(4)     no
  Sr1b  P2    O8    '3 544'  '3 544'  '3 544'   56.6(3)     no
  K1    O1    Sr1a   .        .        .         6.92(14)   no
  K1    O1    Ti1    .        .        .        94.56(4)    no
  K1    O1    Cr1    .        .        .        93.6(2)     no
  K1    O1    P1     .        .        .        90.27(6)    no
  K1    O1    Sr1b   .        .       '2 664'  173.2(2)     no
  K1    O1    K2     .        .        4        88.75(4)    no
  K1    O1    Sr2a   .        .        4        82.94(18)   no
  K1    O1    Sr2b   .        .        4        74.0(3)     no
  Sr1a  O1    Ti1    .        .        .       101.43(14)   no
  Sr1a  O1    Cr1    .        .        .       100.4(2)     no
  Sr1a  O1    P1     .        .        .        85.15(14)   no
  Sr1a  O1    Sr1b   .        .       '2 664'  174.2(2)     no
  Sr1a  O1    K2     .        .        4        88.73(13)   no
  Sr1a  O1    Sr2a   .        .        4        82.2(2)     no
  Sr1a  O1    Sr2b   .        .        4        70.7(3)     no
  Ti1   O1    Cr1    .        .        .         2.3(2)     no
  Ti1   O1    P1     .        .        .       131.42(7)    no
  Ti1   O1    Sr1b   .        .       '2 664'   81.7(2)     no
  Ti1   O1    K2     .        .        4        96.47(5)    no
  Ti1   O1    Sr2a   .        .        4       103.33(19)   no
  Ti1   O1    Sr2b   .        .        4       125.3(2)     no
  Cr1   O1    P1     .        .        .       129.43(19)   no
  Cr1   O1    Sr1b   .        .       '2 664'   82.9(3)     no
  Cr1   O1    K2     .        .        4        98.52(18)   no
  Cr1   O1    Sr2a   .        .        4       105.3(3)     no
  Cr1   O1    Sr2b   .        .        4       127.0(3)     no
  P1    O1    Sr1b   .        .       '2 664'   96.4(2)     no
  P1    O1    K2     .        .        4       131.99(7)    no
  P1    O1    Sr2a   .        .        4       125.2(2)     no
  P1    O1    Sr2b   .        .        4       102.5(2)     no
  Sr1b  O1    K2    '2 664'   .        4        86.1(2)     no
  Sr1b  O1    Sr2a  '2 664'   .        4        92.4(3)     no
  Sr1b  O1    Sr2b  '2 664'   .        4       103.5(3)     no
  K2    O1    Sr2a   4        .        4         8.7(2)     no
  K2    O1    Sr2b   4        .        4        32.2(2)     no
  Sr2a  O1    Sr2b   4        .        4        23.8(3)     no
  K1    O2    Sr1a   .        .        .         8.59(18)   no
  K1    O2    Sr1b   .        .        .        30.8(3)     no
  K1    O2    P1     .        .        .        96.21(6)    no
  K1    O2    Ti1    .        .       '2 665'  124.35(6)    no
  K1    O2    Cr1    .        .       '2 665'  120.63(15)   no
  K1    O2    K2     .        .        3       107.10(4)    no
  K1    O2    Sr2b   .        .        4        69.2(2)     no
  Sr1a  O2    Sr1b   .        .        .        22.5(3)     no
  Sr1a  O2    P1     .        .        .       104.80(18)   no
  Sr1a  O2    Ti1    .        .       '2 665'  116.73(17)   no
  Sr1a  O2    Cr1    .        .       '2 665'  112.4(2)     no
  Sr1a  O2    K2     .        .        3       104.74(17)   no
  Sr1a  O2    Sr2b   .        .        4        71.0(3)     no
  Sr1b  O2    P1     .        .        .       125.8(3)     no
  Sr1b  O2    Ti1    .        .       '2 665'   99.9(3)     no
  Sr1b  O2    Cr1    .        .       '2 665'   93.6(3)     no
  Sr1b  O2    K2     .        .        3        91.2(3)     no
  Sr1b  O2    Sr2b   .        .        4        83.9(3)     no
  P1    O2    Ti1    .        .       '2 665'  131.79(7)    no
  P1    O2    Cr1    .        .       '2 665'  139.78(17)   no
  P1    O2    K2     .        .        3       100.95(6)    no
  P1    O2    Sr2b   .        .        4        83.2(2)     no
  Ti1   O2    Cr1   '2 665'   .       '2 665'   9.78(18)    no
  Ti1   O2    K2    '2 665'   .        3        91.51(5)    no
  Ti1   O2    Sr2b  '2 665'   .        4        87.9(2)     no
  Cr1   O2    K2    '2 665'   .        3        84.17(17)   no
  Cr1   O2    Sr2b  '2 665'   .        4        94.6(3)     no
  K2    O2    Sr2b   3        .        4       174.80(19)   no
  K1    O3    Sr1a   .       '1 545'   .         8.87(17)   no
  K1    O3    Sr1b   .       '1 545'   .        27.5(2)     no
  K1    O3    Ti2    .       '1 545'  '1 545'   97.36(4)    no
  K1    O3    Cr2    .       '1 545'  '1 545'   86.91(12)   no
  K1    O3    P1     .       '1 545'  '1 545'  131.80(5)    no
  K1    O3    K2     .       '1 545'  '3 545'   82.83(4)    no
  Sr1a  O3    Sr1b   .       '1 545'   .        19.0(3)     no
  Sr1a  O3    Ti2    .       '1 545'  '1 545'  101.45(15)   no
  Sr1a  O3    Cr2    .       '1 545'  '1 545'   90.3(2)     no
  Sr1a  O3    P1     .       '1 545'  '1 545'  128.63(16)   no
  Sr1a  O3    K2     .       '1 545'  '3 545'   74.64(17)   no
  Sr1b  O3    Ti2    .       '1 545'  '1 545'  103.6(2)     no
  Sr1b  O3    Cr2    .       '1 545'  '1 545'   91.8(2)     no
  Sr1b  O3    P1     .       '1 545'  '1 545'  124.3(2)     no
  Sr1b  O3    K2     .       '1 545'  '3 545'   55.7(2)     no
  Ti2   O3    Cr2   '1 545'  '1 545'  '1 545'   11.78(12)   no
  Ti2   O3    P1    '1 545'  '1 545'  '1 545'  129.88(6)    no
  Ti2   O3    K2    '1 545'  '1 545'  '3 545'   96.54(4)    no
  Cr2   O3    P1    '1 545'  '1 545'  '1 545'  141.01(13)   no
  Cr2   O3    K2    '1 545'  '1 545'  '3 545'   89.87(14)   no
  P1    O3    K2    '1 545'  '1 545'  '3 545'   98.47(6)    no
  Sr1b  O4    P1     .       '2 665'  '2 665'   99.5(2)     no
  Sr1b  O4    K2     .       '2 665'  '3 545'   54.8(2)     no
  Sr1b  O4    Sr2a   .       '2 665'  '3 545'   61.2(3)     no
  Sr1b  O4    Sr2b   .       '2 665'  '3 545'   82.5(3)     no
  Sr1b  O4    Ti2    .       '2 665'  '3 545'   90.9(2)     no
  Sr1b  O4    Cr2    .       '2 665'  '3 545'   97.3(2)     no
  P1    O4    K2    '2 665'  '2 665'  '3 545'  126.52(5)    no
  P1    O4    Sr2a  '2 665'  '2 665'  '3 545'  128.20(16)   no
  P1    O4    Sr2b  '2 665'  '2 665'  '3 545'  134.8(3)     no
  P1    O4    Ti2   '2 665'  '2 665'  '3 545'  134.57(6)    no
  P1    O4    Cr2   '2 665'  '2 665'  '3 545'  123.53(13)   no
  K2    O4    Sr2a  '3 545'  '2 665'  '3 545'    6.40(16)   no
  K2    O4    Sr2b  '3 545'  '2 665'  '3 545'   28.2(2)     no
  K2    O4    Ti2   '3 545'  '2 665'  '3 545'   95.47(4)    no
  K2    O4    Cr2   '3 545'  '2 665'  '3 545'  107.08(12)   no
  Sr2a  O4    Sr2b  '3 545'  '2 665'  '3 545'   21.9(3)     no
  Sr2a  O4    Ti2   '3 545'  '2 665'  '3 545'   95.55(15)   no
  Sr2a  O4    Cr2   '3 545'  '2 665'  '3 545'  107.12(19)   no
  Sr2b  O4    Ti2   '3 545'  '2 665'  '3 545'   90.3(3)     no
  Sr2b  O4    Cr2   '3 545'  '2 665'  '3 545'  100.7(3)     no
  Ti2   O4    Cr2   '3 545'  '2 665'  '3 545'   11.61(12)   no
  K1    O11   K2     .        .        .        99.00(4)    no
  K1    O11   Sr2a   .        .        .        94.34(17)   no
  K1    O11   Sr2b   .        .        .        76.3(2)     no
  K1    O11   Ti1    .        .        .        95.85(4)    no
  K1    O11   Cr1    .        .        .        89.07(18)   no
  K1    O11   Ti2    .        .        .       100.30(5)    no
  K1    O11   Sr1b   .        .       '3 554'  156.0(2)     no
  K2    O11   Sr2a   .        .        .         8.47(18)   no
  K2    O11   Sr2b   .        .        .        31.6(3)     no
  K2    O11   Ti1    .        .        .       102.91(5)    no
  K2    O11   Cr1    .        .        .       111.75(19)   no
  K2    O11   Ti2    .        .        .       114.83(5)    no
  K2    O11   Sr1b   .        .       '3 554'   57.1(2)     no
  Sr2a  O11   Sr2b   .        .        .        23.4(3)     no
  Sr2a  O11   Ti1    .        .        .       110.58(18)   no
  Sr2a  O11   Cr1    .        .        .       119.0(3)     no
  Sr2a  O11   Ti2    .        .        .       109.09(17)   no
  Sr2a  O11   Sr1b   .        .       '3 554'   62.2(3)     no
  Sr2b  O11   Ti1    .        .        .       126.5(2)     no
  Sr2b  O11   Cr1    .        .        .       132.1(3)     no
  Sr2b  O11   Ti2    .        .        .        97.5(2)     no
  Sr2b  O11   Sr1b   .        .       '3 554'   82.1(3)     no
  Ti1   O11   Cr1    .        .        .        10.3(2)     no
  Ti1   O11   Ti2    .        .        .       135.59(6)    no
  Ti1   O11   Sr1b   .        .       '3 554'   88.7(2)     no
  Cr1   O11   Ti2    .        .        .       130.10(17)   no
  Cr1   O11   Sr1b   .        .       '3 554'   98.0(3)     no
  Ti2   O11   Sr1b   .        .       '3 554'   92.6(2)     no
  K1    O12   Sr1a   .       '1 545'   .         8.90(17)   no
  K1    O12   Sr1b   .       '1 545'   .        30.5(3)     no
  K1    O12   Sr2b   .       '1 545'   .        73.1(2)     no
  K1    O12   Ti2    .       '1 545'  '1 545'   96.77(5)    no
  K1    O12   Cr2    .       '1 545'  '1 545'   94.22(15)   no
  K1    O12   K2     .       '1 545'  '3 545'   82.52(4)    no
  K1    O12   Ti1    .       '1 545'  '3 545'  129.12(6)    no
  K1    O12   Cr1    .       '1 545'  '3 545'  128.41(15)   no
  Sr1a  O12   Sr1b   .       '1 545'   .        21.8(3)     no
  Sr1a  O12   Sr2b   .       '1 545'   .        80.6(3)     no
  Sr1a  O12   Ti2    .       '1 545'  '1 545'  101.23(16)   no
  Sr1a  O12   Cr2    .       '1 545'  '1 545'   98.8(2)     no
  Sr1a  O12   K2     .       '1 545'  '3 545'   74.54(16)   no
  Sr1a  O12   Ti1    .       '1 545'  '3 545'  125.35(17)   no
  Sr1a  O12   Cr1    .       '1 545'  '3 545'  124.3(2)     no
  Sr1b  O12   Sr2b   .       '1 545'   .        95.6(3)     no
  Sr1b  O12   Ti2    .       '1 545'  '1 545'  115.8(3)     no
  Sr1b  O12   Cr2    .       '1 545'  '1 545'  113.9(3)     no
  Sr1b  O12   K2     .       '1 545'  '3 545'   59.0(2)     no
  Sr1b  O12   Ti1    .       '1 545'  '3 545'  109.3(3)     no
  Sr1b  O12   Cr1    .       '1 545'  '3 545'  107.7(3)     no
  Sr2b  O12   Ti2    .       '1 545'  '1 545'   94.6(2)     no
  Sr2b  O12   Cr2    .       '1 545'  '1 545'   92.8(2)     no
  Sr2b  O12   K2     .       '1 545'  '3 545'  154.6(2)     no
  Sr2b  O12   Ti1    .       '1 545'  '3 545'   92.0(2)     no
  Sr2b  O12   Cr1    .       '1 545'  '3 545'   93.9(3)     no
  Ti2   O12   Cr2   '1 545'  '1 545'  '1 545'    2.78(15)   no
  Ti2   O12   K2    '1 545'  '1 545'  '3 545'   95.33(5)    no
  Ti2   O12   Ti1   '1 545'  '1 545'  '3 545'  133.41(7)    no
  Ti2   O12   Cr1   '1 545'  '1 545'  '3 545'  134.49(16)   no
  Cr2   O12   K2    '1 545'  '1 545'  '3 545'   96.11(16)   no
  Cr2   O12   Ti1   '1 545'  '1 545'  '3 545'  135.73(16)   no
  Cr2   O12   Cr1   '1 545'  '1 545'  '3 545'  136.9(2)     no
  K2    O12   Ti1   '3 545'  '1 545'  '3 545'   97.94(6)    no
  K2    O12   Cr1   '3 545'  '1 545'  '3 545'   95.68(18)   no
  Ti1   O12   Cr1   '3 545'  '1 545'  '3 545'    2.32(18)   no
  K1    O5    Ti1    .       '3 544'   .        97.47(5)    no
  K1    O5    Cr1    .       '3 544'   .        89.3(2)     no
  K1    O5    P2     .       '3 544'  '3 544'  103.23(6)    no
  K1    O5    K2     .       '3 544'   4        87.12(4)    no
  K1    O5    Sr2a   .       '3 544'   4        78.92(17)   no
  Ti1   O5    Cr1    .       '3 544'   .         9.91(18)   no
  Ti1   O5    P2     .       '3 544'  '3 544'  132.98(7)    no
  Ti1   O5    K2     .       '3 544'   4        95.15(4)    no
  Ti1   O5    Sr2a   .       '3 544'   4        97.06(15)   no
  Cr1   O5    P2     .       '3 544'  '3 544'  141.4(2)     no
  Cr1   O5    K2     .       '3 544'   4        89.12(18)   no
  Cr1   O5    Sr2a   .       '3 544'   4        90.0(2)     no
  P2    O5    K2    '3 544'  '3 544'   4       127.30(6)    no
  P2    O5    Sr2a  '3 544'  '3 544'   4       127.97(15)   no
  K2    O5    Sr2a   4       '3 544'   4         8.25(17)   no
  Sr1a  O6    Sr1b   .        4        .        18.5(3)     no
  Sr1a  O6    P2     .        4        4       128.95(12)   no
  Sr1a  O6    Ti1    .        4       '2 665'   95.16(11)   no
  Sr1a  O6    Cr1    .        4       '2 665'   94.4(2)     no
  Sr1a  O6    Sr2b   .        4        4        65.3(3)     no
  Sr1b  O6    P2     .        4        4       128.3(2)     no
  Sr1b  O6    Ti1    .        4       '2 665'   95.2(2)     no
  Sr1b  O6    Cr1    .        4       '2 665'   91.2(3)     no
  Sr1b  O6    Sr2b   .        4        4        83.8(4)     no
  P2    O6    Ti1    4        4       '2 665'  135.50(8)    no
  P2    O6    Cr1    4        4       '2 665'  136.5(2)     no
  P2    O6    Sr2b   4        4        4       101.7(2)     no
  Ti1   O6    Cr1   '2 665'   4       '2 665'   10.19(19)   no
  Ti1   O6    Sr2b  '2 665'   4        4        90.82(16)   no
  Cr1   O6    Sr2b  '2 665'   4        4        99.7(3)     no
  K1    O7    K2     .       '3 544'   .        94.31(4)    no
  K1    O7    Sr2a   .       '3 544'   .        89.04(16)   no
  K1    O7    Sr2b   .       '3 544'   .        74.0(3)     no
  K1    O7    Ti2    .       '3 544'  '1 545'   88.50(5)    no
  K1    O7    Cr2    .       '3 544'  '1 545'   78.75(13)   no
  K1    O7    P2     .       '3 544'  '3 544'   95.16(5)    no
  K1    O7    Sr1b   .       '3 544'  '3 544'  177.5(2)     no
  K2    O7    Sr2a   .       '3 544'   .         8.13(17)   no
  K2    O7    Sr2b   .       '3 544'   .        30.2(2)     no
  K2    O7    Ti2    .       '3 544'  '1 545'  134.55(5)    no
  K2    O7    Cr2    .       '3 544'  '1 545'  127.32(14)   no
  K2    O7    P2     .       '3 544'  '3 544'   94.94(6)    no
  K2    O7    Sr1b   .       '3 544'  '3 544'   84.2(2)     no
  Sr2a  O7    Sr2b   .       '3 544'   .        22.1(3)     no
  Sr2a  O7    Ti2    .       '3 544'  '1 545'  128.32(17)   no
  Sr2a  O7    Cr2    .       '3 544'  '1 545'  120.1(2)     no
  Sr2a  O7    P2     .       '3 544'  '3 544'  101.61(17)   no
  Sr2a  O7    Sr1b   .       '3 544'  '3 544'   89.2(3)     no
  Sr2b  O7    Ti2    .       '3 544'  '1 545'  110.6(2)     no
  Sr2b  O7    Cr2    .       '3 544'  '1 545'  100.6(3)     no
  Sr2b  O7    P2     .       '3 544'  '3 544'  118.3(2)     no
  Sr2b  O7    Sr1b   .       '3 544'  '3 544'  103.8(3)     no
  Ti2   O7    Cr2   '1 545'  '3 544'  '1 545'   12.18(13)   no
  Ti2   O7    P2    '1 545'  '3 544'  '3 544'  130.03(7)    no
  Ti2   O7    Sr1b  '1 545'  '3 544'  '3 544'   91.2(2)     no
  Cr2   O7    P2    '1 545'  '3 544'  '3 544'  137.45(15)   no
  Cr2   O7    Sr1b  '1 545'  '3 544'  '3 544'  100.6(3)     no
  P2    O7    Sr1b  '3 544'  '3 544'  '3 544'   87.0(2)     no
  K1    O8    Sr1a   .        .        .         8.68(17)   no
  K1    O8    Sr1b   .        .        .        29.6(3)     no
  K1    O8    Sr2b   .        .        .        72.3(4)     no
  K1    O8    Ti2    .        .        .       103.0(8)     no
  K1    O8    Cr2    .        .        .       112.7(8)     no
  K1    O8    K2     .        .        3       104.81(17)   no
  K1    O8    P2     .        .        .       119.0(4)     no
  Sr1a  O8    Sr1b   .        .        .        21.0(3)     no
  Sr1a  O8    Sr2b   .        .        .        79.1(4)     no
  Sr1a  O8    Ti2    .        .        .       110.2(8)     no
  Sr1a  O8    Cr2    .        .        .       119.2(8)     no
  Sr1a  O8    K2     .        .        3        98.6(3)     no
  Sr1a  O8    P2     .        .        .       113.6(5)     no
  Sr1b  O8    Sr2b   .        .        .        93.0(4)     no
  Sr1b  O8    Ti2    .        .        .       129.1(7)     no
  Sr1b  O8    Cr2    .        .        .       136.1(7)     no
  Sr1b  O8    K2     .        .        3        86.2(4)     no
  Sr1b  O8    P2     .        .        .        96.8(6)     no
  Sr2b  O8    Ti2    .        .        .        78.5(6)     no
  Sr2b  O8    Cr2    .        .        .        88.0(7)     no
  Sr2b  O8    K2     .        .        3       174.3(7)     no
  Sr2b  O8    P2     .        .        .        95.8(3)     no
  Ti2   O8    Cr2    .        .        .        11.64(15)   no
  Ti2   O8    K2     .        .        3        97.59(5)    no
  Ti2   O8    P2     .        .        .       133.79(9)    no
  Cr2   O8    K2     .        .        3        88.61(16)   no
  Cr2   O8    P2     .        .        .       126.8(2)     no
  K2    O8    P2     3        .        .        89.9(8)     no




data_BaKTP

 
#------------------------------------------------------------------------------
# B1. CRYSTAL DATA for the BaKTP structure
#------------------------------------------------------------------------------
 
_chemical_formula_sum                 'Ba0.06 K0.88 O5 P Ti'
_chemical_formula_moiety              'Ba0.06 K0.88 Ti O P O4'
_chemical_formula_weight               201.6
_chemical_melting_point               'not measured'
 
_symmetry_cell_setting                 orthorhombic
_symmetry_space_group_name_H-M        'P n a 21'
_symmetry_space_group_name_Hall       'p 2c -2n'
 
loop_
_symmetry_equiv_pos_as_xyz
  +x,+y,+z  -x,-y,1/2+z  1/2-x,1/2+y,1/2+z  1/2+x,1/2-y,+z

_cell_special_details
;
Reflections used for the determination of the unit cell:
  (20 0 -6), (-20 0 6), (16 -4 0), (-16 4 0),
  (0 4 12), (0 -4 12), (16 0 0), (-16 0 0),
  (0 10 0), (0 -10 0), (0 0 20), (0 0 -20).
;

_cell_length_a                         12.851(6)
_cell_length_b                         6.418(3)
_cell_length_c                         10.620(5)
_cell_angle_alpha                      90.000
_cell_angle_beta                       90.000
_cell_angle_gamma                      90.000
_cell_volume                           876.0(7)
_cell_formula_units_Z                  8
_cell_measurement_reflns_used          12
_cell_measurement_theta_min            25.3
_cell_measurement_theta_max            45.0
_cell_measurement_temperature          120(1)
_cell_measurement_radiation            ?
_cell_measurement_wavelength          ?
  
_exptl_crystal_density_diffrn          3.057
_exptl_crystal_density_meas           'not measured'
_exptl_crystal_density_method          ?

_exptl_crystal_description             prism

_exptl_crystal_size_max                0.032
_exptl_crystal_size_mid                0.024
_exptl_crystal_size_min                0.016
_exptl_crystal_size_rad                ?
_exptl_crystal_colour                 'light green-brown'

_exptl_crystal_F_000                   776.86
_exptl_absorpt_coefficient_mu          3.605 
_exptl_absorpt_correction_type         analytical
_exptl_absorpt_process_details
;
Alcock, N. W. 1974. Absorption and Extinction Corrections: Calculation
Methods and Standard Tests. Acta Cryst. A30, 332-335
;
_exptl_absorpt_correction_T_min        .8959
_exptl_absorpt_correction_T_max        .9446


#------------------------------------------------------------------------------
# B2. EXPERIMENTAL DATA for the BaKTP structure
#------------------------------------------------------------------------------

_exptl_special_details
;  ?
;

_diffrn_special_details
;  ?
;

_diffrn_radiation_type                'synchrotron x-ray vertical wiggler'
_diffrn_radiation_wavelength           .75000(9)
_diffrn_radiation_source              'photon factory bl14a'
_diffrn_ambient_temperature            120(1)
_diffrn_ambient_environment            ?
 
_diffrn_measurement_device_type       'bl14a 4-circle'
_diffrn_measurement_method             ω-2θ   
_diffrn_radiation_monochromator        si(111)  
_diffrn_radiation_detector            'avalanche photo diode'

_diffrn_detector_area_resol_mean       ?
_diffrn_measured_fraction_theta_max    ?
_diffrn_measured_fraction_theta_full   ?

_diffrn_reflns_number                  10098

_diffrn_reflns_theta_min               3.35 
_diffrn_reflns_theta_max               32.38
_diffrn_reflns_theta_full              ?
_diffrn_reflns_av_R_equivalents        .079
_diffrn_reflns_av_sigmaI/netI          .059
_diffrn_reflns_limit_h_min            -18
_diffrn_reflns_limit_h_max             18
_diffrn_reflns_limit_k_min            -9
_diffrn_reflns_limit_k_max             9
_diffrn_reflns_limit_l_min            -15
_diffrn_reflns_limit_l_max             15
_diffrn_reflns_reduction_process      'equatorial monochr Lp'

_diffrn_standards_number               6
_diffrn_standards_interval_count       94
_diffrn_standards_decay_%              2

loop_
_diffrn_standard_refln_index_h
_diffrn_standard_refln_index_k
_diffrn_standard_refln_index_l
   0   0   4
   0   0  -4
   0   4   0
   0  -4   0
   8   0   0
  -8   0   0

 
#------------------------------------------------------------------------------
# B3. REFINEMENT DATA for the BaKTP structure
#------------------------------------------------------------------------------

_refine_special_details
;
No constrints or restraints used.
;

_reflns_number_total                   2663
_reflns_number_gt                      2631
_reflns_Friedel_coverage               .906
_reflns_threshold_expression           F>2σ(F)

_reflns_limit_h_min                    0
_reflns_limit_h_max                    18
_reflns_limit_k_min                    0
_reflns_limit_k_max                    9
_reflns_limit_l_min                   -15
_reflns_limit_l_max                    15
_reflns_d_resolution_high              .7
_reflns_d_resolution_low               6.417 
 
_refine_ls_structure_factor_coef       F
_refine_ls_matrix_type                 full
_refine_ls_R_factor_all                .033
_refine_ls_R_factor_gt                 .031
_refine_ls_wR_factor_all               .051
_refine_ls_wR_factor_ref               .045
_refine_ls_goodness_of_fit_all         3.34
_refine_ls_goodness_of_fit_ref         2.97
_refine_ls_number_reflns               2631
_refine_ls_number_parameters           150
_refine_ls_weighting_scheme            calc
_refine_ls_weighting_details           w=1/σ²(F)
_refine_ls_number_restraints           0
_refine_ls_number_constraints          0
_refine_ls_hydrogen_treatment          none
_refine_ls_shift/su_max                .001
_refine_ls_shift/su_mean               .0001
_refine_diff_density_min              -.721
_refine_diff_density_max               .722

_refine_ls_extinction_method          'Gaussian (Zachariasen, 1967)'
_refine_ls_extinction_expression      'Eq22 p292 "Cryst. Comp." Munksgaard 1970'
_refine_ls_extinction_coef             8997(2536)
_refine_ls_abs_structure_details      'Flack xabs refined'
_refine_ls_abs_structure_Flack         0.56(5)


#------------------------------------------------------------------------------
# B4. COMPUTING METHODS for the BaKTP structure
#------------------------------------------------------------------------------
 
_computing_data_collection            'BL14A (Tsukuba, Japan)'
_computing_cell_refinement            'BL14A (Tsukuba, Japan)'
_computing_data_reduction
 'Xtal3.6 (Hall et al., 1999) DIFDAT ADDREF ABSORB SORTRF'
_computing_structure_refinement       'Xtal3.6 (Hall et al., 1999) CRYLSQ'
_computing_molecular_graphics
;
ORTEPIII (Burnett & Johnson, 1996) and Xtal3.6 (Hall et al., 1999) FOURR SLANT
CONTRS
;
_computing_publication_material
 'Xtal3.6 (Hall et al., 1999) BONDLA ATABLE CIFIO'
 
 
#------------------------------------------------------------------------------
# B5. SCATERING FACTORS AND ATOM DATA for the BaKTP structure
#------------------------------------------------------------------------------
 
loop_
_atom_type_symbol
_atom_type_description
_atom_type_oxidation_number
_atom_type_number_in_cell
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
  K   ?  0 '7.020'  .1958   .2781 'Int Tables Vol IV Tables 2.2B and 2.3.1'
  Ba  ?  0 '0.492' -.5402  2.5117 'Int Tables Vol IV Tables 2.2B and 2.3.1'
  Ti  ?  0  8       .2647   .4951 'Int Tables Vol IV Tables 2.2B and 2.3.1'
  P   ?  0  8       .1003   .1055 'Int Tables Vol IV Tables 2.2B and 2.3.1'
  O   ?  0 40       .0093   .0068 'Int Tables Vol IV Tables 2.2B and 2.3.1'

# S.Sasaki (1989) Numerical Tables of Anomalous Scattering Factors
# Calculated by the Cromer and Liberman's Method, KEK Report, 88-14, 1-136.
# Are used for anomalous dispersion correction.

loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_calc_attached_atom
_atom_site_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
  K1   .37678(11) .2210(2)   .30754(18) .0081(6)   Uani  ?  ?  1.000(4)   ?  ?
  K2   .1073(11)  .300(2)    .0568(13)  .007(2)    Uani  ?  ?  0.755(10)  ?  ?
  Ba2  .104(2)    .305(4)    .069(2)    .006(3)    Uiso  ?  ?  0.123(3)   ?  ?
  Ti1  .37269(8)  .50034(16) .00013(17) .0038(4)   Uani  ?  ?  1.00000    ?  ?
  Ti2  .24644(9)  .73294(16) .25070(16) .0035(4)   Uani  ?  ?  1.00000    ?  ?
  P1   .49818(13) .6639(2)   .2582(2)   .0030(6)   Uani  ?  ?  1.00000    ?  ?
  P2   .18075(11) .4977(2)   .5104(2)   .0032(6)   Uani  ?  ?  1.00000    ?  ?
  O1   .4863(4)   .5128(7)   .1485(4)   .006(2)    Uani  ?  ?  1.00000    ?  ?
  O2   .5098(4)   .5347(8)   .3815(4)   .005(2)    Uani  ?  ?  1.00000    ?  ?
  O3   .4003(4)   .8019(7)   .2769(4)   .006(2)    Uani  ?  ?  1.00000    ?  ?
  O4   .5937(3)   .8077(7)   .2389(4)   .0044(19)  Uani  ?  ?  1.00000    ?  ?
  O11  .2752(4)   .5333(7)   .1403(4)   .005(2)    Uani  ?  ?  1.00000    ?  ?
  O12  .2238(4)   .9586(8)   .3873(4)   .005(2)    Uani  ?  ?  1.00000    ?  ?
  O5   .1118(4)   .6887(7)   .5385(4)   .005(2)    Uani  ?  ?  1.00000    ?  ?
  O6   .1110(4)   .3085(7)   .4852(4)   .006(2)    Uani  ?  ?  1.00000    ?  ?
  O7   .2530(4)   .4608(8)   .6259(4)   .006(2)    Uani  ?  ?  1.00000    ?  ?
  O8   .2530(4)   .5388(8)   .397(3)    .005(2)    Uani  ?  ?  1.00000    ?  ?

 

#------------------------------------------------------------------------------
# B6. MOLECULAR GEOMETRY for the BaKTP structure
#------------------------------------------------------------------------------

_geom_special_details
;  ?
; 
 
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag 
  K1   K2    .        .       4.399(14)  no
  K1   Ba2   .        .       4.36(3)    no
  K1   Ti1   .        .       3.725(3)   no
  K1   Ti2   .       '1 545'  3.603(2)   no
  K1   P1    .        .       3.285(2)   no
  K1   P2    .       '3 544'  3.544(3)   no
  K1   O1    .        .       2.888(5)   no
  K1   O2    .        .       2.756(5)   no
  K1   O3    .       '1 545'  2.726(5)   no
  K1   O11   .        .       2.979(5)   no
  K1   O12   .       '1 545'  2.724(5)   no
  K1   O5    .       '3 544'  2.868(5)   no
  K1   O7    .       '3 544'  3.048(5)   no
  K1   O8    .        .       2.755(11)  no
  K1   Ti2   .        .       3.737(2)   no
  K1   K2    .       '3 545'  3.786(14)  no
  K1   Ba2   .       '3 545'  3.86(2)    no
  K1   K2    .        3       4.569(14)  no
  K1   Ba2   .        3       4.67(2)    no
  K1   K2    .        4       3.986(14)  no
  K1   Ba2   .        4       3.87(2)    no
  K2   Ba2   .        .        .14(3)    no
  K2   Ti1   .        .       3.694(14)  no
  K2   P2    .       '3 544'  3.382(14)  no
  K2   O4    .       '4 465'  3.178(14)  no
  K2   O11   .        .       2.771(15)  no
  K2   O7    .       '3 544'  2.918(15)  no
  K2   P1    .       '3 544'  3.557(14)  no
  K2   O2    .       '3 544'  2.939(15)  no
  K2   O8    .       '3 544'  2.99(2)    no
  K2   Ti2   .       '3 544'  3.780(14)  no
  K2   O3    .       '3 544'  2.973(14)  no
  K2   O12   .       '3 544'  2.997(15)  no
  K2   Ti1   .       '4 455'  3.630(14)  no
  K2   O1    .       '4 455'  2.721(15)  no
  K2   O5    .       '2 564'  2.823(15)  no
  Ba2  Ti1   .        .       3.75(3)    no
  Ba2  P2    .       '3 544'  3.45(3)    no
  Ba2  O4    .       '4 465'  3.07(2)    no
  Ba2  O11   .        .       2.75(3)    no
  Ba2  O7    .       '3 544'  2.94(3)    no
  Ba2  Ti2   .        .       3.82(2)    no
  Ba2  O2    .       '3 544'  3.02(2)    no
  Ba2  O8    .       '3 544'  3.11(3)    no
  Ba2  O3    .       '3 544'  3.10(2)    no
  Ba2  O12   .       '3 544'  3.10(3)    no
  Ba2  Ti1   .       '4 455'  3.63(3)    no
  Ba2  O1    .       '4 455'  2.67(3)    no
  Ba2  O5    .       '2 564'  2.79(3)    no
  Ti1  O1    .        .       2.149(5)   no
  Ti1  O11   .        .       1.957(5)   no
  Ti1  O5    .       '3 544'  2.051(5)   no
  Ti1  O6    .       '3 554'  1.996(5)   no
  Ti1  O2    .       '2 664'  1.979(5)   no
  Ti1  O12   .       '3 544'  1.745(5)   no
  Ti2  O3   '1 545'  '1 545'  2.045(5)   no
  Ti2  O12  '1 545'  '1 545'  2.071(5)   no
  Ti2  O7   '1 545'  '3 544'  1.974(5)   no
  Ti2  O4   '1 545'  '4 455'  1.984(5)   no
  Ti2  O11  '1 545'  '1 545'  1.776(5)   no
  Ti2  O8   '1 545'  '1 545'  1.99(2)    no
  P1   O1    .        .       1.525(5)   no
  P1   O2    .        .       1.556(5)   no
  P1   O3    .        .       1.551(5)   no
  P1   O4    .        .       1.549(5)   no
  P2   O5   '3 544'  '3 544'  1.541(5)   no
  P2   O7   '3 544'  '3 544'  1.557(5)   no
  P2   O6   '3 544'  '3 544'  1.533(5)   no
  P2   O8   '3 544'  '3 544'  1.54(2)    no

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
  K2   K1   Ba2   .        .        .         1.8(4)    no
  K2   K1   Ti1   .        .        .        53.31(18)  no
  K2   K1   Ti2   .        .       '1 545'   68.48(18)  no
  K2   K1   P1    .        .        .       100.21(19)  no
  K2   K1   P2    .        .       '3 544'   48.96(18)  no
  K2   K1   O1    .        .        .        87.4(2)    no
  K2   K1   O2    .        .        .       125.2(2)    no
  K2   K1   O3    .        .       '1 545'   97.4(2)    no
  K2   K1   O11   .        .        .        38.4(2)    no
  K2   K1   O12   .        .       '1 545'   72.0(2)    no
  K2   K1   O5    .        .       '3 544'   56.3(2)    no
  K2   K1   O7    .        .       '3 544'   41.4(2)    no
  K2   K1   O8    .        .        .        70.6(5)    no
  K2   K1   Ti2   .        .        .        56.46(18)  no
  K2   K1   K2    .        .       '3 545'  123.3(3)    no
  K2   K1   Ba2   .        .       '3 545'  124.5(4)    no
  K2   K1   K2    .        .        3       107.0(3)    no
  K2   K1   Ba2   .        .        3       108.0(4)    no
  K2   K1   K2    .        .        4       100.6(3)    no
  K2   K1   Ba2   .        .        4       101.7(4)    no
  Ba2  K1   Ti1   .        .        .        54.5(3)    no
  Ba2  K1   Ti2   .        .       '1 545'   68.7(3)    no
  Ba2  K1   P1    .        .        .       100.5(3)    no
  Ba2  K1   P2    .        .       '3 544'   50.6(3)    no
  Ba2  K1   O1    .        .        .        88.4(3)    no
  Ba2  K1   O2    .        .        .       125.1(3)    no
  Ba2  K1   O3    .        .       '1 545'   98.1(3)    no
  Ba2  K1   O11   .        .        .        38.6(3)    no
  Ba2  K1   O12   .        .       '1 545'   71.1(3)    no
  Ba2  K1   O5    .        .       '3 544'   58.1(3)    no
  Ba2  K1   O7    .        .       '3 544'   42.3(3)    no
  Ba2  K1   O8    .        .        .        69.1(6)    no
  Ba2  K1   Ti2   .        .        .        55.7(3)    no
  Ba2  K1   K2    .        .       '3 545'  122.5(4)    no
  Ba2  K1   Ba2   .        .       '3 545'  123.7(5)    no
  Ba2  K1   K2    .        .        3       105.8(4)    no
  Ba2  K1   Ba2   .        .        3       106.8(5)    no
  Ba2  K1   K2    .        .        4       102.3(4)    no
  Ba2  K1   Ba2   .        .        4       103.4(5)    no
  Ti1  K1   Ti2   .        .       '1 545'  105.37(6)   no
  Ti1  K1   P1    .        .        .        56.67(5)   no
  Ti1  K1   P2    .        .       '3 544'   53.93(5)   no
  Ti1  K1   O1    .        .        .        35.13(10)  no
  Ti1  K1   O2    .        .        .        84.65(10)  no
  Ti1  K1   O3    .        .       '1 545'  111.83(11)  no
  Ti1  K1   O11   .        .        .        31.52(10)  no
  Ti1  K1   O12   .        .       '1 545'  124.06(11)  no
  Ti1  K1   O5    .        .       '3 544'   33.13(9)   no
  Ti1  K1   O7    .        .       '3 544'   72.63(10)  no
  Ti1  K1   O8    .        .        .        86.4(5)    no
  Ti1  K1   Ti2   .        .        .        55.18(4)   no
  Ti1  K1   K2    .        .       '3 545'  163.1(2)    no
  Ti1  K1   Ba2   .        .       '3 545'  164.6(4)    no
  Ti1  K1   K2    .        .        3        96.70(18)  no
  Ti1  K1   Ba2   .        .        3        97.8(3)    no
  Ti1  K1   K2    .        .        4        56.0(2)    no
  Ti1  K1   Ba2   .        .        4        57.1(4)    no
  Ti2  K1   P1   '1 545'   .        .       161.17(8)   no
  Ti2  K1   P2   '1 545'   .       '3 544'   53.29(4)   no
  Ti2  K1   O1   '1 545'   .        .       133.80(12)  no
  Ti2  K1   O2   '1 545'   .        .       166.26(12)  no
  Ti2  K1   O3   '1 545'   .       '1 545'   34.28(10)  no
  Ti2  K1   O11  '1 545'   .        .       106.34(11)  no
  Ti2  K1   O12  '1 545'   .       '1 545'   34.82(11)  no
  Ti2  K1   O5   '1 545'   .       '3 544'   78.11(10)  no
  Ti2  K1   O7   '1 545'   .       '3 544'   33.21(10)  no
  Ti2  K1   O8   '1 545'   .        .       115.64(12)  no
  Ti2  K1   Ti2  '1 545'   .        .       121.94(6)   no
  Ti2  K1   K2   '1 545'   .       '3 545'   61.5(2)    no
  Ti2  K1   Ba2  '1 545'   .       '3 545'   63.2(4)    no
  Ti2  K1   K2   '1 545'   .        3       145.64(18)  no
  Ti2  K1   Ba2  '1 545'   .        3       145.3(3)    no
  Ti2  K1   K2   '1 545'   .        4       101.7(2)    no
  Ti2  K1   Ba2  '1 545'   .        4       101.7(4)    no
  P1   K1   P2    .        .       '3 544'  107.88(7)   no
  P1   K1   O1    .        .        .        27.65(10)  no
  P1   K1   O2    .        .        .        28.16(10)  no
  P1   K1   O3    .        .       '1 545'  141.47(12)  no
  P1   K1   O11   .        .        .        62.03(11)  no
  P1   K1   O12   .        .       '1 545'  158.06(12)  no
  P1   K1   O5    .        .       '3 544'   83.09(10)  no
  P1   K1   O7    .        .       '3 544'  129.29(12)  no
  P1   K1   O8    .        .        .        71.9(2)    no
  P1   K1   Ti2   .        .        .        54.99(5)   no
  P1   K1   K2    .        .       '3 545'  134.7(2)    no
  P1   K1   Ba2   .        .       '3 545'  133.1(4)    no
  P1   K1   K2    .        .        3        50.70(18)  no
  P1   K1   Ba2   .        .        3        51.3(3)    no
  P1   K1   K2    .        .        4        64.6(2)    no
  P1   K1   Ba2   .        .        4        64.8(4)    no
  P2   K1   O1   '3 544'   .        .        80.96(11)  no
  P2   K1   O2   '3 544'   .        .       132.73(11)  no
  P2   K1   O3   '3 544'   .       '1 545'   61.18(11)  no
  P2   K1   O11  '3 544'   .        .        69.50(10)  no
  P2   K1   O12  '3 544'   .       '1 545'   82.90(11)  no
  P2   K1   O5   '3 544'   .       '3 544'   25.09(9)   no
  P2   K1   O7   '3 544'   .       '3 544'   25.95(9)   no
  P2   K1   O8   '3 544'   .        .       119.0(5)    no
  P2   K1   Ti2  '3 544'   .        .        96.79(6)   no
  P2   K1   K2   '3 544'   .       '3 545'  110.2(2)    no
  P2   K1   Ba2  '3 544'   .       '3 545'  112.0(4)    no
  P2   K1   K2   '3 544'   .        3       148.69(18)  no
  P2   K1   Ba2  '3 544'   .        3       149.9(3)    no
  P2   K1   K2   '3 544'   .        4        63.0(2)    no
  P2   K1   Ba2  '3 544'   .        4        63.7(4)    no
  O1   K1   O2    .        .        .        52.45(14)  no
  O1   K1   O3    .        .       '1 545'  121.06(15)  no
  O1   K1   O11   .        .        .        55.15(15)  no
  O1   K1   O12   .        .       '1 545'  159.16(15)  no
  O1   K1   O5    .        .       '3 544'   55.90(13)  no
  O1   K1   O7    .        .       '3 544'  104.58(15)  no
  O1   K1   O8    .        .        .        90.2(4)    no
  O1   K1   Ti2   .        .        .        63.51(11)  no
  O1   K1   K2    .        .       '3 545'  147.7(2)    no
  O1   K1   Ba2   .        .       '3 545'  146.9(4)    no 
  O1   K1   K2    .        .        3        77.8(2)    no
  O1   K1   Ba2   .        .        3        78.6(3)    no
  O1   K1   K2    .        .        4        43.1(2)    no
  O1   K1   Ba2   .        .        4        43.7(4)    no
  O2   K1   O3    .        .       '1 545'  133.33(15)  no
  O2   K1   O11   .        .        .        87.14(14)  no
  O2   K1   O12   .        .       '1 545'  144.19(15)  no
  O2   K1   O5    .        .       '3 544'  107.76(14)  no
  O2   K1   O7    .        .       '3 544'  156.94(15)  no
  O2   K1   O8    .        .        .        73.7(2)    no
  O2   K1   Ti2   .        .        .        71.44(11)  no
  O2   K1   K2    .        .       '3 545'  106.8(2)    no
  O2   K1   Ba2   .        .       '3 545'  105.1(4)    no
  O2   K1   K2    .        .        3        38.0(2)    no
  O2   K1   Ba2   .        .        3        38.0(3)    no
  O2   K1   K2    .        .        4        75.8(2)    no
  O2   K1   Ba2   .        .        4        75.5(4)    no
  O3   K1   O11  '1 545'   .        .       129.88(15)  no
  O3   K1   O12  '1 545'   .       '1 545'   60.45(15)  no
  O3   K1   O5   '1 545'   .       '3 544'   78.70(14)  no
  O3   K1   O7   '1 545'   .       '3 544'   56.25(14)  no
  O3   K1   O8   '1 545'   .        .       146.7(2)    no
  O3   K1   Ti2  '1 545'   .        .       153.88(11)  no
  O3   K1   K2   '1 545'   .       '3 545'   51.2(2)    no
  O3   K1   Ba2  '1 545'   .       '3 545'   52.9(4)    no
  O3   K1   K2   '1 545'   .        3       150.1(2)    no
  O3   K1   Ba2  '1 545'   .        3       148.9(3)    no
  O3   K1   K2   '1 545'   .        4        78.7(2)    no
  O3   K1   Ba2  '1 545'   .        4        78.2(4)    no
  O11  K1   O12   .        .       '1 545'  106.57(15)  no
  O11  K1   O5    .        .       '3 544'   58.48(13)  no
  O11  K1   O7    .        .       '3 544'   75.62(14)  no
  O11  K1   O8    .        .        .        56.9(6)    no
  O11  K1   Ti2   .        .        .        27.85(9)   no
  O11  K1   K2    .        .       '3 545'  156.9(2)    no
  O11  K1   Ba2   .        .       '3 545'  157.3(4)    no
  O11  K1   K2    .        .        3        79.5(2)    no
  O11  K1   Ba2   .        .        3        80.7(3)    no
  O11  K1   K2    .        .        4        87.2(2)    no
  O11  K1   Ba2   .        .        4        88.2(4)    no
  O12  K1   O5   '1 545'   .       '3 544'  107.57(14)  no
  O12  K1   O7   '1 545'   .       '3 544'   57.53(13)  no
  O12  K1   O8   '1 545'   .        .        86.2(2)    no
  O12  K1   Ti2  '1 545'   .        .       105.69(12)  no
  O12  K1   K2   '1 545'   .       '3 545'   51.7(2)    no
  O12  K1   Ba2  '1 545'   .       '3 545'   52.8(4)    no
  O12  K1   K2   '1 545'   .        3       110.8(2)    no
  O12  K1   Ba2  '1 545'   .        3       110.5(3)    no
  O12  K1   K2   '1 545'   .        4       136.3(2)    no
  O12  K1   Ba2  '1 545'   .        4       136.2(4)    no
  O5   K1   O7   '3 544'   .       '3 544'   50.05(13)  no
  O5   K1   O8   '3 544'   .        .       115.2(6)    no
  O5   K1   Ti2  '3 544'   .        .        85.73(10)  no
  O5   K1   K2   '3 544'   .       '3 545'  129.9(2)    no
  O5   K1   Ba2  '3 544'   .       '3 545'  131.5(4)    no
  O5   K1   K2   '3 544'   .        3       129.3(2)    no
  O5   K1   Ba2  '3 544'   .        3       130.4(3)    no
  O5   K1   K2   '3 544'   .        4        45.1(2)    no
  O5   K1   Ba2  '3 544'   .        4        46.1(4)    no
  O7   K1   O8   '3 544'   .        .       107.9(4)    no
  O7   K1   Ti2  '3 544'   .        .        97.72(11)  no
  O7   K1   K2   '3 544'   .       '3 545'   94.7(2)    no
  O7   K1   Ba2  '3 544'   .       '3 545'   96.4(4)    no
  O7   K1   K2   '3 544'   .        3       146.8(2)    no
  O7   K1   Ba2  '3 544'   .        3       147.7(3)    no
  O7   K1   K2   '3 544'   .        4        88.0(2)    no
  O7   K1   Ba2  '3 544'   .        4        88.6(4)    no
  O8   K1   Ti2   .        .        .        31.3(5)    no
  O8   K1   K2    .        .       '3 545'  108.6(6)    no
  O8   K1   Ba2   .        .       '3 545'  107.6(6)    no
  O8   K1   K2    .        .        3        39.1(4)    no
  O8   K1   Ba2   .        .        3        39.8(5)    no
  O8   K1   K2    .        .        4       133.2(4)    no
  O8   K1   Ba2   .        .        4       133.9(5)    no
  Ti2  K1   K2    .        .       '3 545'  139.8(2)    no
  Ti2  K1   Ba2   .        .       '3 545'  138.9(4)    no
  Ti2  K1   K2    .        .        3        53.00(18)  no
  Ti2  K1   Ba2   .        .        3        54.2(3)    no
  Ti2  K1   K2    .        .        4       104.8(2)    no
  Ti2  K1   Ba2   .        .        4       105.7(4)    no
  K2   K1   Ba2  '3 545'   .       '3 545'    1.8(4)    no
  K2   K1   K2   '3 545'   .        3       100.0(3)    no
  K2   K1   Ba2  '3 545'   .        3        98.8(4)    no
  K2   K1   K2   '3 545'   .        4       113.7(3)    no
  K2   K1   Ba2  '3 545'   .        4       112.7(4)    no
  Ba2  K1   K2   '3 545'   .        3        98.2(4)    no
  Ba2  K1   Ba2  '3 545'   .        3        97.1(5)    no
  Ba2  K1   K2   '3 545'   .        4       114.1(4)    no
  Ba2  K1   Ba2  '3 545'   .        4       113.1(5)    no
  K2   K1   Ba2   3        .        3         1.2(3)    no
  K2   K1   K2    3        .        4       112.4(3)    no
  K2   K1   Ba2   3        .        4       112.4(4)    no
  Ba2  K1   K2    3        .        4       112.7(4)    no
  Ba2  K1   Ba2   3        .        4       112.6(5)    no
  K2   K1   Ba2   4        .        4         1.1(4)    no
  K1   K2   Ba2   .        .        .        73(12)     no
  K1   K2   Ti1   .        .        .        53.96(19)  no
  K1   K2   P2    .        .       '3 544'   52.2(2)    no
  K1   K2   O4    .        .       '4 465'   76.5(3)    no
  K1   K2   O11   .        .        .        41.9(2)    no
  K1   K2   O7    .        .       '3 544'   43.7(2)    no
  K1   K2   K1    .        .       '3 544'  102.8(3)    no
  K1   K2   P1    .        .       '3 544'  144.2(4)    no
  K1   K2   O2    .        .       '3 544'  136.0(4)    no
  K1   K2   O8    .        .       '3 544'   78.8(5)    no
  K1   K2   K1    .        .       '3 554'  117.6(3)    no
  K1   K2   Ti2   .        .       '3 544'   96.6(3)    no
  K1   K2   O3    .        .       '3 544'  129.1(4)    no
  K1   K2   O12   .        .       '3 544'   80.4(3)    no
  K1   K2   K1    .        .       '4 455'  100.2(3)    no
  K1   K2   Ti1   .        .       '4 455'  133.8(4)    no
  K1   K2   O1    .        .       '4 455'   98.5(4)    no
  K1   K2   O5    .        .       '2 564'  146.1(4)    no
  Ba2  K2   Ti1   .        .        .       111(12)     no
  Ba2  K2   P2    .        .       '3 544'  120(12)     no
  Ba2  K2   O4    .        .       '4 465'   42(12)     no
  Ba2  K2   O11   .        .        .        80(12)     no
  Ba2  K2   O7    .        .       '3 544'   96(12)     no
  Ba2  K2   K1    .        .       '3 544'  136(12)     no
  Ba2  K2   P1    .        .       '3 544'  140(12)     no
  Ba2  K2   O2    .        .       '3 544'  124(12)     no
  Ba2  K2   O8    .        .       '3 544'  146(12)     no
  Ba2  K2   K1    .        .       '3 554'  121(12)     no
  Ba2  K2   Ti2   .        .       '3 544'  167(12)     no
  Ba2  K2   O3    .        .       '3 544'  157(12)     no
  Ba2  K2   O12   .        .       '3 544'  135(12)     no
  Ba2  K2   K1    .        .       '4 455'   33(12)     no
  Ba2  K2   Ti1   .        .       '4 455'   91(12)     no
  Ba2  K2   O1    .        .       '4 455'   69(12)     no
  Ba2  K2   O5    .        .       '2 564'   76(12)     no
  Ti1  K2   P2    .        .       '3 544'   55.4(2)    no
  Ti1  K2   O4    .        .       '4 465'   82.8(3)    no
  Ti1  K2   O11   .        .        .        31.30(18)  no
  Ti1  K2   O7    .        .       '3 544'   74.5(3)    no
  Ti1  K2   K1    .        .       '3 544'   98.5(3)    no
  Ti1  K2   P1    .        .       '3 544'  107.0(3)    no
  Ti1  K2   O2    .        .       '3 544'  124.8(4)    no
  Ti1  K2   O8    .        .       '3 544'   63.1(3)    no
  Ti1  K2   K1    .        .       '3 554'   65.7(2)    no
  Ti1  K2   Ti2   .        .       '3 544'   56.0(2)    no
  Ti1  K2   O3    .        .       '3 544'   82.3(3)    no
  Ti1  K2   O12   .        .       '3 544'   27.82(16)  no
  Ti1  K2   K1    .        .       '4 455'  143.8(4)    no
  Ti1  K2   Ti1   .        .       '4 455'  157.6(4)    no
  Ti1  K2   O1    .        .       '4 455'  147.4(5)    no
  Ti1  K2   O5    .        .       '2 564'  154.3(5)    no
  P2   K2   O4   '3 544'   .       '4 465'  126.0(4)    no
  P2   K2   O11  '3 544'   .        .        74.3(3)    no
  P2   K2   O7   '3 544'   .       '3 544'   27.37(16)  no
  P2   K2   K1   '3 544'   .       '3 544'   54.0(2)    no
  P2   K2   P1   '3 544'   .       '3 544'   92.0(3)    no
  P2   K2   O2   '3 544'   .       '3 544'   89.3(4)    no
  P2   K2   O8   '3 544'   .       '3 544'   27.2(5)    no
  P2   K2   K1   '3 544'   .       '3 554'  105.3(4)    no
  P2   K2   Ti2  '3 544'   .       '3 544'   53.7(2)    no
  P2   K2   O3   '3 544'   .       '3 544'   83.3(3)    no
  P2   K2   O12  '3 544'   .       '3 544'   61.6(3)    no
  P2   K2   K1   '3 544'   .       '4 455'  132.5(4)    no
  P2   K2   Ti1  '3 544'   .       '4 455'  109.8(4)    no
  P2   K2   O1   '3 544'   .       '4 455'   95.1(4)    no
  P2   K2   O5   '3 544'   .       '2 564'  143.9(5)    no
  O4   K2   O11  '4 465'   .        .        54.6(3)    no
  O4   K2   O7   '4 465'   .       '3 544'  118.2(5)    no
  O4   K2   K1   '4 465'   .       '3 544'  177.8(4)    no
  O4   K2   P1   '4 465'   .       '3 544'  135.8(4)    no
  O4   K2   O2   '4 465'   .       '3 544'  144.7(5)    no
  O4   K2   O8   '4 465'   .       '3 544'  145.5(5)    no
  O4   K2   K1   '4 465'   .       '3 554'   82.2(3)    no
  O4   K2   Ti2  '4 465'   .       '3 544'  129.9(4)    no
  O4   K2   O3   '4 465'   .       '3 544'  127.2(5)    no
  O4   K2   O12  '4 465'   .       '3 544'   97.9(4)    no
  O4   K2   K1   '4 465'   .       '4 455'   65.1(3)    no
  O4   K2   Ti1  '4 465'   .       '4 455'  118.4(4)    no
  O4   K2   O1   '4 465'   .       '4 455'  109.6(5)    no
  O4   K2   O5   '4 465'   .       '2 564'   88.1(4)    no
  O11  K2   O7    .        .       '3 544'   81.0(4)    no
  O11  K2   K1    .        .       '3 544'  126.1(4)    no
  O11  K2   P1    .        .       '3 544'  135.6(5)    no
  O11  K2   O2    .        .       '3 544'  156.1(6)    no
  O11  K2   O8    .        .       '3 544'   91.0(5)    no
  O11  K2   K1    .        .       '3 554'   78.3(3)    no
  O11  K2   Ti2   .        .       '3 544'   87.1(4)    no
  O11  K2   O3    .        .       '3 544'  110.1(5)    no
  O11  K2   O12   .        .       '3 544'   56.3(3)    no
  O11  K2   K1    .        .       '4 455'  112.5(4)    no
  O11  K2   Ti1   .        .       '4 455'  170.6(5)    no
  O11  K2   O1    .        .       '4 455'  136.8(5)    no
  O11  K2   O5    .        .       '2 564'  141.7(5)    no
  O7   K2   K1   '3 544'   .       '3 544'   60.7(3)    no
  O7   K2   P1   '3 544'   .       '3 544'  106.0(4)    no
  O7   K2   O2   '3 544'   .       '3 544'   92.4(4)    no
  O7   K2   O8   '3 544'   .       '3 544'   49.7(5)    no
  O7   K2   K1   '3 544'   .       '3 554'  132.5(5)    no
  O7   K2   Ti2  '3 544'   .       '3 544'   79.9(3)    no
  O7   K2   O3   '3 544'   .       '3 544'  105.9(4)    no
  O7   K2   O12  '3 544'   .       '3 544'   87.6(4)    no
  O7   K2   K1   '3 544'   .       '4 455'  105.3(4)    no
  O7   K2   Ti1  '3 544'   .       '4 455'   99.0(4)    no
  O7   K2   O1   '3 544'   .       '4 455'   73.1(4)    no
  O7   K2   O5   '3 544'   .       '2 564'  130.5(5)    no
  K1   K2   P1   '3 544'   .       '3 544'   45.61(16)  no
  K1   K2   O2   '3 544'   .       '3 544'   35.30(19)  no
  K1   K2   O8   '3 544'   .       '3 544'   35.6(2)    no
  K1   K2   K1   '3 544'   .       '3 554'  100.0(3)    no
  K1   K2   Ti2  '3 544'   .       '3 544'   52.14(17)  no
  K1   K2   O3   '3 544'   .       '3 544'   54.9(2)    no
  K1   K2   O12  '3 544'   .       '3 544'   84.0(3)    no
  K1   K2   K1   '3 544'   .       '4 455'  113.1(3)    no
  K1   K2   Ti1  '3 544'   .       '4 455'   60.6(2)    no
  K1   K2   O1   '3 544'   .       '4 455'   68.4(3)    no
  K1   K2   O5   '3 544'   .       '2 564'   91.5(3)    no
  P1   K2   O2   '3 544'   .       '3 544'   25.52(15)  no
  P1   K2   O8   '3 544'   .       '3 544'   65.4(5)    no
  P1   K2   K1   '3 544'   .       '3 554'   64.7(2)    no
  P1   K2   Ti2  '3 544'   .       '3 544'   52.8(2)    no
  P1   K2   O3   '3 544'   .       '3 544'   25.53(15)  no
  P1   K2   O12  '3 544'   .       '3 544'   79.9(3)    no
  P1   K2   K1   '3 544'   .       '4 455'  107.7(4)    no
  P1   K2   Ti1  '3 544'   .       '4 455'   53.5(2)    no
  P1   K2   O1   '3 544'   .       '4 455'   85.4(4)    no
  P1   K2   O5   '3 544'   .       '2 564'   64.2(3)    no
  O2   K2   O8   '3 544'   .       '3 544'   67.8(4)    no
  O2   K2   K1   '3 544'   .       '3 554'   89.9(3)    no
  O2   K2   Ti2  '3 544'   .       '3 544'   69.1(3)    no
  O2   K2   O3   '3 544'   .       '3 544'   49.6(3)    no
  O2   K2   O12  '3 544'   .       '3 544'  100.8(4)    no
  O2   K2   K1   '3 544'   .       '4 455'   91.3(4)    no
  O2   K2   Ti1  '3 544'   .       '4 455'   33.00(18)  no
  O2   K2   O1   '3 544'   .       '4 455'   60.4(3)    no
  O2   K2   O5   '3 544'   .       '2 564'   57.3(3)    no
  O8   K2   K1   '3 544'   .       '3 554'   88.3(5)    no
  O8   K2   Ti2  '3 544'   .       '3 544'   31.6(4)    no
  O8   K2   O3   '3 544'   .       '3 544'   56.9(5)    no
  O8   K2   O12  '3 544'   .       '3 544'   54.1(3)    no
  O8   K2   K1   '3 544'   .       '4 455'  143.8(5)    no
  O8   K2   Ti1  '3 544'   .       '4 455'   96.1(4)    no
  O8   K2   O1   '3 544'   .       '4 455'   97.6(5)    no
  O8   K2   O5   '3 544'   .       '2 564'  125.1(6)    no
  K1   K2   Ti2  '3 554'   .       '3 544'   56.9(2)    no
  K1   K2   O3   '3 554'   .       '3 544'   45.6(2)    no
  K1   K2   O12  '3 554'   .       '3 544'   45.5(2)    no
  K1   K2   K1   '3 554'   .       '4 455'  122.1(4)    no
  K1   K2   Ti1  '3 554'   .       '4 455'  108.0(3)    no
  K1   K2   O1   '3 554'   .       '4 455'  143.9(5)    no
  K1   K2   O5   '3 554'   .       '2 564'   89.3(4)    no
  Ti2  K2   O3   '3 544'   .       '3 544'   32.55(17)  no
  Ti2  K2   O12  '3 544'   .       '3 544'   33.09(17)  no
  Ti2  K2   K1   '3 544'   .       '4 455'  160.1(4)    no
  Ti2  K2   Ti1  '3 544'   .       '4 455'  102.1(3)    no
  Ti2  K2   O1   '3 544'   .       '4 455'  120.5(4)    no
  Ti2  K2   O5   '3 544'   .       '2 564'  116.1(4)    no
  O3   K2   O12  '3 544'   .       '3 544'   54.7(3)    no
  O3   K2   K1   '3 544'   .       '4 455'  130.1(4)    no
  O3   K2   Ti1  '3 544'   .       '4 455'   79.0(3)    no
  O3   K2   O1   '3 544'   .       '4 455'  110.0(5)    no
  O3   K2   O5   '3 544'   .       '2 564'   84.2(4)    no
  O12  K2   K1   '3 544'   .       '4 455'  162.0(5)    no
  O12  K2   Ti1  '3 544'   .       '4 455'  133.0(4)    no
  O12  K2   O1   '3 544'   .       '4 455'  151.5(6)    no
  O12  K2   O5   '3 544'   .       '2 564'  132.3(5)    no
  K1   K2   Ti1  '4 455'   .       '4 455'   58.3(2)    no
  K1   K2   O1   '4 455'   .       '4 455'   46.4(2)    no
  K1   K2   O5   '4 455'   .       '2 564'   46.0(2)    no
  Ti1  K2   O1   '4 455'   .       '4 455'   36.1(2)    no
  Ti1  K2   O5   '4 455'   .       '2 564'   34.26(19)  no
  O1   K2   O5   '4 455'   .       '2 564'   58.2(3)    no
  K1   Ba2  K2    .        .        .       106(12)     no
  K1   Ba2  Ti1   .        .        .        54.1(3)    no
  K1   Ba2  P2    .        .       '3 544'   52.4(4)    no
  K1   Ba2  O4    .        .       '4 465'   78.1(5)    no
  K1   Ba2  O11   .        .        .        42.5(4)    no
  K1   Ba2  O7    .        .       '3 544'   44.3(4)    no
  K1   Ba2  Ti2   .        .        .        53.9(3)    no
  K1   Ba2  K1    .        .       '3 544'  101.8(5)    no
  K1   Ba2  O2    .        .       '3 544'  134.6(8)    no
  K1   Ba2  O8    .        .       '3 544'   78.3(7)    no
  K1   Ba2  K1    .        .       '3 554'  116.9(6)    no
  K1   Ba2  O3    .        .       '3 544'  126.5(7)    no
  K1   Ba2  O12   .        .       '3 544'   80.0(6)    no
  K1   Ba2  K1    .        .       '4 455'  102.8(5)    no
  K1   Ba2  Ti1   .        .       '4 455'  135.1(6)    no
  K1   Ba2  O1    .        .       '4 455'  100.2(6)    no
  K1   Ba2  O5    .        .       '2 564'  150.2(7)    no
  K2   Ba2  Ti1   .        .        .        67(12)     no
  K2   Ba2  P2    .        .       '3 544'   58(12)     no
  K2   Ba2  O4    .        .       '4 465'  137(12)     no
  K2   Ba2  O11   .        .        .        97(12)     no
  K2   Ba2  O7    .        .       '3 544'   81(12)     no
  K2   Ba2  Ti2   .        .        .       118(12)     no
  K2   Ba2  K1    .        .       '3 544'   43(11)     no
  K2   Ba2  O2    .        .       '3 544'   54(12)     no
  K2   Ba2  O8    .        .       '3 544'   33(11)     no
  K2   Ba2  K1    .        .       '3 554'   57(11)     no
  K2   Ba2  O3    .        .       '3 544'   22(12)     no
  K2   Ba2  O12   .        .       '3 544'   43(12)     no
  K2   Ba2  K1    .        .       '4 455'  146(13)     no
  K2   Ba2  Ti1   .        .       '4 455'   87(12)     no
  K2   Ba2  O1    .        .       '4 455'  108(12)     no
  K2   Ba2  O5    .        .       '2 564'  102(12)     no
  Ti1  Ba2  P2    .        .       '3 544'   54.4(4)    no
  Ti1  Ba2  O4    .        .       '4 465'   83.3(6)    no
  Ti1  Ba2  O11   .        .        .        30.4(3)    no
  Ti1  Ba2  O7    .        .       '3 544'   73.4(6)    no
  Ti1  Ba2  Ti2   .        .        .        54.3(4)    no
  Ti1  Ba2  K1    .        .       '3 544'   95.9(5)    no
  Ti1  Ba2  O2    .        .       '3 544'  120.7(7)    no
  Ti1  Ba2  O8    .        .       '3 544'   61.5(5)    no
  Ti1  Ba2  K1    .        .       '3 554'   64.5(4)    no
  Ti1  Ba2  O3    .        .       '3 544'   79.8(5)    no
  Ti1  Ba2  O12   .        .       '3 544'   27.5(2)    no
  Ti1  Ba2  K1    .        .       '4 455'  146.9(7)    no
  Ti1  Ba2  Ti1   .        .       '4 455'  153.5(7)    no
  Ti1  Ba2  O1    .        .       '4 455'  146.9(9)    no
  Ti1  Ba2  O5    .        .       '2 564'  152.6(8)    no
  P2   Ba2  O4   '3 544'   .       '4 465'  127.0(8)    no
  P2   Ba2  O11  '3 544'   .        .        73.3(6)    no
  P2   Ba2  O7   '3 544'   .       '3 544'   26.7(2)    no
  P2   Ba2  Ti2  '3 544'   .        .        96.7(6)    no
  P2   Ba2  K1   '3 544'   .       '3 544'   52.6(3)    no
  P2   Ba2  O2   '3 544'   .       '3 544'   86.6(6)    no
  P2   Ba2  O8   '3 544'   .       '3 544'   26.6(5)    no
  P2   Ba2  K1   '3 544'   .       '3 554'  102.3(6)    no
  P2   Ba2  O3   '3 544'   .       '3 544'   80.2(5)    no
  P2   Ba2  O12  '3 544'   .       '3 544'   59.8(5)    no
  P2   Ba2  K1   '3 544'   .       '4 455'  134.3(7)    no
  P2   Ba2  Ti1  '3 544'   .       '4 455'  108.1(6)    no
  P2   Ba2  O1   '3 544'   .       '4 455'   94.3(7)    no
  P2   Ba2  O5   '3 544'   .       '2 564'  141.5(9)    no
  O4   Ba2  O11  '4 465'   .        .        56.1(5)    no
  O4   Ba2  O7   '4 465'   .       '3 544'  120.9(8)    no
  O4   Ba2  Ti2  '4 465'   .        .        31.1(3)    no
  O4   Ba2  K1   '4 465'   .       '3 544'  179.2(8)    no
  O4   Ba2  O2   '4 465'   .       '3 544'  146.2(10)   no
  O4   Ba2  O8   '4 465'   .       '3 544'  144.7(10)   no
  O4   Ba2  K1   '4 465'   .       '3 554'   82.3(6)    no
  O4   Ba2  O3   '4 465'   .       '3 544'  126.2(8)    no
  O4   Ba2  O12  '4 465'   .       '3 544'   98.0(7)    no
  O4   Ba2  K1   '4 465'   .       '4 455'   67.6(5)    no
  O4   Ba2  Ti1  '4 465'   .       '4 455'  121.3(8)    no
  O4   Ba2  O1   '4 465'   .       '4 455'  114.0(8)    no
  O4   Ba2  O5   '4 465'   .       '2 564'   90.8(7)    no
  O11  Ba2  O7    .        .       '3 544'   81.0(7)    no
  O11  Ba2  Ti2   .        .        .        25.2(3)    no
  O11  Ba2  K1    .        .       '3 544'  123.3(8)    no
  O11  Ba2  O2    .        .       '3 544'  151.1(9)    no
  O11  Ba2  O8    .        .       '3 544'   88.9(8)    no
  O11  Ba2  K1    .        .       '3 554'   77.2(6)    no
  O11  Ba2  O3    .        .       '3 544'  107.0(8)    no
  O11  Ba2  O12   .        .       '3 544'   55.2(5)    no
  O11  Ba2  K1    .        .       '4 455'  116.5(7)    no
  O11  Ba2  Ti1   .        .       '4 455'  175.6(8)    no
  O11  Ba2  O1    .        .       '4 455'  140.5(9)    no
  O11  Ba2  O5    .        .       '2 564'  145.0(10)   no
  O7   Ba2  Ti2  '3 544'   .        .        97.9(7)    no
  O7   Ba2  K1   '3 544'   .       '3 544'   59.0(4)    no
  O7   Ba2  O2   '3 544'   .       '3 544'   90.4(7)    no
  O7   Ba2  O8   '3 544'   .       '3 544'   48.5(6)    no
  O7   Ba2  K1   '3 544'   .       '3 554'  128.9(8)    no
  O7   Ba2  O3   '3 544'   .       '3 544'  102.2(7)    no
  O7   Ba2  O12  '3 544'   .       '3 544'   85.4(7)    no
  O7   Ba2  K1   '3 544'   .       '4 455'  107.8(7)    no
  O7   Ba2  Ti1  '3 544'   .       '4 455'   98.5(7)    no
  O7   Ba2  O1   '3 544'   .       '4 455'   73.5(6)    no
  O7   Ba2  O5   '3 544'   .       '2 564'  131.0(9)    no
  Ti2  Ba2  K1    .        .       '3 544'  148.3(7)    no
  Ti2  Ba2  O2    .        .       '3 544'  167.8(8)    no
  Ti2  Ba2  O8    .        .       '3 544'  114.1(8)    no
  Ti2  Ba2  K1    .        .       '3 554'   80.5(5)    no
  Ti2  Ba2  O3    .        .       '3 544'  121.2(7)    no
  Ti2  Ba2  O12   .        .       '3 544'   75.1(5)    no
  Ti2  Ba2  K1    .        .       '4 455'   93.6(5)    no
  Ti2  Ba2  Ti1   .        .       '4 455'  151.7(7)    no
  Ti2  Ba2  O1    .        .       '4 455'  131.2(7)    no
  Ti2  Ba2  O5    .        .       '2 564'  121.6(8)    no
  K1   Ba2  O2   '3 544'   .       '3 544'   34.2(3)    no
  K1   Ba2  O8   '3 544'   .       '3 544'   34.6(3)    no
  K1   Ba2  K1   '3 544'   .       '3 554'   97.1(4)    no
  K1   Ba2  O3   '3 544'   .       '3 544'   53.2(4)    no
  K1   Ba2  O12  '3 544'   .       '3 544'   81.2(5)    no
  K1   Ba2  K1   '3 544'   .       '4 455'  113.3(6)    no
  K1   Ba2  Ti1  '3 544'   .       '4 455'   59.4(3)    no
  K1   Ba2  O1   '3 544'   .       '4 455'   66.8(5)    no
  K1   Ba2  O5   '3 544'   .       '2 564'   89.7(6)    no
  O2   Ba2  O8   '3 544'   .       '3 544'   65.3(5)    no
  O2   Ba2  K1   '3 544'   .       '3 554'   87.4(5)    no
  O2   Ba2  O3   '3 544'   .       '3 544'   47.8(4)    no
  O2   Ba2  O12  '3 544'   .       '3 544'   96.8(6)    no
  O2   Ba2  K1   '3 544'   .       '4 455'   92.4(7)    no
  O2   Ba2  Ti1  '3 544'   .       '4 455'   33.0(3)    no
  O2   Ba2  O1   '3 544'   .       '4 455'   59.8(5)    no
  O2   Ba2  O5   '3 544'   .       '2 564'   56.7(5)    no
  O8   Ba2  K1   '3 544'   .       '3 554'   85.3(6)    no
  O8   Ba2  O3   '3 544'   .       '3 544'   54.4(6)    no
  O8   Ba2  O12  '3 544'   .       '3 544'   52.1(5)    no
  O8   Ba2  K1   '3 544'   .       '4 455'  144.0(8)    no
  O8   Ba2  Ti1  '3 544'   .       '4 455'   94.0(6)    no
  O8   Ba2  O1   '3 544'   .       '4 455'   95.8(8)    no
  O8   Ba2  O5   '3 544'   .       '2 564'  121.9(9)    no
  K1   Ba2  O3   '3 554'   .       '3 544'   44.5(3)    no
  K1   Ba2  O12  '3 554'   .       '3 544'   44.4(3)    no
  K1   Ba2  K1   '3 554'   .       '4 455'  123.3(7)    no
  K1   Ba2  Ti1  '3 554'   .       '4 455'  106.3(6)    no
  K1   Ba2  O1   '3 554'   .       '4 455'  142.2(9)    no
  K1   Ba2  O5   '3 554'   .       '2 564'   88.3(6)    no
  O3   Ba2  O12  '3 544'   .       '3 544'   52.5(4)    no
  O3   Ba2  K1   '3 544'   .       '4 455'  129.9(8)    no
  O3   Ba2  Ti1  '3 544'   .       '4 455'   77.4(5)    no
  O3   Ba2  O1   '3 544'   .       '4 455'  107.5(8)    no
  O3   Ba2  O5   '3 544'   .       '2 564'   82.4(6)    no
  O12  Ba2  K1   '3 544'   .       '4 455'  163.9(8)    no
  O12  Ba2  Ti1  '3 544'   .       '4 455'  129.1(7)    no
  O12  Ba2  O1   '3 544'   .       '4 455'  147.5(9)    no
  O12  Ba2  O5   '3 544'   .       '2 564'  129.3(8)    no
  K1   Ba2  Ti1  '4 455'   .       '4 455'   59.4(4)    no
  K1   Ba2  O1   '4 455'   .       '4 455'   48.3(4)    no
  K1   Ba2  O5   '4 455'   .       '2 564'   47.7(4)    no
  Ti1  Ba2  O1   '4 455'   .       '4 455'   35.9(3)    no
  Ti1  Ba2  O5   '4 455'   .       '2 564'   34.1(3)    no
  O1   Ba2  O5   '4 455'   .       '2 564'   59.1(6)    no
  K1   Ti1  K2    .        .        .        72.7(2)    no
  K1   Ti1  Ba2   .        .        .        71.4(3)    no
  K1   Ti1  O1    .        .        .        50.64(14)  no
  K1   Ti1  O11   .        .        .        52.72(15)  no
  K1   Ti1  O5    .        .       '3 544'   49.83(13)  no
  K1   Ti1  O6    .        .       '3 554'  123.05(15)  no
  K1   Ti1  O2    .        .       '2 664'  119.51(15)  no
  K1   Ti1  O12   .        .       '3 544'  122.53(17)  no
  K1   Ti1  K2    .        .        4        65.6(2)    no
  K1   Ti1  Ba2   .        .        4        63.4(4)    no
  K2   Ti1  Ba2   .        .        .         2.0(4)    no
  K2   Ti1  O1    .        .        .       121.4(3)    no
  K2   Ti1  O11   .        .        .        47.4(3)    no
  K2   Ti1  O5    .        .       '3 544'   73.6(3)    no
  K2   Ti1  O6    .        .       '3 554'  117.0(3)    no
  K2   Ti1  O2    .        .       '2 664'  140.2(3)    no
  K2   Ti1  O12   .        .       '3 544'   53.3(3)    no
  K2   Ti1  K2    .        .        4       123.7(3)    no
  K2   Ti1  Ba2   .        .        4       122.3(5)    no
  Ba2  Ti1  O1    .        .        .       119.7(4)    no
  Ba2  Ti1  O11   .        .        .        45.4(4)    no
  Ba2  Ti1  O5    .        .       '3 544'   74.0(4)    no
  Ba2  Ti1  O6    .        .       '3 554'  116.4(4)    no
  Ba2  Ti1  O2    .        .       '2 664'  142.1(4)    no
  Ba2  Ti1  O12   .        .       '3 544'   55.1(4)    no
  Ba2  Ti1  K2    .        .        4       123.7(4)    no
  Ba2  Ti1  Ba2   .        .        4       122.3(6)    no
  O1   Ti1  O11   .        .        .        82.7(2)    no
  O1   Ti1  O5    .        .       '3 544'   79.89(19)  no
  O1   Ti1  O6    .        .       '3 554'   87.1(2)    no
  O1   Ti1  O2    .        .       '2 664'   87.3(2)    no
  O1   Ti1  O12   .        .       '3 544'  172.6(2)    no
  O1   Ti1  K2    .        .        4        48.3(3)    no
  O1   Ti1  Ba2   .        .        4        46.9(4)    no
  O11  Ti1  O5    .        .       '3 544'   90.9(2)    no
  O11  Ti1  O6    .        .       '3 554'   91.2(2)    no
  O11  Ti1  O2    .        .       '2 664'  170.0(2)    no
  O11  Ti1  O12   .        .       '3 544'   94.8(2)    no
  O11  Ti1  K2    .        .        4       117.6(3)    no
  O11  Ti1  Ba2   .        .        4       115.4(4)    no
  O5   Ti1  O6   '3 544'   .       '3 554'  166.5(2)    no
  O5   Ti1  O2   '3 544'   .       '2 664'   86.7(2)    no
  O5   Ti1  O12  '3 544'   .       '3 544'   93.2(2)    no
  O5   Ti1  K2   '3 544'   .        4        50.8(3)    no
  O5   Ti1  Ba2  '3 544'   .        4        49.8(4)    no
  O6   Ti1  O2   '3 554'   .       '2 664'   89.0(2)    no
  O6   Ti1  O12  '3 554'   .       '3 544'   99.9(2)    no
  O6   Ti1  K2   '3 554'   .        4       116.9(3)    no
  O6   Ti1  Ba2  '3 554'   .        4       117.7(4)    no
  O2   Ti1  O12  '2 664'   .       '3 544'   95.0(2)    no
  O2   Ti1  K2   '2 664'   .        4        54.0(3)    no
  O2   Ti1  Ba2  '2 664'   .        4        56.2(4)    no
  O12  Ti1  K2   '3 544'   .        4       128.5(3)    no
  O12  Ti1  Ba2  '3 544'   .        4       129.5(4)    no
  K2   Ti1  Ba2   4        .        4         2.2(4)    no
  K1   Ti2  O3    .       '1 545'  '1 545'   48.67(13)  no
  K1   Ti2  O12   .       '1 545'  '1 545'   48.69(15)  no
  K1   Ti2  O7    .       '1 545'  '3 544'   57.76(15)  no
  K1   Ti2  K1    .       '1 545'  '1 545'  121.94(5)   no
  K1   Ti2  Ba2   .       '1 545'  '1 545'  158.7(3)    no
  K1   Ti2  O4    .       '1 545'  '4 455'  125.78(14)  no
  K1   Ti2  O11   .       '1 545'  '1 545'  129.89(17)  no
  K1   Ti2  O8    .       '1 545'  '1 545'  113.2(5)    no
  K1   Ti2  K2    .       '1 545'  '3 545'   61.7(2)    no
  O3   Ti2  O12  '1 545'  '1 545'  '1 545'   83.6(2)    no
  O3   Ti2  O7   '1 545'  '1 545'  '3 544'   85.8(2)    no
  O3   Ti2  K1   '1 545'  '1 545'  '1 545'   74.63(13)  no
  O3   Ti2  Ba2  '1 545'  '1 545'  '1 545'  133.4(4)    no
  O3   Ti2  O4   '1 545'  '1 545'  '4 455'  173.4(2)    no
  O3   Ti2  O11  '1 545'  '1 545'  '1 545'   92.6(2)    no
  O3   Ti2  O8   '1 545'  '1 545'  '1 545'   89.4(2)    no
  O3   Ti2  K2   '1 545'  '1 545'  '3 545'   51.5(3)    no
  O12  Ti2  O7   '1 545'  '1 545'  '3 544'   87.3(2)    no
  O12  Ti2  K1   '1 545'  '1 545'  '1 545'  124.38(15)  no
  O12  Ti2  Ba2  '1 545'  '1 545'  '1 545'  142.1(4)    no
  O12  Ti2  O4   '1 545'  '1 545'  '4 455'   89.8(2)    no
  O12  Ti2  O11  '1 545'  '1 545'  '1 545'  175.3(2)    no
  O12  Ti2  O8   '1 545'  '1 545'  '1 545'   84.1(6)    no
  O12  Ti2  K2   '1 545'  '1 545'  '3 545'   52.2(3)    no
  O7   Ti2  K1   '3 544'  '1 545'  '1 545'  139.32(16)  no
  O7   Ti2  Ba2  '3 544'  '1 545'  '1 545'  101.3(4)    no
  O7   Ti2  O4   '3 544'  '1 545'  '4 455'   93.4(2)    no
  O7   Ti2  O11  '3 544'  '1 545'  '1 545'   95.2(2)    no
  O7   Ti2  O8   '3 544'  '1 545'  '1 545'  170.6(5)    no
  O7   Ti2  K2   '3 544'  '1 545'  '3 545'  119.4(3)    no
  K1   Ti2  Ba2  '1 545'  '1 545'  '1 545'   70.4(4)    no
  K1   Ti2  O4   '1 545'  '1 545'  '4 455'  109.76(14)  no
  K1   Ti2  O11  '1 545'  '1 545'  '1 545'   51.60(16)  no
  K1   Ti2  O8   '1 545'  '1 545'  '1 545'   46.0(5)    no
  K1   Ti2  K2   '1 545'  '1 545'  '3 545'   74.9(2)    no
  Ba2  Ti2  O4   '1 545'  '1 545'  '4 455'   53.1(4)    no
  Ba2  Ti2  O11  '1 545'  '1 545'  '1 545'   41.2(4)    no
  Ba2  Ti2  O8   '1 545'  '1 545'  '1 545'   87.9(6)    no
  Ba2  Ti2  K2   '1 545'  '1 545'  '3 545'  139.0(4)    no
  O4   Ti2  O11  '4 455'  '1 545'  '1 545'   94.0(2)    no
  O4   Ti2  O8   '4 455'  '1 545'  '1 545'   90.5(2)    no
  O4   Ti2  K2   '4 455'  '1 545'  '3 545'  124.2(3)    no
  O11  Ti2  O8   '1 545'  '1 545'  '1 545'   93.1(6)    no
  O11  Ti2  K2   '1 545'  '1 545'  '3 545'  123.1(3)    no
  O8   Ti2  K2   '1 545'  '1 545'  '3 545'   51.8(5)    no
  K1   P1   O1    .        .        .        61.5(2)    no
  K1   P1   O2    .        .        .        56.7(2)    no
  K1   P1   O3    .        .        .        95.07(18)  no
  K1   P1   K2    .        .        3        83.7(2)    no
  K1   P1   O4    .        .        .       155.91(18)  no
  O1   P1   O2    .        .        .       108.3(3)    no
  O1   P1   O3    .        .        .       112.3(3)    no
  O1   P1   K2    .        .        3       143.1(3)    no
  O1   P1   O4    .        .        .       110.9(3)    no
  O2   P1   O3    .        .        .       105.9(3)    no
  O2   P1   K2    .        .        3        54.4(3)    no
  O2   P1   O4    .        .        .       110.6(3)    no
  O3   P1   K2    .        .        3        55.7(3)    no
  O3   P1   O4    .        .        .       108.6(2)    no
  K2   P1   O4    3        .        .       105.9(3)    no
  K1   P2   K2    .       '3 544'   .        78.8(2)    no
  K1   P2   Ba2   .       '3 544'   .        77.0(4)    no
  K1   P2   O5    .       '3 544'  '3 544'   52.11(18)  no
  K1   P2   O7    .       '3 544'  '3 544'   59.0(2)    no
  K1   P2   O6    .       '3 544'  '3 544'  110.7(2)    no
  K1   P2   O8    .       '3 544'  '3 544'  138.8(5)    no
  K2   P2   Ba2   .       '3 544'   .         2.0(4)    no
  K2   P2   O5    .       '3 544'  '3 544'   88.7(3)    no
  K2   P2   O7    .       '3 544'  '3 544'   59.5(3)    no
  K2   P2   O6    .       '3 544'  '3 544'  162.1(3)    no
  K2   P2   O8    .       '3 544'  '3 544'   62.1(7)    no
  Ba2  P2   O5    .       '3 544'  '3 544'   88.4(5)    no
  Ba2  P2   O7    .       '3 544'  '3 544'   57.8(4)    no
  Ba2  P2   O6    .       '3 544'  '3 544'  162.2(5)    no
  Ba2  P2   O8    .       '3 544'  '3 544'   64.0(7)    no
  O5   P2   O7   '3 544'  '3 544'  '3 544'  108.1(3)    no
  O5   P2   O6   '3 544'  '3 544'  '3 544'  109.1(3)    no
  O5   P2   O8   '3 544'  '3 544'  '3 544'  111.2(3)    no
  O7   P2   O6   '3 544'  '3 544'  '3 544'  111.5(3)    no
  O7   P2   O8   '3 544'  '3 544'  '3 544'  106.5(7)    no
  O6   P2   O8   '3 544'  '3 544'  '3 544'  110.5(6)    no
  K1   O1   Ti1   .        .        .        94.23(18)  no
  K1   O1   P1    .        .        .        90.8(2)    no
  K1   O1   K2    .        .        4        90.5(3)    no
  K1   O1   Ba2   .        .        4        88.0(5)    no
  Ti1  O1   P1    .        .        .       130.7(3)    no
  Ti1  O1   K2    .        .        4        95.6(3)    no
  Ti1  O1   Ba2   .        .        4        97.2(5)    no
  P1   O1   K2    .        .        4       133.3(4)    no
  P1   O1   Ba2   .        .        4       132.0(6)    no
  K2   O1   Ba2   4        .        4         2.8(6)    no
  K1   O2   P1    .        .        .        95.2(2)    no
  K1   O2   Ti1   .        .       '2 665'  124.9(2)    no
  K1   O2   K2    .        .        3       106.7(3)    no
  K1   O2   Ba2   .        .        3       107.9(5)    no
  P1   O2   Ti1   .        .       '2 665'  132.0(3)    no
  P1   O2   K2    .        .        3       100.0(4)    no
  P1   O2   Ba2   .        .        3       101.7(5)    no
  Ti1  O2   K2   '2 665'   .        3        93.1(3)    no
  Ti1  O2   Ba2  '2 665'   .        3        90.8(5)    no
  K2   O2   Ba2   3        .        3         2.2(5)    no
  K1   O3   Ti2   .       '1 545'  '1 545'   97.05(17)  no
  K1   O3   P1    .       '1 545'  '1 545'  131.9(2)    no
  K1   O3   K2    .       '1 545'  '3 545'   83.1(3)    no
  K1   O3   Ba2   .       '1 545'  '3 545'   82.7(5)    no
  Ti2  O3   P1   '1 545'  '1 545'  '1 545'  130.0(3)    no
  Ti2  O3   K2   '1 545'  '1 545'  '3 545'   96.0(3)    no
  Ti2  O3   Ba2  '1 545'  '1 545'  '3 545'   96.9(5)    no
  P1   O3   K2   '1 545'  '1 545'  '3 545'   98.8(3)    no
  P1   O3   Ba2  '1 545'  '1 545'  '3 545'   98.4(5)    no
  K2   O3   Ba2  '3 545'  '1 545'  '3 545'    1.0(6)    no
  K2   O4   Ba2   .       '4 465'   .         1.7(5)    no
  K2   O4   Ti2   .       '4 465'   .        95.1(3)    no
  K2   O4   P1    .       '4 465'  '4 465'  126.6(3)    no
  Ba2  O4   Ti2   .       '4 465'   .        95.8(5)    no
  Ba2  O4   P1    .       '4 465'  '4 465'  126.4(5)    no
  Ti2  O4   P1    .       '4 465'  '4 465'  134.2(3)    no
  K1   O11  K2    .        .        .        99.7(3)    no
  K1   O11  Ba2   .        .        .        99.0(5)    no
  K1   O11  Ti1   .        .        .        95.8(2)    no
  K1   O11  Ti2   .        .        .       100.6(2)    no
  K2   O11  Ba2   .        .        .         2.9(5)    no
  K2   O11  Ti1   .        .        .       101.3(3)    no
  K2   O11  Ti2   .        .        .       116.0(4)    no
  Ba2  O11  Ti1   .        .        .       104.2(5)    no
  Ba2  O11  Ti2   .        .        .       113.6(6)    no
  Ti1  O11  Ti2   .        .        .       135.5(3)    no
  K1   O12  Ti2   .       '1 545'  '1 545'   96.50(18)  no
  K1   O12  K2    .       '1 545'  '3 545'   82.7(3)    no
  K1   O12  Ba2   .       '1 545'  '3 545'   82.8(5)    no
  K1   O12  Ti1   .       '1 545'  '3 545'  129.2(3)    no
  Ti2  O12  K2   '1 545'  '1 545'  '3 545'   94.7(3)    no
  Ti2  O12  Ba2  '1 545'  '1 545'  '3 545'   96.5(5)    no
  Ti2  O12  Ti1  '1 545'  '1 545'  '3 545'  133.5(3)    no
  K2   O12  Ba2  '3 545'  '1 545'  '3 545'    1.8(5)    no
  K2   O12  Ti1  '3 545'  '1 545'  '3 545'   98.9(3)    no
  Ba2  O12  Ti1  '3 545'  '1 545'  '3 545'   97.4(5)    no
  K1   O5   Ti1   .       '3 544'   .        97.04(17)  no
  K1   O5   P2    .       '3 544'  '3 544'  102.8(2)    no
  K1   O5   K2    .       '3 544'   4        88.9(3)    no
  K1   O5   Ba2   .       '3 544'   4        86.2(5)    no
  Ti1  O5   P2    .       '3 544'  '3 544'  132.9(3)    no
  Ti1  O5   K2    .       '3 544'   4        94.9(3)    no
  Ti1  O5   Ba2   .       '3 544'   4        96.0(5)    no
  P2   O5   K2   '3 544'  '3 544'   4       127.3(4)    no
  P2   O5   Ba2  '3 544'  '3 544'   4       127.2(6)    no
  K2   O5   Ba2   4       '3 544'   4         2.8(5)    no
  Ti1  O6   P2    .       '3 554'  '3 554'  135.2(3)    no
  K1   O7   K2    .       '3 544'   .        95.0(3)    no
  K1   O7   Ba2   .       '3 544'   .        93.5(5)    no
  K1   O7   Ti2   .       '3 544'  '1 545'   89.03(17)  no
  K1   O7   P2    .       '3 544'  '3 544'   95.1(2)    no
  K2   O7   Ba2   .       '3 544'   .         2.7(5)    no
  K2   O7   Ti2   .       '3 544'  '1 545'  136.1(4)    no
  K2   O7   P2    .       '3 544'  '3 544'   93.1(3)    no
  Ba2  O7   Ti2   .       '3 544'  '1 545'  133.9(5)    no
  Ba2  O7   P2    .       '3 544'  '3 544'   95.5(5)    no
  Ti2  O7   P2   '1 545'  '3 544'  '3 544'  130.1(3)    no
  K1   O8   Ti2   .        .        .       102.7(10)   no
  K1   O8   K2    .        .        3       105.3(4)    no
  K1   O8   Ba2   .        .        3       105.5(5)    no
  K1   O8   P2    .        .        .       119.3(5)    no
  Ti2  O8   K2    .        .        3        96.7(3)    no
  Ti2  O8   Ba2   .        .        3        98.0(5)    no
  Ti2  O8   P2    .        .        .       133.6(3)    no
  K2   O8   Ba2   3        .        3         1.4(5)    no
  K2   O8   P2    3        .        .        90.7(11)   no
  Ba2  O8   P2    3        .        .        89.4(11)   no

 
